Upload
others
View
23
Download
0
Embed Size (px)
Citation preview
Deformation-Induced Crystallization
In Rubber-Like Materials
Vom Fachbereich Mechanik derTechnischen Universitat Darmstadt
zur Erlangung des akademischen Grades einesDOKTORS DER INGENIEURWISSENSCHAFTEN
genehmigteDISSERTATION
von
Chem. Eng. Motasem Saidan
aus Jordanien
Referent: Prof. Dr. T. AltsKorreferent: Prof. K. Hutter, Ph. D./ Cornell University
Tag der Einreichung: 1. Dez. 2004Tag der mundlichen Prufung: 21. Jan. 2005
Darmstadt 2005D 17
To my beloved brother, Khaled,
who passed away on 18th Apr 2003.
God bless you my brother,
you are always in my heart, Khaled.
Acknowledgment
Most of all, I would like to express my thanks to God, in him alone I putmy trust. His mercy and blessing saved, guided and enabled me to run towardsmy ambitions. Also, I would like to express my sincere gratitude and heartfeltappreciations to my doctor-father, Prof. Thorsten Alts, for his guidance, encour-agement, and support during my graduate studies. His impressive knowledge,technical skill, and creative thinking have been an invaluable help throughoutthe course of this work. The expertise that he shared me will remain a tremen-dous source of professional growth to me. I am really sure that I can not be herewithout him.
I am profoundly grateful to Prof. K. Hutter. His insight, kindness, and gen-uine concern for his students made staying in his group a memorable experience.I also wish to thank my committee members, Prof. Dr.-Ing. Ch. Tsakmakis,Prof. (jun.) Dr.-Ing. R. Muller, and Prof. Dr. M. Wilhelm, for their time,counsel, and valuable contributions to this work.
I owe much gratitude to DFG (German research foundation) for providing thefinancial support throughout my study.
I wish to thank Dr. Eisele, Bayer AG, Leverkusen for the polyisoprene rub-ber samples that he has provided for this work. Also, I would like to express mysincere thanks to Prof. Dr. Rolf Hosemann, Bundesanstalt fur MaterialprufungBAM-Berlin for performing the tensile loading-unloading experiments for poly-isoprene rubber samples and providing us with the Wide Angle X-ray Diffraction(WAXD) data.
We are indebted to Rieter Automative Germany GmbH for providing us withEthylene-butene copolymers materials. Finally, I would like to express my grati-tude to the German Polymer Institute DKI -Darmstadt. Especially, Dr. -Ing. M.Moneke, PD Dr. G. P. Hellmann, Dr. Reza Ghahary, and Reinhold Damko fortheir highly appreciated cooperation and help including the preparations of sam-ples and running the tensile loading-unloading tests of ethylene-butene copoly-mers.
I would like to acknowledge mechanic AG3 staff for providing an enjoyableeducational atmosphere. Getting international friends in our group and profes-sional discussion with them made my work more valuable. Especially, I would liketo thank Dr. habil. Yongqi Wang, Dr. Shiva Prasad Pudasaini, and Dr. BerndMugge for their appreciated help with LINUX system and LaTex software. I wish
to thank Mahmoud Reza Maneshkarimi, M. Eng., Dr. Luca Placcidi, Dr. ha-bil. Ralf Greve, Dipl.-Phys. Angelika Humbert, Dr. Sergio Faria, Chung Fang,M. Sc., Min-Ching Chiou, M. Sc., Dr. Ana Ursescu, for their endless friend-ship. I will never forget their supportive encouragement and sympathies whenmy brother passed away last year. I have more friends whom I wish to thank: Dr.Hazim Rahahleh, Dr.-Ing. Muhanned Hararah, Dr.-Ing. Muhanned Marashdeh,Dr.-Ing. Imad Mosallam.
Foremost, my parents, sisters, and brothers have always encouraged me tofollow my dreams and believed in me, I dedicate this work to them. I wish tothank them who always provided me with invaluable guidance and without theirsupport my dream of PhD degree would not have come true and my academic en-deavors would not have been fulfilling. This dissertation is their accomplishmentas much as it is mine.
Contents
1 Introduction 1
1.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1
1.2 Objectives and Justification . . . . . . . . . . . . . . . . . . . . . 3
1.3 Summary of Contents . . . . . . . . . . . . . . . . . . . . . . . . . 4
2 Thermodynamic constitutive theory 5
2.1 Thermodynamic Constitutive Theory . . . . . . . . . . . . . . . . 5
2.2 Uniaxial Extension . . . . . . . . . . . . . . . . . . . . . . . . . . 17
2.2.1 Approximations . . . . . . . . . . . . . . . . . . . . . . . . 22
2.2.1.1 Incompressible, thermoelastic materials . . . . . . 22
2.2.1.2 Incompressible, thermoelastic materials with ther-mal volume expansion . . . . . . . . . . . . . . . 26
2.2.1.3 Continuum theory and Deformation-Induced Crys-tallization . . . . . . . . . . . . . . . . . . . . . . 26
3 Polymer Crystallization 31
3.1 Semi-Crystalline Polymers . . . . . . . . . . . . . . . . . . . . . . 31
3.2 Models of Semi-Crystalline Polymers . . . . . . . . . . . . . . . . 32
3.2.1 Fringed-micelle model . . . . . . . . . . . . . . . . . . . . 32
i
ii CONTENTS
3.2.2 Folded-chain model . . . . . . . . . . . . . . . . . . . . . . 33
3.2.3 Extended-chain crystallite . . . . . . . . . . . . . . . . . . 33
3.3 Crystallization Kinetics . . . . . . . . . . . . . . . . . . . . . . . . 37
4 Statistical Approach 41
4.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 41
4.2 Overview of the Model . . . . . . . . . . . . . . . . . . . . . . . . 42
4.2.1 Thermodynamic approach of an amorphous network . . . . 46
4.2.2 Thermodynamic approach of a partially crystalline network 49
4.2.3 Mooney representations . . . . . . . . . . . . . . . . . . . 66
5 Model Application 69
5.1 Model Parameters . . . . . . . . . . . . . . . . . . . . . . . . . . . 69
5.1.1 Degree of crystallinity ξ . . . . . . . . . . . . . . . . . . . 69
5.1.2 Parameter a . . . . . . . . . . . . . . . . . . . . . . . . . 70
5.1.3 Number of segments exposed to deformation, Nforce . . . 72
5.1.4 Entropy constant Kξ of partially crystallized chains . . . . 72
5.2 Application of the Model . . . . . . . . . . . . . . . . . . . . . . . 73
5.2.1 Polyisoprene crosslinked rubber . . . . . . . . . . . . . . . 73
5.2.1.1 Crystallization results for the statistical model . . 74
5.2.1.2 Experimental part . . . . . . . . . . . . . . . . . 77
5.2.1.3 Uniaxial stress-strain results . . . . . . . . . . . . 77
5.2.1.4 Mooney representation results . . . . . . . . . . . 84
5.2.1.5 Volume change . . . . . . . . . . . . . . . . . . . 88
CONTENTS iii
5.2.2 Polyolefin thermoplastic elastomers . . . . . . . . . . . . . 90
5.2.2.1 Crystallization results for the model . . . . . . . 90
5.2.2.2 Experimental part . . . . . . . . . . . . . . . . . 93
5.2.2.3 Uniaxial stress-strain results . . . . . . . . . . . . 93
5.2.2.4 Mooney representations . . . . . . . . . . . . . . 101
6 Conclusions and Recommendations 107
6.1 Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 107
6.2 Recommendations . . . . . . . . . . . . . . . . . . . . . . . . . . . 108
A 111
B 113
Bibliography 115
iv CONTENTS
List of Figures
1.1 Schematic of fiber spinning process (This picture is from the web-site: www.fibersource.com/f-tutor/techpag.htm). . . . . . . . . . . 2
2.1 Stress-temperature curve of uniaxial extension. . . . . . . . . . . . 24
3.1 Two different semi-crystalline structures: (a) Fringed-micelle struc-ture (b) Spherulite structure. . . . . . . . . . . . . . . . . . . . 32
3.2 Structure change and selectedWide Angle X-ray Diffraction (WAXD)patterns during stretching and retraction process of rubber. Whereλ is the deformation ratio. . . . . . . . . . . . . . . . . . . . . . . 36
4.1 Example of a long chain of freely rotating segments. . . . . . . . . 42
4.2 Statistical schematic of a freely rotating segments around bonds. . 43
4.3 A schematic view of (a) polymer configuration and (b) polymerconformation. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 44
4.4 End-to-end chain length, with N segments: five segments areshown somewhere in the chain, the remaining ones of which arerepresented by the dotted line till the N th segment. The angle αiis the angle between the ith segment and the r axis. . . . . . . . . 44
4.5 Conformational change in polymer. . . . . . . . . . . . . . . . . . 45
4.6 Boltzmann grave stone in Vienna. . . . . . . . . . . . . . . . . . . 47
4.7 An affine deformation of a material. . . . . . . . . . . . . . . . . . 48
v
vi LIST OF FIGURES
4.8 A schematic of the proposed model of partially crystalline chain . 50
4.9 Mooney-Rivlin representation for cross-linked natural rubber, wheref ∗ equals to σ1
(λ1− 1
λ21)and α−1 equals 1
λ1. . . . . . . . . . . . . . . . 67
5.1 Structural formula of one isoprene molecule. . . . . . . . . . . . . 74
5.2 Theoretical results which show the effect of temperature on crys-tallization of polyisoprene rubber at low strain rate of 0.039 min−1
during the loading process. . . . . . . . . . . . . . . . . . . . . . . 75
5.3 Theoretical results which show the crystallization of polyisoprenerubber at 21◦C and different strain rates during the loading-unloadingprocesses (arrows indicate load path direction). . . . . . . . . . . 76
5.4 Theoretical results which show the crystallization of polyisoprenerubber at 50◦C and different strain rates during the loading-unloadingprocesses (arrows indicate load path direction). . . . . . . . . . . 76
5.5 Theoretical results which show crystallization of polyisoprene rub-ber at 80◦C and low strain rates during the loading-unloading pro-cesses (arrows indicate load path direction). . . . . . . . . . . . . 77
5.6 Temperature effect at 0.039min−1 strain rate on, (a) stress-straincurves for uniaxial loading of polyisoprene rubber (theoretical re-sults are represented by the solid line, while the experimental re-sults by points) and, (b) crystallinity for uniaxial loading of poly-isoprene rubber (theoretical results). . . . . . . . . . . . . . . . . 79
5.7 Effect of strain rates on uniaxial loading-unloading of polyisoprenerubber for, (a) stress-hysteresis at 21◦C (theoretical results are rep-resented by solid and dashed lines, while the experimental resultsby points) and, (b)crystallization at 21◦C (arrows indicate loadpath direction). . . . . . . . . . . . . . . . . . . . . . . . . . . . . 80
5.8 Effect of strain rates on uniaxial loading-unloading of polyisoprenerubber for, (a) stress-hysteresis at 50◦C (theoretical results are rep-resented by solid and dashed lines, while the experimental resultsby points) and, (b) crystallization at 50◦C (arrows indicate loadpath direction). . . . . . . . . . . . . . . . . . . . . . . . . . . . . 81
LIST OF FIGURES vii
5.9 Effect of strain rate on uniaxial loading-unloading of polyisoprenerubber for, (a) stress-hysteresis at 80◦C (theoretical results are rep-resented by solid and dashed lines, while the experimental resultsby points) and, (b) crystallization at 80◦C (arrows indicate loadpath direction). . . . . . . . . . . . . . . . . . . . . . . . . . . . . 82
5.10 Shish-Kebab structure of a polyisoprene rubber sample. . . . . . . 84
5.11 WAXD of polyisoprene rubber at 21◦C and high strain rate 2.34min−1, provided by Prof. T. Alts, for, (a) an undeformed state(λ1 = 1) and, (b) maximum deformation ratio (λ1 = 5). . . . . . 84
5.12 Mooney-representation for uniaxial loading-unloading of polyiso-prene rubber at 21◦C (theoretical results are represented by solidthe line, the experimental results by points , while the dashed lineis Kuhn’s model when no change in crystallinity is assumed in ourstatistical model) for, (a) low strain rate = 0.039 (min−1) and, (b)high strain rate = 2.34 (min−1). . . . . . . . . . . . . . . . . . . . 86
5.13 Mooney-representation for uniaxial loading-unloading of polyiso-prene rubber at 50◦C (theoretical results are represented by thesolid line, the experimental results by points , while the dashedline is Kuhn’s model when no change in crystallinity is assumedin our statistical model) for, (a) low strain rate = 0.039 (min−1)and, (b) high strain rate = 2.34 (min−1). . . . . . . . . . . . . . . 87
5.14 Mooney-representation for uniaxial loading-unloading of polyiso-prene rubber at 80◦C (theoretical results are represented by thesolid line, the experimental results by points , while the dashedline is Kuhn’s model when no change in crystallinity is assumed inour statistical model) for low strain rate = 0.039 (min−1). . . . . . 88
5.15 Change of volume, model results, at different strain rates for, (a)21◦C, (b) 50◦C and, (c) 80◦C. . . . . . . . . . . . . . . . . . . . . 89
5.16 Chemical structure of ethylene-butene copolymer. . . . . . . . . . 90
5.17 Theoretical crystallization of ENX-7256 at different strain ratesfor two temperatures of, (a) at 23◦C, and (b) at 50◦C. . . . . . . . 91
5.18 Theoretical crystallization of ENX-7086 at different strain ratesfor two temperatures of, (a) at 23◦C, and (b) at 50◦C. . . . . . . . 92
viii LIST OF FIGURES
5.19 Effect of temperature on stress-strain loading curves at 0.09 (min−1)strain rate for, (a) at 23◦C and, (b) at 50◦C. (Theoretical resultsare represented by the solid line, while the experimental results bypoints). . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 95
5.20 Stress-strain curves at 5.4 (min−1) strain rates for, (a) ENX-7086and, (b) ENX-7256 (theoretical results are represented by the solidline, while the experimental results by points). . . . . . . . . . . . 97
5.21 Effect of strain rate on stress-strain curves at 23◦C for, (a) ENX-7086 and, (b) ENX-7256 (theoretical results are represented bysolid and dashed lines, while the experimental results by points.Arrows indicate load path direction). . . . . . . . . . . . . . . . . 98
5.22 Effect of strain rate on stress-strain curves at 50◦C for, (a) forENX-7086 and, (b) for ENX-7256 (theoretical results are repre-sented by solid and dashed lines, while the experimental results bypoints. Arrows indicate load path direction). . . . . . . . . . . . . 99
5.23 Three deformation cycles at three maximum strains for ENX-7256at 23◦C and 5.4 min−1 strain rate: (a) stress-strain curves (b)crystallinity-strain curves (theoretical results are represented bysolid and dashed lines, while the experimental results by points.Arrows indicate load path direction). . . . . . . . . . . . . . . . . 100
5.24 Mooney-representation of stress-strain for ENX-7256 at 23◦C for,(a) low strain rate = 0.09 (min−1) and, (b) high strain rate = 5.4(min−1) (theoretical results are represented by the solid line, theexperimental results by points , while the dashed line is Kuhn’smodel when no change in crystallinity is assumed in our statisticalmodel. Arrows indicate load path direction). . . . . . . . . . . . . 102
5.25 Mooney-representation stress-strain for ENX-7256 at 50◦C for, (a)low strain rate = 0.09 (min−1) and, (b) high strain rate = 5.4(min−1) (theoretical results are represented by the solid line, theexperimental results by points , while the dashed line is Kuhn’smodel when no change in crystallinity is assumed in our statisticalmode. Arrows indicate load path directionl). . . . . . . . . . . . . 103
LIST OF FIGURES ix
5.26 Mooney-representation of stress-strain for ENX-7086 at 23◦C for,(a) low strain rate = 0.09 (min−1) and, (b) high strain rate = 5.4(min−1) (theoretical results are represented by the solid line, theexperimental results by points , while the dashed line is Kuhn’smodel when no change in crystallinity is assumed in our statisticalmodel. Arrows indicate load path direction). . . . . . . . . . . . 104
5.27 Mooney-representation of stress-strain for ENX-7086 at 50◦C for,(a) low strain rate = 0.09 (min−1) and, (b) high strain rate = 5.4(min−1) (theoretical results are represented by the solid line, theexperimental results by points , while the dashed line is Kuhn’smodel when no change in crystallinity is assumed in our statisticalmodel. Arrows indicate load path direction). . . . . . . . . . . . 105
x LIST OF FIGURES
List of Tables
5.1 Effect of strain rate on the constants of the relaxation time forloading-unloading polyisoprene rubber at all temperatures . . . . 69
5.2 Effect of strain rate on the constants of the relaxation time forloading-unloading of the thermoplastic elastomer (both types) atall temperatures . . . . . . . . . . . . . . . . . . . . . . . . . . . 70
5.3 Parameter a values for loading process of polyisoprene . . . . . . 71
5.4 Parameter a values for loading process of ENX-7086 . . . . . . . 71
5.5 Parameter a values for loading process of ENX-7256 . . . . . . . 71
5.6 Values of νo for three different polymeric materials. . . . . . . . . 73
5.7 Physical and chemical properties of the thermoplastic ethylene-butene copolymer . . . . . . . . . . . . . . . . . . . . . . . . . . 90
A.1 Parameter a: Values of adjustable constants during unloading pro-cess for polyisoprene rubber: . . . . . . . . . . . . . . . . . . . . 111
A.2 Parameter a: Values of adjustable constants during unloading pro-cess for ENX-7256 elastomer: . . . . . . . . . . . . . . . . . . . . 111
A.3 Parameter a: Values of adjustable constants during unloading pro-cess for ENX-7086 elastomer: . . . . . . . . . . . . . . . . . . . . 111
B.1 Nforce: Values of adjustable constants during loading process forpolyisoprene rubber: . . . . . . . . . . . . . . . . . . . . . . . . . 113
xi
xii LIST OF TABLES
B.2 Nforce: Values of adjustable constants during loading process forENX−7256 elastomer: . . . . . . . . . . . . . . . . . . . . . . . . 113
B.3 Nforce: Values of adjustable constants during loading process forENX−7086 elastomer: . . . . . . . . . . . . . . . . . . . . . . . . 113
Zusammenfassung
Deformations-induzierte Kristallisation ist entscheidend fur die Vorherbestim-mung der endgultigen mechanischen Eigenschaften von Elastomeren und Gummi.Elastomere Netzwerke zeigen einen steilen Anstieg in der Spannungs-DehnungsKurve mit bedeutenden Hysteresis-Effekten, beides wird dem Phanomen derdeformations-induzierten Kristallisation zugeordnet.
Die Thermodynamik von gummi-ahnlichen Polymeren ist untersucht worden;und uni-axiale Dehnungen mit einigen Approximationen werden diskutiert, umeinen Uberblick uber die vorgeschlagene thermodynamische Materialtheorie zuerhalten.
Ein thermodynamisch statistisches Modell wird vorgeschlagen zum Studiumdes Spannungs-Dehnungs Verhaltens von elastomeren Netzwerken und die Abhang-igkeit der Spannungskoeffizienten vom Kristallisationsgrad wird berechnet. Diesberuht auf einer modifizierten Verteilungsfunktion von Kettensegmenten fur Ket-ten von endlicher Lange.
Die Berechnung der Kristallisation basiert auf Gleichungen aus der Thermo-dynamik der irreversible Prozesse; hierbei werden Deformationsgeschwindigkeitund Temperatur berucksichtigt.
Mooney Darstellungen der Spannungs-Dehnungs Kurven werden eingefuhrt,um die starke Abhangigkeit der Spannungskoeffizenten vom Kristallisationsgradzu zeigen.
Uni-axiale Belastungsprozesse mit anschliessender Entlastung werden unter-sucht fur mehrere Deformationsgeschwindigkeiten und Temperaturen, um die Ef-fekte der molekularen Orientierung und der dehnungs-induzierten Kristallisationzu zeigen in Polyisopren Gummi und in Ethylen-Butan Kopolymeren (thermo-plastische Elastomere, TPE). Der Einfluss des Relaxationsprozesses und der De-formationsgeschwindigkeit auf die Kristallisation wird illustriert.
Die Hysteresis der Spannungs-Dehnungs Relation und das inelastische Defor-mationsverhalten wird der dehnungs-induzierten Kristallisation und ihrer Umwand-lung zugeordnet; dies wird insbesondere evident fur grosse Deformationsgeschwindig-keiten und tiefe Temperaturen (d.h. oberhalb der Glasubergangstemperatur).
Die Modell-Ergebnisse zeigen gute Ubereinstimmung mit Experimenten, diein dieser Studie durchgefuhrt worden sind.
Abstract
Deformation induced crystallization is crucial for determining the final me-chanical properties of elastomers-rubber. Elastomeric networks show high upturnin the stress-strain curves with a significant hysteresis, this is attributed to thedeformation induced crystallization phenomenon.
Thermodynamics of rubber-like high polymers have been studied, and uniaxialextension with some approximations is discussed to obtain an overview of theproposed thermodynamic constitutive theory.
A thermodynamical statistical model is presented for studying the stress-strain behaviour of elastomeric networks, and the dependence of the stress coef-ficients on the degree of crystallinity. This is based on the modified distributionof chains of finite length.
A crystallization formulation based on irreversible thermodynamics is adoptedto describe the crystallization taking into account the effects of strain rate andtemperature.
Mooney representation curves are introduced in this study to show the strongdependence of stress coefficients on the degree of crystallinity.
Both uniaxial loading and unloading are investigated for a range of strainrates and temperatures, to explain the effect of molecular orientation and straininduced crystallization in polyisoprene rubber and ethylene-butene copolymers(thermoplastic elastomers). The effect of relaxation process, and the rate ofdeformation on crystallization has been illustrated.
The hysteresis of the stress-strain relation and inelastic deformation behaviouris attributed to the deformation induced crystallites and their transformation; thisis clearly shown at high strain rates and low temperatures (i.e. above the glasstransition temperature).
The model results show good agreement with experimental data that havebeen determined in this study.
Chapter 1
Introduction
1.1 Introduction
Of all the materials known to man, no material can match the remarkablebehaviour of rubber and rubberlike materials (i.e. thermoplastic elastomers).They are capable of sustaining large deformations without rupture; a maximumextension of five to ten times the undeformed lengths is a common property ofthem. When a rubber-elastomeric material is stretched, it achieves its highestmodulus of elasticity at maximum deformations. It possesses the capacity torecover spontaneously its original dimensions, with little appreciable fraction ofpseudo-plastic residual deformation.
A wide spectrum of polymeric materials have been developed to replace thenaturally occuring materials. Therefore, thermoplastic elastomers (TPEs) arewidely used, due to the ease of processing; they behave like a cross-linked rubberunder ambient conditions. TPEs differ from cross-linked rubber inso far as thecross-links are not covalent bonds but physical links, e.g. consisting of crystallizedchain segments. These can be molten by heating, thus allowing thermoplasticprocessing.
Elastomeric polymers are commonly used in everyday life. In order to suc-cessfully manipulate their applicability, it is indispensable to completely under-stand the relationship between the structure and the properties of the polymer.The mechanical behaviour is closely related to the morphology and consequentlydepends on the thermal and deformation histories experienced by the polymerduring the process.
A number of polymers including natural and synthetic rubbers and thermo-plastic elastomers have the tendency to crystallize both mechanically and ther-
1
2 CHAPTER 1. INTRODUCTION
mally. In many applications, the formation of highly oriented or extended crystalshas a beneficial impact on the mechanical behaviour of the polymer. This canbe noticed in film blowing, injection molding and, drastically, in fiber spinningas shown in figure.
Figure 1.1: Schematic of fiber spinning process (This picture is from the website:www.fibersource.com/f-tutor/techpag.htm).
In fibers, the formation of the extended crystalline phase in the direction ofextension greatly reinforces and increases the strength of the fiber.
The phenomenon of orientation in polymers is shown by the larvae of silkmoth, and by spiders. The former weave their heads about inside of cocoon, sothat as they spin their silk, it is pulled and oriented. The latter, by suddenlydropping on their drag line, produce a highly oriented and very strong fiber.
Recent fields of research on elastomeric networks have focused on mechan-ical properties under deformation. It has been frequently observed that somenetworks show rapid upturn in stress-strain isotherm. Many considerable views
1.2. OBJECTIVES AND JUSTIFICATION 3
have been proposed to interprete the cause of the upturn. It was interpretedmainly as a result of limited chain extensibility as being due to approximationinherent in the Gaussian theory. The other considerable view of this behaviouris attributed to deformation-induced-crystallization.
It is therefore indispensable to provide a qualitative understanding of the be-haviour of the elastomeric network, and to completely predict the crystallizationfrom macroscopic deformation during drawing.
1.2 Objectives and Justification
The foregoing discussion of polymer crystallization morphology, with its em-phasis on the importance of deformation-induced crystallization would not becomplete without a brief mention of the statistical approach to predict crystal-lization of elastomeric networks. According to this approach, a polymer is treatedas a network of freely-jointed chains crosslinked at junction points, whose motionsare affine to the macroscopic deformation.
Stress-strain dependence of crosslinked networks was first described by theclassical Gaussian rubber elasticity theory in the pioneering work of Kuhn [41],[42].A thermodynamic theory of strain-induced crystallization was first developed byFlory [21]. Both theories do not describe the real behaviour of physically orchemically crosslinked networks.
The goals of the present study may be summarized as follows:
(1) Gain a better understanding of the mechanism of deformation-induced-crystalization.
(2) Develop a model to simulate crystallization taking place at different strainrates and temperatures for uniaxial loading-unloading processes of elastomericnetwork chains.
(3) Modify the Gaussian distribution for chains of finite lengths to describethe end-to-end vector distribution function and the contribution of chain to crys-tallinity.
(4) Based on the results of the above mentioned objectives, to propose astatistical model for stress-strain-crystallinity prediction.
(5) Perform tensile experiments for both amorphous and semi-crystalline elas-tomeric network chains, to validate the modeled results of the 4 above points.
4 CHAPTER 1. INTRODUCTION
1.3 Summary of Contents
The dissertation is organized in the following way.
Chapter 2 deals with thermodynamics of rubber-like high polymers. Anoverview of the thermodynamic constitutive theory is obtained by discussinguniaxial extension at certain constant conditions (mainly temperature and exter-nal pressure). Approximations and internal constraints have been employed tosimplify the theory [8].
In chapter 3, a review of the fundamental aspects of polymer crystallization isgiven, including various explanations of rubber as well as thermoplastic copolymercrystallization. The main section of this chapter is to develop the mathemati-cal model and to simulate stress-induced crystallization taking place at differentparameters. This model is given according to irreversible thermodynamics. It iscapable to calculate the degree of crystallinity for both the uniaxial stretchingloading and retraction unloading processes for a range of strain rates and tem-peratures. In this model, hysteresis loops and inelastic deformation behaviour(pseudo-plastic residual strain) is discussed in detail.
In chapter 4, a modified Gaussian distribution, based on affine deformation,is employed for chains of finite lengths to describe the end-to-end vector distri-bution function and the contribution of that chain to crystallinity. Stress-strain-crystallinity relations are then derived from conformational entropy. This is donein the context of statistical thermodynamics.
Chapter 5 is a discussion of the model results as well as experimental re-sults. The experimental results of uniaxial loading-unloading extension are fullydiscussed and compared with those predicted for validation. The different poly-meric elastomers (i.e. with different values of reference degree of crystallinity)that have been used in these experiments were obtained from Rieter Automotivesystem company-Gundernhausen. The experimental part has been performed inthe laboratories of the German Polymer Institute-Darmstadt. Observed hystere-sis loops and residual strain (pseudo-plastic effect) have been investigated forrubber and thermoplastic elastomer experiments at different ranges of the defor-mation ratios, temperatures, and strain rates. Model parameters and fittings arediscussed in this section as well.
Chapter 6 gives the general conclusions and recommendations for potentialfuture work.
Chapter 2
Thermodynamics of Rubber-Like
High Polymers
2.1 Thermodynamic Constitutive Theory
The goal of thermodynamics of rubber-like high polymers is the determinationof the fields of density ρ(x, t), of the motion xi = χi(Xα, t), of the temperatureT (x, t) and the degree of crystallisation ξ(x, t). Thus, the equations for thedetermination are the balance equations for mass, linear momentum, moment ofmomentum, internal energy and degree of crystallinity:
ρ = −ρvi,i , ρvi = tij,j ,
tij = tji , ρu = −qj,j + tijvi,j , (2.1)
ρξ = −ψj,j + A ,
where vi, tij, qj, ψj are components of the velocity v, the Cauchy-stress t, theheat flux q and the flux of crystallinity ψψψ (through a material surface, moving withmaterial velocity v) with respect to a Cartesian co-ordinate system (observer-system), which is rigidly connected to an inertial system. u denotes the specificinternal energy and A has the meaning of a transformation rate (per unit volumeand time) of chain segments from the amorphous into the crystalline state. Thegravitation is neglected. The symbols ,i and ˙ denote partial derivatives withrespect to spatial co-ordinates and the material time derivative, respectively.Hence, for a function f (x, t)
f,i :=∂f
∂xi, f :=
∂f
∂t+ vl
∂f
∂xl. (2.2)
According to Einstein’s summation convention, doubly repeated co-ordinate in-dices denote summation from 1 to 3. The symmetry of the stress tensor t is
5
6 CHAPTER 2. THERMODYNAMIC CONSTITUTIVE THEORY
a consequence of conservation of moment of momentum in non-polar materials.The velocity vi and the deformation gradient Fiα are obtained by partial deriva-tives of the material motion χi(Xα, t):
vi :=∂χi(Xα, t)
∂t, Fiα :=
∂χi(Xα, t)
∂Xα
. (2.3)
Xα denotes the co-ordinates of a material element in some reference configuration,which we want to identify with some undeformed equilibrium state of the materialwith fixed values T = TR of temperature, p = pR of pressure and ξ = ξR of degreeof crystallinity. In this reference state Fiα|R = δiα, the unit tensor.
We now assume, that the material does not fracture during deformation.Then, due to det F > 0, the inverse deformation Xα = Xα(xi, t) exists. Conse-quently the inverse deformation gradient
(F−1)αi :=∂Xα(xi, t)
∂xi(2.4)
is well defined. It holds
(F−1)αiFiβ = δαβ , Fiα(F−1)αj = δij , (2.5)
where δαβ and δij are Cartesian components of the unit tensor [71].
The mass balance (2.1)1 can be integrated using (2.3), the result being
det F =ρR
ρ=
v
vR
, (2.6)
where v = 1/ρ is the specific volume, and ρR, and vR = 1/ρ
R,respectively, are
the density and the specific volume in the reference state.
With (2.6) one can introduce a new deformation measure
Giα := (v
vR
)−1/3Fiα , detG = 1 . (2.7)
This measure has the special property, that it does not contain volume changes.Pure volume changes and isochoric deformations can be treated separately.
The decomposition (2.7) is rather important for the treatment of rubber-likehigh polymers, since the total deformation can be separated into inelastic andelastic contributions. The inelastic deformation -thermal volume expansion anda change of the volume by a change of the internal structure- is contained in thevolume change ( v
vR
), while the elastic deformation is described by Giα. The last
one is isochoric by definition. With this all deformations which are due to volume
2.1. THERMODYNAMIC CONSTITUTIVE THEORY 7
changes are explicity separated. This is of crucial importance for the constitutivetheory of rubber-like high polymers.
To come to the main goal of thermodynamics - which means to transformthe balance equations to a set of field equations for the determination of thefields ρ(x, t), xi = χi(Xα, t), T (x, t), and ξ(x, t)- the fields of stress tij(x, t), heatflux qi(x, t), internal energy u(x, t), crystallization flux ψi(x, t) and crystallizationrate A(x, t) must be related in a materially dependent manner to the independentfields ρ, χi, T, ξ. Such relations are called constitutive equations.
For rubber-like high polymers we make the following assumptions:
tij(x, t) = tij(v, T, ξ, Giα, T,i) ,
qi(x, t) = qi(v, T, ξ, Giα, T,i) ,
ψi(x, t) = 0 , (2.8)
u(x, t) = u(v, T, ξ, Giα, T,i) ,
A(x, t) = A(v, T, ξ, Giα, T,i) .
Herein the hypothesis of equipresence has been applied, according to which it isassumed that a variable which appears in one constitutive equation can appear inall of them. In this way one avoids prejudices in the formulation of constitutiveequations.
The constitutive equation (2.8)3 about the flux of crystallization means, thatthe crystallites move with material velocity and do not diffuse against this veloc-ity. This relates to the microscopic view, that crystallites inside their amorphoussurroundings are just transformed during deformation, but cannot move relativeto their amorphous surroundings.
We now introduce by the definition
p := −1
3tll = p(v, T, ξ, Giα, T,i) , (2.9)
an internal pressure p(x, t). Since rubber-like high polymers are compressible,∂p/∂v 6= 0, the constitutive equation (2.9) can be inverted with respect to thespecific volume
v(x, t) = v(p, T, ξ, Giα, T,i) ; (2.10)
instead of the specific volume the internal pressure can be chosen as an indepen-
8 CHAPTER 2. THERMODYNAMIC CONSTITUTIVE THEORY
dent field variable. Hence, we obtain
tij(x, t) = −p(x, t)δij + tij(p, T, ξ, Giα, T,i) with tll = 0 ,
qi(x, t) = qi(p, T, ξ, Giα, T,i) ,
ψi(x, t) = 0 , (2.11)
u(x, t) = u(p, T, ξ, Giα, T,i) ,
A(x, t) = A(p, T, ξ, Giα, T,i) .
The constitutive equations (2.10) and (2.11) are equivalent to (2.8). The formof (2.10) and (2.11) is better suited for the description of the material behaviourof rubber-like high polymers, as we shall see later. Therefore we choose thisformulation, [5].
If one inserts the constitutive equations (2.8) or (2.10) and (2.11) into the bal-ance equations (2.1), these become field equations for the independent fields. Ev-ery solution of the field equations to a Cauchy-problem (Boundary-value and/orinitial value problem) is called a thermodynamic process.
If the constitutive equations would be known, the exercise of thermodynamicswould be to solve the field equations, and this is a purely mathematical problem.The constitutive equations, however, are in reality not known for no material, soneither for high polymers. For this reason the main exercise of thermodynamics isfirst of all to restrict the dependence of constitutive equations (on their variables)by general requirements. This is the content of the thermodynamic constitutivetheory, which we shall formulate now.
There exist three generally valid requirements for the restriction of constitu-tive equations. These are the principle of material symmetry [71], The principleof material observer invariance, and the entropy principle [5, 54].
The principle of material symmetry states, that the constitutive equationsare form invariant with respect to symmetry transformations in the undeformedstate. For the isotropic high polymers considered here (with inversion symmetry)this means, that the constitutive equations can depend on Giα only via the leftCauchy-Green deformation tensor
βij := GiαGjα . (2.12)
The principle of material observer invariance states, that the constitutiveequations which are measured by an observer in an inertial frame, are the sameas for another observer in a frame, which is translated and rotated against theinertial frame. Then, the constitutive equations are form invariant under Eu-clidean transformations. From this one concludes, that the constitutive functions
2.1. THERMODYNAMIC CONSTITUTIVE THEORY 9
are isotropic functions of T,i and βij and possess the following irreducible repre-sentations [64]:
u = u(p, T, ξ, Iα, Hα) , A = A(p, T, ξ, Iα, Hα) , v = v(p, T, Iα, Hα) ,
qi = −[κ1δij + κ2βij + κ3(βββ2)ij]T,j , (2.13)
tij = −pδij −2
3(C1I1 + 2C2I2)δij + 2(C1 + C2I1)βij − 2C2(βββ
2)ij
+α1
[
(T⊗T)ij −H1
3δij
]
+ α2
[1
2(T⊗ βββ ·T + βββT⊗T)ij −H2δij
]
+α3
[1
2
(T⊗ βββ2T + βββ2T⊗T
)
ij−H3δij
]
.
Here Iα(α = 1, 2) are
I1 := trβββ = βll , I2 :=1
2[(trβββ)2 − trβββ2] , (2.14)
the principal invariants of the elastic deformation (I3 := detβββ = 1),
Ha := T · (βββa−1T) = T,i(βββa−1)ijT,j (a = 1, 2, 3) . (2.15)
Ha are the irreducible invariants, which can be formed with the temperaturegradient.
The scalar coefficients κ1, κ2, κ3 in the heat flux and C1, C2 and α1, α2, α3 inthe stress tensor are in general functions of p, T, ξ, Iα, Ha . The terms in the stresstensor are trace free, except for the pressure part, e.g. tr(t + p1) = tll + 3p = 0.One can easily prove this with the help of the Hamilton-Cayley-Theorem :
(βββ3)ij = I1(βββ2)ij − I2βij + δij . (2.16)
As a third general principle for the restrictions on constitutive equations servesthe entropy principle . We postulate it in the form given by Muller [54].
i) There exists a mass - proportional entropy. This satisfies a balance equationof the form:
ρs = −φi,i + πs . (2.17)
ii) The specific entropy s and the (non-convective) entropy flux φi are given byconstitutive equations, which satisfy the principle of material symmetry and theprinciple of material observer invariance. For rubber-like isotropic high polymerswe then have
s(x, t) = s(p, T, ξ, Giα, T,i) = s(p, T, ξ, Iα, Ha) , (2.18)
φj(x, t) = φj(p, T, ξ, Giα, T,i) = −[ϕ1δij + ϕ2βij + ϕ3(βββ2)ij]T,j ,
10 CHAPTER 2. THERMODYNAMIC CONSTITUTIVE THEORY
where ϕ1, ϕ2, ϕ3 are scalar functions of p, T, ξ, Iα, Ha.
iii) At heat conducting material walls with continuous temperature, the nor-mal component of the entropy flux is continuous,
[[φj]]ej = 0 for [[T ]] = 0 , (2.19)
[[ψ]] := ψ+ − ψ− means the difference of single sided limiting values when ap-proaching the wall from either side, eee is the unit normal vector of the heat con-ducting wall.
iv) The entropy production density is non-negative for all thermodynamicprocesses,
πs ≥ 0 ∀ thermodynamic processes . (2.20)
The key for drawing inferences from the entropy principle is inequality (2.20).It doesn’t hold for arbitrary fields ρ, χi, T, ξ, but only for thermodynamic pro-cesses. The inequality is therefore valid for all solutions of the fields equations,which follow from the balance laws. These field equations formulate restrictionsfor the independent fields. One can account for these restrictions by the introduc-tion of Lagrangian parameters. One then obtains an inequality that is equivalentto (2.20) and (2.17) of the following form:
ρs + φi,i − ∧ρ(ρ+ ρvi,j)− ∧vi (ρvi − tij,j)
− ∧u(ρu+ qj,j − tijvi,j)− ∧ξ(ρξ + ψj,j − A) ≥ 0 , (2.21)
which is valid for arbitrary (unrestricted) fields ρ, χi, T and ξ [43].
According to (2.3), (2.4), and (2.7) the velocity gradient may be written as
vi,j = Fiα(F−1)αj =
1
3
v
vδij + Giα(G
−1)αj . (2.22)
Now, one inserts into (2.21) the constitutive equations (2.18), (2.10) and (2.11)
2.1. THERMODYNAMIC CONSTITUTIVE THEORY 11
and performs the differentiations. One obtains thus with v = 1/ρ and (2.22)
ρ
[∂s
∂p− ∧u
(∂u
∂p+ p
∂v
∂p
)]
p+ ρ
[∂s
∂T− ∧u
(∂u
∂T+ p
∂v
∂T
)]
T
+ ρ
[∂s
∂ξ− ∧u
(∂u
∂ξ+ p
∂v
∂ξ
)
− ∧ξ]
ξ
+ ρ
[∂s
∂Giα
− ∧u(
∂u
∂Giα
+ p∂v
∂Giα
− vtij(G−1)αj
)
− ∧ρ(G−1)αi
]
Giα
+ ρ
[∂s
∂T,i− ∧u
(∂u
∂T,i+ p
∂v
∂T,i
)]
(T,i)− ρ ∧vi vi + ∧ξA (2.23)
+
[
∂φj∂p
− ∧u∂qj∂p− ∧vj + ∧vk
∂tkj∂p
]
p,j
+
[
∂φj∂T
− ∧u∂qj∂T
+ ∧vk∂tkj∂T
]
T,j +
[
∂φj∂ξ
− ∧u∂qj∂ξ
+ ∧vk∂tkj∂ξ
]
ξ,j
+
[
∂φj∂Giα
− ∧u ∂qj∂Giα
+ ∧vk∂tkj∂Giα
]
Giα,j
+
[
∂φj∂T,i
− ∧u ∂qj∂T,i
+ ∧vk∂tkj∂T,i
]
T,ij ≥ 0 .
This inequality is valid for arbitrary variations of the (independent) fields. With-out restriction of generality one can choose the Lagrange parameters ∧u,∧ξ,∧ρ insuch a way, that the expressions in the brackets in front of T , ξ and Giα disappear.Then these Lagrange parameters are functions of the variables p, T, ξ, Giα, T,i ofthe constitutive equations. Further, the Lagrange parameter ∧vi can be chosensuch, that it is independent of vi. Then ∧vi = 0 must vanish, since otherwisethe inequality can be contradicted. Now it follows, that the inequality (2.23) is
linear in p, (T,j ), p,j, ξ,j, Giα,j and T,ij. It could, consequently, be violated forarbitrary variations of these fields, except if the corresponding forefactors vanish.This gives
∂s
∂T= ∧u
(∂u
∂T+ p
∂v
∂T
)
,
∂s
∂p= ∧u
(∂u
∂p+ p
∂v
∂p
)
, (2.24)
∂s
∂ξ= ∧u
(∂u
∂ξ+ p
∂v
∂ξ
)
+ ∧ξ ,
∂s
∂Giα
= ∧u(
∂u
∂Giα
+ p∂v
∂Giα
− vtij(G−1)αj
)
+ ∧ρ(G−1)αj ,
∂s
∂T,i= ∧u
(∂u
∂T,i+ p
∂v
∂T,i
)
;
12 CHAPTER 2. THERMODYNAMIC CONSTITUTIVE THEORY
∧vi = 0 , (2.25)
∂φj∂p
= ∧u ∂qj∂p
,
∂φj∂ξ
= ∧u ∂qj∂ξ
, (2.26)
∂φj∂Giα
= ∧u ∂qj∂Giα
,
∂φ(j∂T,ij)
= ∧u ∂q(j∂T,ij)
.
There remains the residual inequality
πs =
(
∂φj∂T
− ∧u∂qj∂T
)
T,j + ∧ξA ≥ 0 , (2.27)
which holds for unrestricted processes.
It seems, that we do not come closer to our wanted goal, namely to findrestrictions on the constitutive equations for v, u, tij, qj, A, because we introduced
new unknown constitutive functions s, φj and unknown Lagrangean parameters∧u,∧ξ,∧ρ. But this only seems so, because the new constitutive functions canbe eliminated. First we recognise, that the ” Ansatz” φj = ∧uqj satisfies therelations (2.26), provided ∧u is only a function of T,
φj = ∧u(T ) qj . (2.28)
This is a sufficient solution of (2.26). That it is also necessary, can be proven withthe help of the representations (2.18)2 for the entropy flux and (2.13)4 for theheat flux after lengthly calculations. The entropy flux is therefore proportionalto the heat flux with a factor of proportionality ∧u(T ), which is only a function oftemperature. To determine this factor we use the requirement (iii) of the entropyprinciple on heat conducting material walls. At these walls, as a consequence ofthe energy law, the normal component of the heat flux must be continuous:
[[qi]] ei = 0 . (2.29)
If the heat conducting wall is nothing else but the interface between two heatconducting rubber-like high polymers + and −, the temperature is continuousand it follows from (2.29) and (2.19)
∧u+(T ) = ∧u−(T ) . (2.30)
2.1. THERMODYNAMIC CONSTITUTIVE THEORY 13
The Lagrange parameter ∧u(T ) is continuous on heat conducting interfaces. Con-sequently, it is a universal function of temperature for all heat conducting rubber-like high polymers.
For an ideal gas the Lagrange parameter ∧ug (T ) = 1/T is identified with (1over the absolute ideal gas temperature). If one contacts the high polymer via aheat conducting interface with an ideal gas, one has
∧u(T ) = 1
T. (2.31)
The Lagrange parameter ∧u(T ) for high polymers is identified with the reciprocal(absolute) temperature.
Now we use this result and insert it in (2.24). With the specific enthalpy
h := u+ pv , (2.32)
we obtain
∂s
∂T=
1
T
∂h
∂T,
∂s
∂p=
1
T(∂h
∂p− v) , (2.33)
∂s
∂ξ=
1
T
∂h
∂ξ+ ∧ξ ,
∂s
∂Giα
=1
T
(
∂h
∂Giα
− vtij(G−1)αj
)
− ∧ρ(G−1)αi ,
∂s
∂T,i=
1
T
∂h
∂T,i.
We assume, that the entropy is twice continuously differentiable. From the in-terchangement of the second derivatives one concludes, among other things,
∂h
∂T,i= 0 ,
∂v
∂T,i= 0 ,
∂∧ξ∂T,i
= 0 ,∂∧ρ∂T,i
= 0 ,∂tkj∂T,i
= 0 . (2.34)
The specific enthalpy, the specific volume, the trace-free contribution of theCauchy-stress and the Lagrange parameters ∧ξ and ∧ρ are independent of thetemperature gradient. The same result holds according to (2.33)5 and (2.32) forthe entropy and the internal energy
∂s
∂T,i= 0 ,
∂u
∂T,i= 0 . (2.35)
14 CHAPTER 2. THERMODYNAMIC CONSTITUTIVE THEORY
This implies important simplifications in the representations (2.13) and (2.18) ofthe constitutive functions: The specific volume, the internal energy, the entropy,the enthalpy and the coefficients C1 and C2 of the stress tensor are independentof the invariants Ha (a = 1, 2, 3). Further, the coefficients of the stress tensor
α1 = α2 = α3 = 0 (2.36)
vanish. The chemical production density A, and the coefficients κ1, κ2, κ3 in theheat flux may, however, further depend on Ha (a = 1, 2, 3).
We insert now the representations (2.13) under the use of (2.36) and (2.33)and obtain with (2.12), (2.14) and (2.16), using the following mathematical ex-pressions
∂s
∂Giα
=∂s
∂I1× ∂I1∂Giα
+∂s
∂I2× ∂I2∂Giα
,
∂h
∂Giα
=∂h
∂I1× ∂I1∂Giα
+∂h
∂I2× ∂I2∂Giα
,
after lengthy calculations1:
∧ρ = v
T
2
3(C1I1 + 2C2I2) (2.37)
and
∂s
∂T=
1
T
∂h
∂T,
∂s
∂p=
1
T(∂h
∂p− v) , (2.38)
∂s
∂ξ=
1
T
∂h
∂ξ+ ∧ξ ,
∂s
∂Iα=
1
T(∂h
∂Iα− vCα) , (α = 1, 2) .
To simplify notation, the hats ˆ above the constitutive functions have beendropped.
The Cauchy stress tensor can be somewhat simplified using the Hamilton-Cayley Theorem (2.16) and (2.36):
tij = −pδij −2
3(C1I1 − C2I2)δij + 2C1βij − 2C2(βββ
−1)ij . (2.39)
If one introduces the specific free enthalpy
g := h− Ts , (2.40)
1These calculations are available upon request.
2.1. THERMODYNAMIC CONSTITUTIVE THEORY 15
then relations (2.38) simplify formally to
∂g
∂T= −s ,
∂g
∂p= v ,
∂g
∂ξ= −T∧ξ ,
∂g
∂Iα= vCα (α = 1, 2) . (2.41)
With these, the Lagrangean parameter ∧ξ has finally been identified. It is givenby the derivative of the free enthalpy with respect to the degree of crystallinity.
The integrability conditions for the free enthalpy are
∂s
∂p= − ∂v
∂T,∂s
∂ξ=∂(T∧ξ)∂T
,∂s
∂Iα= −∂(vCα)
∂T, (2.42)
∂v
∂ξ= −T ∂∧
ξ
∂P,
∂v
∂Iα=∂(vCα)
∂P, T
∂∧ξ∂Iα
= −∂(vCα)
∂ξ,
∂(vC1)
∂I2=∂(vC2)
∂I1.
We shall produce some further relations. We introduce by cp :=∂h∂T
the specificheat capacity at constant pressure. From (2.38) we conclude with (2.42)
∂h
∂T= cp = T
∂s
∂T,
∂h
∂p= v − T
∂v
∂T, (2.43)
∂h
∂ξ= T 2 ∂∧ξ
∂T,
∂h
∂Iα= vCα − T
∂(vCα)
∂T.
These relations imply the integrabitlity conditions
∂cp∂p
= −T ∂2v
∂T,∂cp∂ξ
=∂
∂T(T 2∂∧ξ
∂T) ,
∂cp∂Iα
= −T ∂2(vCα)
∂T 2. (2.44)
For the internal energy u = h− pv we obtain with (2.43)
∂u
∂T= cp − p
∂v
∂T,
∂u
∂p= −T ∂v
∂T− p
∂v
∂p, (2.45)
∂u
∂ξ= T 2 ∂∧ξ
∂T− p
∂v
∂ξ,
∂u
∂Iα= vCα − T
∂(vCα)
∂T− p
∂v
∂Iα.
With this all general relations for rubber-like high polymers are derived.
16 CHAPTER 2. THERMODYNAMIC CONSTITUTIVE THEORY
There remains to draw conclusions from the residual-inequality (2.27). Thissimplifies with (2.28) and (2.31) to
Πs = −1
T 2qj T,j + ∧ξA ≥ 0 . (2.46)
We define thermostatic equilibrium as a state with spatially and temporarilyconstant temperature T, with temporarily constant deformation Giα, temporarilyconstant pressure p and temporarily constant degree of crystallization ξ. Accord-ing to (2.1) and (2.11)3 the chemical production density A = 0. We denote thisthermostatic equilibrium state by |E (equilibrium).
The entropy production assumes in equilibrium its minimum value zero. Nec-essary conditions are
∂Πs
∂T,j|E= 0 ,
∂Πs
∂A|E= 0 , (2.47)
∣∣∣∣∣∣∣
∣∣∣∣∣∣∣
∂2Πs
∂T,iT,j|E
∂2Πs
∂T,i ∂A|E
∂2Πs
∂A ∂T,j|E
∂2Πs
∂A2|E
∣∣∣∣∣∣∣
∣∣∣∣∣∣∣
∼ non− negative definite (2.48)
Relations (2.47) give
qi|E = 0 , ∧ξ|E= 0 . (2.49)
According to (2.13)4, (2.49)1 is satisfied automatically, (2.49)2 means accordingto (2.41)3
∧ξ|E= − 1
T
∂g
∂ξ|E= 0 . (2.50)
This relation determines the equilibrium value ξ|E= ξ(T, p, Iα) of the degree of
crystallinity.
The matrix of the second derivatives in equilibrium is, according to (2.13) and(2.43)3,
∂2Πs
∂T,iT,j|E
= − 1
T 2
∂q(i∂T,j)
|E=
1
T 2
[κ1|Eδij + κ2|Eβij + κ3|E(βββ2)ij
],
∂2Πs
∂T,i∂A|E
=∂∧ξ∂T,j
|E= 0 ,
∂2Πs
∂A2|E
=∂∧ξ∂A
|E.
2.2. UNIAXIAL EXTENSION 17
From (2.48), there follows
κ1|Eδij + κ2|Eβij + κ3|E(βββ2)ij ∼ non− negative difinite , (2.51)
∂∧ξ∂A
|E≥ 0 . (2.52)
With these all general restrictions on the constitutive equations of rubber-likehigh polymers are obtained.
2.2 Uniaxial Extension
To obtain a first overview about the content of the thermodynamic constitu-tive theory, we will discuss the uniaxial extension at constant temperature T andconstant external pressure P. The direction of extension shall be the 1-direction.Let the extensional force per unit cross section in the reference state be σ1 (nom-inal stress). This is related to the 11-component of the 1st Kirchhoff-Piola-stress
Tiα = tij(F−1)αj detF (2.53)
as follows:
σ1 = T11 + P (F−1)11 detF . (2.54)
The states of stress and deformation are uniform and along the Eigen-direction,where for the Cauchy-stress the following boundary conditions at the free surfacesperpendicular to the direction of extension apply:
t22 = t33 = −P , (2.55)
Furthermore, the deformation gradient in the used Cartesian co-ordinate systemhas the representation
||Fiα|| =
Λ1 0 00 Λ2 00 0 Λ3
. (2.56)
Λ1 is the ratio of the length L at constant T and constant P of the extendedmaterial probe to the length LR in the undeformed reference state at the referencetemperature TR, reference pressure PR and crystallinity ξR, namely
Λ1 :=L
LR
. (2.57)
Using (2.6) the deformations Λ2 = Λ3 perpendicular to the extensional directionbecome
Λ2 = Λ3 =
√v
vR
1
Λ1
. (2.58)
18 CHAPTER 2. THERMODYNAMIC CONSTITUTIVE THEORY
The isochoric strain tensor is also in principal form
||Giα|| =
λ1 0 00 λ2 00 0 λ3
. (2.59)
The corresponding isochoric principal strains λ2 = λ3 perpendicular to the ex-tensional direction follow from (2.7)2 as
λ2 = λ3 =
√1
λ1. (2.60)
The relationship between the deformation measures in (2.56) and (2.59) followsfrom (2.7)1 as
λ1 = (v
vR)− 13Λ1 , λ2 = (
v
vR)1/6 1√
Λ1
. (2.61)
The left Cauchy-Green deformation tensor (2.12) has then the representation
||βij|| =
λ21 0 00 1
λ10
0 0 1λ1
. (2.62)
The main invariants (2.14) are consequently
I1 = λ21 +2
λ1, I2 = 2λ1 +
1
λ21. (2.63)
The components of the Cauchy-stress follow from (2.39):
t11 = −p+ 4
3(λ21 −
1
λ1)(C1 + C2
1
λ1) ,
t22 = −p− 2
3(λ21 −
1
λ1)(C1 + C2
1
λ1) = t33 . (2.64)
From the boundary condition (2.55) we obtain the internal pressure
p = P − 2
3(λ21 −
1
λ1)(C1 + C2
1
λ1) . (2.65)
The 11-component of the 1st Kirchhoff-Piola-stress (2.53) is then given by
T11 = t1j(F−1)1j detF = t11
1
Λ1
Λ1Λ22 = t11
v
vR
1
Λ1
(2.66)
= (v
vR)2/3
t111
λ1= (
v
vR)2/3 1
λ1
[
−p+ 4
3(λ21 −
1
λ1)(C1 + C2
1
λ1)
]
.
2.2. UNIAXIAL EXTENSION 19
Thus, from (2.54), with the help of (2.65), one deduces for the nominal extensionalstress
σ1 = (v
vR)2/3
(λ1 −1
λ21) (2C1 + 2C2
1
λ1) . (2.67)
In the uniaxial extension experiment the independently given variables, andtherefore measurable quantities, are the external pressure P , the temperature Tand the length ratio Λ1. It is therefore necessary for the experimental testing,to introduce P, T,Λ1 (besides ξ) as independent variables. Any state functionψ(p, T, ξ, Iα) is thus representable as
ψ(p, T, ξ, Iα) = ψ(P, T, ξ,Λ1) , (2.68)
where the dependence on the set of variables on the right-hand side is denotedby a ˜ above the function symbol. The specific volume is then given by
v = v(P, T, ξ,Λ1) . (2.69)
For the deformation invariants (2.63), (2.61) implies
I1 = I1(P, T, ξ,Λ1) = (v
vR)−2/3
(Λ21 +
2
Λ1
v
vR) , (2.70)
I2 = I2(P, T, ξ,Λ1) = (v
vR)−1/3
(2Λ1 +1
Λ21
v
vR) ,
and for the internal pressure (2.65) and the nominal extensional stress (2.66) weget the expressions
p = p(P, T, ξ,Λ1)
= P − 1
3
1
vR(v
vR)−2/3
(
Λ1 −1
Λ21
v
vR
)[
2(vC1) + 2(vC2)1
Λ1
(v
vR)1/3]
, (2.71)
σ1 = σ1(P, T, ξ,Λ1)
=1
vR(v
vR)−2/3
(
Λ1 −1
Λ21
v
vR
)[
2(vC1) + 2(vC2)1
Λ1
(v
vR)1/3]
. (2.72)
The crystallinity ξ in non-equilibrium is, contrary to P, T,Λ1, not directlymeasurable in uniaxial, isothermal and isochoric extension tests. The volumerelaxation and the stress relaxation are measurable, because at fixed values ofP, T, and Λ1 the specific volume v as well as the nominal stress σ1 are measurableas functions of time. In the relations
˙v|P,T,Λ1 =∂v
∂ξξ|P,T,Λ1 , ˙σ1|P,T,Λ1 =
∂σ1∂ξ
ξ|P,T,Λ1 (2.73)
20 CHAPTER 2. THERMODYNAMIC CONSTITUTIVE THEORY
the left-hand sides are known and, consequently, also the ratio
˙σ1|P,T,Λ1˙v|P,T,Λ1
=∂σ1/∂ξ
∂v/∂ξ=∂σ1∂v|P,T,Λ1
. (2.74)
If one knows in addition the time rate of change of ξ, ∂v/∂ξ and ∂σ1/∂ξ areindirectly determinable from (2.73). To calculate ξ approximately, we employ thefollowing reasoning: For small departures of crystallinity ξ from its equilibriumvalue ξ(P, T,Λ1), the chemical production rate density A is proportional to the”affinity” ∧ξ. Then one has
A = a|E∧ξ . (2.75)
According to (2.52) a|E≥ 0. If one develops ∧ξ in a Taylor series for fixed values
of T, P,Λ1 with respect to ξ about the equilibrium value ξ, one obtains, on using(2.41), (2.42) and (2.50),
∧ξ = ∧ξ|E+
(
∂∧ξ∂ξ
+∂∧ξ∂p
∂p
∂ξ+∑
α
∂∧ξ∂Iα
∂Iα∂ξ
)
|E(ξ − ξ) (2.76)
= − 1
T
[
∂2g
∂ξ2+∂v
∂ξ
∂p
∂ξ+∑
α
∂(vCα)
∂ξ
∂Iα∂ξ
]
|E(ξ − ξ) .
In equilibrium the free enthalpy assumes at fixed values of T, p = p|E, Iα = Iα|E an
extremum. If we assume that this extremum is a minimum, then ∂2g/∂ξ2|E> 0,
and the crystallization equilibrium is stable. Then, the content of the squarebrackets can in (2.76) be positive.
We insert now (2.75) and (2.76) into the balance equation (2.1)5 and obtainwith ψj = 0
ξ = −1
τ(ξ − ξ) (2.77)
for the time rate of change of the crystallinity. τ = τ(p, T, ξ, Iα) = τ(p, T,Λ1) hasthe meaning of a relaxation time and is given by
1
τ:=
a|E
T
[
∂2g
∂ξ2+∂v
∂ξ
∂p
∂ξ+∑
α
∂(vCα)
∂ξ
∂Iα∂ξ
]
|E
. (2.78)
For some uniaxial deformation history λ1(t) at constant temperature T andconstant external pressure P , ξ = ξ(t) and τ = τ(t) are functions of time. Inte-gration of (2.77) yields then for the non-equilibrium crystallinity ξ (the internalvariable)
ξ(t) = ξ(0) e−∫ t0
dt′
τ(t′) + e−∫ t0
dxτ(x)
∫ t
0
dt′[ξ(t′)
τ(t′)e∫ t′
0dt′′
τ(t′′)
]
, (2.79)
2.2. UNIAXIAL EXTENSION 21
where ξ(0) is the equilibrium crystallinity at the beginning of deformation. ξ(t) isan after effect functional of stress history. This is the reason for volume and stressrelaxation and stress-strain hysteresis. Conclusions from (2.79) will be drawn inthe sequel.
In uniaxial extension experiments λ1(t) is prescribed at given values of thetemperature T and the external pressure P . So, the independent variables areT, P, λ1 and ξ. We need all equations in this set of variables. The derivatives ofthe function ψ with respect to T, P, ξ, λ1 are, according to (2.68)-(2.72),
∂ψ
∂T=
∂ψ
∂T+∂ψ
∂p
∂p
∂T+∑
α
∂ψ
∂Iα
∂Iα∂T
,
∂ψ
∂P= +
∂ψ
∂p
∂p
∂P+∑
α
∂ψ
∂Iα
∂Iα∂P
, (2.80)
∂ψ
∂ξ=
∂ψ
∂ξ+∂ψ
∂p
∂p
∂ξ+∑
α
∂ψ
∂Iα
∂Iα∂ξ
,
∂ψ
∂λ1= +
∂ψ
∂p
∂p
∂λ1+∑
α
∂ψ
∂Iα
∂Iα∂λ1
.
Identifying ψ with the free enthalpy g we obtain, on using (2.41),
∂g
∂T= −s + v
∂p
∂T+∑
α
vCα∂Iα∂T
,
∂g
∂P= +v
∂p
∂P+∑
α
vCα∂Iα∂P
, (2.81)
∂g
∂ξ= −T ∧ξ + v
∂p
∂ξ+∑
α
vCα∂Iα∂ξ
,
∂g
∂λ1= +v
∂p
∂λ1+∑
α
vCα∂Iα∂λ1
.
With u = g − pv + T s the derivatives of the internal energy are directly
22 CHAPTER 2. THERMODYNAMIC CONSTITUTIVE THEORY
obtained from (2.81),
∂u
∂T= T
∂s
∂T− p
∂v
∂T+∑
α
vCα∂Iα∂T
,
∂u
∂P= T
∂s
∂P− p
∂v
∂P+∑
α
vCα∂Iα∂P
, (2.82)
∂u
∂ξ= T
∂s
∂ξ− p
∂v
∂ξ+∑
α
vCα∂Iα∂ξ
− T ∧ξ ,
∂u
∂Λ1
= T∂s
∂λ1− p
∂v
∂λ1+∑
α
vCα∂Iα∂λ1
.
Finally, the derivatives of the free energy f := g + pv = u− T s are
∂f
∂T= −s − p
∂v
∂T+∑
α
vCα∂Iα∂T
,
∂f
∂P= −p ∂v
∂P+∑
α
vCα∂Iα∂P
, (2.83)
∂f
∂ξ= −T ∧ξ − p
∂v
∂ξ+∑
α
vCα∂Iα∂ξ
,
∂f
∂λ1= −p ∂v
∂λ1+∑
α
vCα∂Iα∂λ1
.
2.2.1 Approximations
All relations given so far are generally valid. They are correspondingly com-plicated. Especially, the choice of the pressure as an independent state variable,seems to make the formulas complicated. However, they are in this form espe-cially well suited for approximations. This will be demonstrated now.
2.2.1.1 Incompressible, thermoelastic materials
In the older theories of rubber-elasticity, Kuhn [41] , Mooney [52], Rivlin [55],it is assumed, that rubber is an incompressible thermoelastic material, whoseelasticity is solely traced back to the deformation dependence of the entropy.This theory is included as a special case of ours, if we assume that no statequantity depends on crystallinity, that the internal energy is independent of de-formation and that the specific volume is independent of temperature, pressureand deformation, namely
s = s(T, p, Iα) , u = u(T, p) , v = vR = const . (2.84)
2.2. UNIAXIAL EXTENSION 23
From the consequence of equations (2.84) and (2.42)7, the stress coefficients areindependent of pressure, and they are linear homogeneous functions of the (ab-solute) temperature
Cα(T, Iβ) = T Kα(Iβ) ,∂K1
∂I2=∂K2
∂I1. (2.85)
The specific heat capacity depends only on temperature,
cp = cp(T ) ,∂cp∂p
= 0 ,∂cp∂Iα
= 0 , (2.86)
the entropy is independent of pressure
∂S
∂T=cpT,∂S
∂p= 0,
∂S
∂Iα= −vR
∂Cα
∂T
and given by
s(T, Iα) = sR +
∫ T
TR
cp(T′)
T ′dT ′ − vR
∂
∂T
[
T
(∫ I1
3
K1(I′1, 3)dI
′1
+
∫ I2
3
K2(I1, I′2)dI
′2
)]
, (2.87)
and the internal energy is only a function of temperature
u(T ) = uR +
∫ T
TR
cp(T′) dT ′ . (2.88)
For uni-axial extension, from (2.61) λ1 = Λ1 and from (2.70), we obtain
I1 = I1(Λ1) = Λ21 +
2
Λ1
, I2 = I2(Λ1) = 2Λ1 +1
Λ21
. (2.89)
With this the stress coefficients (2.85) take the form
Cα(T,Λ1) = TKα(Λ1) , (2.90)
and the entropy and internal energy are
s(T,Λ1) = sR +
∫ T
TR
cp(T′)
T ′dT ′ − vR
∂
∂T
[
2T
∫ Λ1
1
⟨
K1(Λ′1) +
1
Λ′1K2(Λ
′1)
⟩
×(
Λ′1 −1
Λ′21
)
dΛ′1
]
(2.91)
u(T ) = uR +
∫ T
TR
cp(T′) dT ′ .
24 CHAPTER 2. THERMODYNAMIC CONSTITUTIVE THEORY
Finally, according to (2.67), for nominal extension the stress σ1 follows as
σ1 = 2T
(
Λ1 −1
Λ21
)(
K1 +1
Λ1
K2
)
= − 1
vRT∂s
∂Λ1
. (2.92)
This relationship shows that the nominal tension stress is given by the defor-mation derivative of the entropy. This behaviour is called Entropy Elasticity ofrubber. This implies two effects which are typical for rubber:
1. If one increases the temperature at constant stress σ1 and constant externalpressure P , the rubber sample shrinks (Gough-effect )[28].
2. If one extends a rubber sample under adiabatic isolation (e.g. at constantentropy s), and constant external pressure, the temperature is increased (Joule-Effect [34])2.
From (2.92) follows additionally, that the stress at constant deformation andconstant external pressure is a linear homogeneous function of temperature,
σ1 − T∂σ1∂T
= 0 . (2.93)
This means graphically, that the stress-temperature curves at constant extensionare straight lines which for extrapolation to T → 0 approach the origin σ1 =0, and whose inclination increases with increasing deformation as explained byequation (2.92) and shown in figure 2.1.
0 TRT
1~σ
1Λ
Figure 2.1: Stress-temperature curve of uniaxial extension.
In the statistical theories of rubber elasticity, first treated by Kuhn [42], it isassumed that the molecular chain between two crosslinking points can be divided
2For materials, which are essentially energy-elastic (e.g. metals) both effects are exactlyreversed.
2.2. UNIAXIAL EXTENSION 25
into (statistically equivalent) segments, which are connected to each other by freerotations. For this model the conformational entropy is calculated for small andmedium deformations (strong coiling : distance crosslinking point
Maximum length of stretched chain<< 1) in the
so called Gaussian approximation, under the assumptions that crosslinking pointsmove affinely to the macroscopic deformation and that the model substance isincompressible. From this model, there result constant stress coefficients,
vRK1 =k
2Nmo
, K2 = 0 . (2.94)
Here, k is Boltzmann’s constant, N is the number of segments between twocrosslinking points, and mo is the mass of one segment. The observed stress-strain curves can be described with this for small deformations. Especially, theeffect is well described, that weakly cross-linked rubber can be deformed moreeasily than strongly cross-linked rubber.
For medium and large deformations the stress-strain behaviour is not correctlydescribed by (2.94). The reason is, besides others, that the Gaussian approxi-mation is employed for calculating the conformational entropy, even though forlarge deformations the strong coiling of the chain molecule is no longer valid. Ifone weakens this Gaussian assumption, then the conformational entropy can becalculated only approximately using a complicated Taylor series expansion in Λ1,see Treloar [70]. With this one may derive by differentiation according to (2.92) aseries expansion for the stress, which contains just one fitting parameter, k
Nmo
1vR.
In a continuum theory one has, in contrast to the statistical theory, two stresscoefficients. Mooney [52] assumed that K1 and K2 are constants for uniaxialextension tests. With this, the measurements can be explained up to intermediatedeformations. However, the steep upturn of the stress for large deformationscannot be described with constant values of stress coefficients.
Rivlin and Saunders [56] were able to describe also the steep upturn. Theyassume, that K1 is constant and K2 depends on the deformation. According to(2.85), K2 can then depend only on the second deformation invariant,
K1 = const , K2 = K2(I2) . (2.95)
With this, Rivlin and Saunders can also explain quite well bi-axial stress-strain experiments, however they report, that K2 seems to depend weekly ontime in such a way that K2, in the course of time, decreases at constant load.This time dependence cannot be understood with any theory of thermo-elasticity.
26 CHAPTER 2. THERMODYNAMIC CONSTITUTIVE THEORY
2.2.1.2 Incompressible, thermoelastic materials with thermal volume
expansion
Mayer and Ferri [51] and Anthony, Casten and Guth [9] report, that thestress-temperature curve can be reproduced only, if as a deformation measurethe thermal convective length ratio
λ1 =L(T )
Lo(T )=
Length under load at temperature T
Length without load at temperature T
is used as a curve parameter. If, however, the deformation measure Λ1 = L(T )LR
is used, the measured curves for T → 0 do not merge into the point σ1 = 0.This observation is called thermo-elastic inversion. The relationship between the
deformation measures λ1 and Λ1 is λ1 = L(T )LR
LR
Lo(T )= Λ1
(vvR
)−1/3according to
(2.61)1. From this must be concluded, that for the description of the thermoe-lastic inversion the thermal convective deformation measure must be used.
The measurements show, that the nominal stress σ1 in uni-axial extension atconstant external pressure P and fixed thermal convective length ratio λ1 is ahomogeneous linear function of absolute temperature, i.e.,
σ1 − T
(∂σ1∂T
)
λ1,P
= 0 , (2.96)
For the stress coefficients, after insertion of (2.67), one obtains
Cα(T, λ1) =
(v(T )
vR
)−2/3TKα(λ1) . (2.97)
The stress coefficients are, consequently, not exactly linear in T (as in the ap-
proximation (2.85)), but they contain the volume factor(v(T )vR
)−2/3.
2.2.1.3 Continuum theory and Deformation-Induced Crystallization
For simplification of the theory, some approximations have been assumedabout the specific volume v = v(T, p, ξ, Iα). We make now the following linear(Taylor) series expansion of the specific volume about the reference state:
v = vR [1 + αo(T − TR) + βo(p− pR) + γo(ξ − ξR) + δo(I1 − 3) + εo(I2 − 3)] .(2.98)
For small departures of T, p, ξ, I1, I2 from the reference state values such an ex-pansion should be valid.
2.2. UNIAXIAL EXTENSION 27
The coefficients in this expansion are, in the reference state,
αo =1
vR
(∂v
∂T
)
pR,ξR
= 6.6× 10−41
K,
βo =1
vR
(∂v
∂p
)
TR,ξR
= −5.1× 10−51
bar,
γo =1
vR
(∂v
∂ξ
)
TR,pR
, (2.99)
δo =1vR
(∂v∂I1
)
TR,pR,ξR,
εo =1vR
(∂v∂I2
)
TR,pR,ξR,
where αo is the classical coefficient of thermal volume expansion, βo the isothermalcompressibility, γo the coefficient of volume expansion due to crystallization, δoand εo are volume expansion coefficients due to the deformation. The ordersof magnitude of γo, δo, εo are unknown. Specialization to uniaxial extension atT = TR and P = pR yields, with (2.63) and (2.65),
v = vR
[
1 + γo(ξ − ξR)− βo2
3(λ21 −
1
λ1)(C1 +
1
λ1C2)
+ δo(λ21 +
2
λ1− 3) + εo(2λ1 +
1
λ21− 3)
]
. (2.100)
For simplification, the change of volume with deformation is assumed to be linear,
when ξ − ξR =(
∂ξ∂λ1
)
TR,pR,λ1=1(λ1 − 1) holds. For the equilibrium volume thus
follows
v = vR
[
1 + γo
(∂ξ
∂λ1
)
TR,pR
(λ1 − 1)− βo2
3(λ21 −
1
λ1)(C1 +
1
λ1C2)
+ δo(λ21 +
2
λ1− 3) + εo(2λ1 +
1
λ21− 3)
]
. (2.101)
Cα = Cα(TR, pR, ξ, λ1) (α = 1, 2) denote the values of the stress coefficients incrystallization equilibrium. For deformation up to 100% the Mooney approxi-mation is valid. Then the stress-coefficients in equilibrium are independent ofdeformation and pressure, and functions of temperature alone, Cα = Cα(TR). Inthis case, ∆v
vR= v−vR
vRis a linear function of λ1 − 1, only if βo = δo = εo = 0. This
explains the experimental findings of Goritz [31].
The linear increase of volume up to deformations of about 100% can be ex-plained only, if the compressibility and the dependence of the volume from thedeformation invariants are neglected. Then,
v = v(T, ξ) . (2.102)
28 CHAPTER 2. THERMODYNAMIC CONSTITUTIVE THEORY
This explains the linear increase of the specific equilibrium volume for smalldeformation ratios.
With the approximation (2.102) the formulas (2.42) to (2.45) simplify as fol-lows:
∂Cα
∂p= 0 ,
∂C1
∂I2=∂C2
∂I1,
∂∧ξ∂p
= − 1
T
∂v
∂ξ,
∂∧ξ∂Iα
= − 1
T
∂(vCα)
∂ξ, (2.103)
∂cp∂p
= − 1
T
∂2v
∂T 2,∂cp∂ξ
= − ∂
∂T
(
T 2∂∧ξ∂T
)
,∂cp∂Iα
= −T ∂2(vCα)
∂T 2,
∂s
∂T=
cpT
,∂s
∂p= − ∂v
∂T,∂s
∂ξ=
∂
∂T(T∧ξ), ∂s
∂Iα= −∂(vCα)
∂T,
∂u
∂T= cp − p
∂v
∂T,
∂u
∂p= −T ∂v
∂T,
∂u
∂ξ= T 2∂∧ξ
∂T− p
∂v
∂ξ,
∂u
∂Iα= vCα − T
∂(vCα)
∂T.
The stress coefficients are consequently independent of the pressure.
These relations shall now be integrated, starting in the reference state T =TR, p = pR, ξ = ξR, Iα = 3 (α = 1, 2). From (2.103)3,4
∧ξ(T, p, ξ, Iα) = ∧ξ(T, ξ)− 1
T
∂v(T, ξ)
∂ξ(p− pR)
− 1
T
∂
∂ξ
[
v(T, ξ)
∫ I1
3
C1(T, ξ, I′1, 3) dI
′1
]
(2.104)
− 1
T
∂
∂ξ
[
v(T, ξ)
∫ I2
3
C2(T, ξ, I1, I′2) dI
′2
]
.
The integration function ∧ξ must be interpreted as ∧ξ(T, pR, ξ, 3, 3). The equilib-rium values ∧ξ|
E= ∧ξ(T, p, ξ, Iα) = 0 are zero according to (2.50). This implies,
since the reference state has been chosen as an equilibrium state, that
∧ξ|R= ∧ξ(TR, pR) = 0 (2.105)
Moreover, with ∧ξ|E= ∧ξ(T, p, ξ, Iα) = 0, (2.104) is an equation for the determi-
nation of the equilibrium values ξ|E= ξ(T, p, Iα) of the degree of crystallization
outside the reference state.
Next we integrate formulas (2.103)5−7 for the specific heat capacity. Use of
2.2. UNIAXIAL EXTENSION 29
(2.104) yields
cp(T, p, ξ, Iα) = cp(T )− T∂2v(T, ξ)
∂T 2(p− pR)
+∂
∂T
[
T 2 ∂
∂T
∫ ξ
ξR
∧ξ(T, ξ′) dξ′]
(2.106)
−T ∂2
∂T 2
[
v(T, ξ)
∫ I1
3
C1(T, ξ, I′1, 3) dI
′1
]
−T ∂2
∂T 2
[
v(T, ξ)
∫ I2
3
C2(T, ξ, I1, I′2) dI
′2
]
.
Here cp(T ) denotes the specific heat capacity at p = pR, ξ = ξR, I1 = I2 = 3.
With this result, using (2.104), we now integrate formulas (2.103)8−11 and(2.103)12−15 for the specific entropy and the specific internal energy. After somecalculation the following formulas are obtained:
s(T, p, ξ, Iα) = sR +
∫ T
TR
cp(T′)
T ′T ′ − ∂v(T, ξ)
∂T(p− pR)
+∂
∂T
[
T
∫ ξ
ξR
∧ξ(T, ξ′) dξ′]
(2.107)
−T ∂
∂T
[
v(T, ξ)
∫ I1
3
C1(T, ξ, I′1, 3) dI
′1
]
−T ∂
∂T
[
v(T, ξ)
∫ I2
3
C2(T, ξ, I1, I′2) dI
′2
]
,
u(T, p, ξ, Iα) = uR +
∫ T
TR
cp dT′ − pR[v(T, ξ)− vR]
−T ∂v(T, ξ)∂T
(p− pR) + T 2 ∂
∂T
∫ ξ
ξR
∧ξ(T, ξ′) dξ′
+
[
v(T, ξ)
∫ I1
3
C1(T, ξ, I′1, 3) dI
′I
]
(2.108)
+
[
v(T, ξ)
∫ I2
3
C2(T, ξ, I1, I′2) dI
′2
]
−T ∂
∂T
[
v(T, ξ)
∫ I1
3
C1(T, ξ, I′1, 3) dI
′1
]
−T ∂
∂T
[
v(T, ξ)
∫ I2
3
C2(T, ξ, I1, I′2) dI
′2
]
.
30 CHAPTER 2. THERMODYNAMIC CONSTITUTIVE THEORY
sR and uR, respectively, denote the specific entropy and specific internal energyin the reference state.
The problem of deformation induced crystallization and the description of therelated time effects (stress relaxation, hysteresis , reversible thermoplasticity, timedelayed heat effects) would be solved, if cp(T ), v(T, ξ), ∧ξ(T, ξ), Cα(T, ξ, I1, I2)would be known as functions of the given variables, and if the crystallizationrate A(T, p, ξ, Iα) would be determined as a function of the given variables. Thesolution of the differential equation (2.1)5 with ψj = 0 would determine ξ(t) atfixed external pressure as a result of integration over the histories of deformationand temperature. Insertion of the result of integration (2.79) for ξ(t) in (2.39),(2.107) and (2.108) will give the Cauchy stress tij, the internal energy u and theentropy s as integrals over the histories of deformation and temperature.
However, the solution of this problem requires, first the determination of theexplicit dependence of all involved functions upon their variables.
According to (2.63),(2.67), (2.102), (2.107) and (2.108) the formula for thenominal stress is
σ1 = 2
(v(T, ξ)
vR
)2/3
(λ1 −1
λ21)
[
C1(T, ξ, Iα(λ1)) +1
λ1C2(T, ξ, Iα(λ1))
]
(2.109)
Based on (2.95) we assume in addition with Rivlin and Saunders [56] that the firststress coefficient is independent of Iα. Then, according to (2.103)2, the secondstress coefficient is independent of I1:
C1 = C1(T, ξ) , C2 = C2(T, ξ, I2) . (2.110)
For qualitative understanding of stress-strain curves, one needs first the depen-dences of the stress coefficients Cα on the degree of crystallinity ξ. This will insequel be derived within the framework of the statistical theory.
Chapter 3
Polymer Crystallization
Crystallization of polymers has been the focus of attention in the past fourdecades. It plays an important role in polymer applications, primarily in manymanufacturing processes such as fiber spinning, extrusion drawing, film blowing,blow molding, and injection molding.
The mechanical behaviour of polymers is strongly depending on their mor-phology, which in turn is influenced by the thermo-mechanical history duringprocessing. Molecular orientation affects the crystallization behaviour of poly-mers in two different aspects: thermodynamic and hydrodynamic. The thermo-dynamic effect involves the reduction of entropy in extended chains and this willincrease the opportunity of crystal formation by increasing the melting point,while kinetically the extended chain is closer to a crystal state than a randomchain. The hydrodynamic effect is a phase transformation, which is responsiblefor the resultant morphology such as shish, kebab or spherulite. Several on-goingprojects are designed to explore the underlying physics of this subject.
Mechanically, deformation induced crystallization in rubbery polymers pro-duces internal inhomogeneity in their structure and leads to a significant redistri-bution of stresses, since the orientation of the crystals has a beneficial impact onthe mechanical properties of the rubbery polymers. Crystallization of rubberlikepolymer networks exhibits clear upturns in the stress-strain curve at high elon-gation. This is mainly due to the reinforcing effect of the crystallites that aregenerated.
3.1 Semi-Crystalline Polymers
Depending on the processing conditions, polymer-crystallization behaviouris attributed to the long chain length of the polymeric molecules, which makes
31
32 CHAPTER 3. POLYMER CRYSTALLIZATION
it difficult for these chains to disentangle from each other in disorganized andentangled melt and subsequently to achieve a regular conformation and alignparallel to each other to form an ordered structure (i.e. crystal). Therefore,whether polymers are able to crystallize or not depends on their structure.
3.2 Models of Semi-Crystalline Polymers
The most obvious question that needs to be answered about polymer crys-tallites is ‘How can long molecules give rise to small crystallites? ’. Two princi-pal types of answer have been given: they lead to the fringed-micelle and thechain-folded model for polymer crystallites. A further type of crystallites is thechain-extended crystallite which will be discussed in detail.
3.2.1 Fringed-micelle model
The fringed-micelle model was an early attempt to inter-relate long molecules,small crystals and a ‘sea’ of amorphous material [22]. The crystalline regions aremade up of different chains of short lengths aligned parallel to each other, whilethe amorphous regions are comprised of disordered conformations.
The model suggests the occurrence of fibrillar crystallites, which can growboth parallel and perpendicular to the chain axes. The long chain character ofpolymer allows a given chain to pass through several different crystallites [49, 48,47] as shown in figure 3.1a. This model explains the mechanical properties of thesample based on the physical linkages (fringes) between two regions.
(a) (b)
Figure 3.1: Two different semi-crystalline structures: (a) Fringed-micelle struc-ture (b) Spherulite structure.
3.2. MODELS OF SEMI-CRYSTALLINE POLYMERS 33
3.2.2 Folded-chain model
It was reported by Keller [37, 38] that polyethylene single crystals, grown froma dilute solution, appear in the form of thin plates or Lamellae when viewed byelectron diffraction to be composed of large crystallites with the chain axes normalto the plane of the lamellae. The only possibility to explain this was that chainsfolded back and forth upon themselves, so that adjacent segments were paralleland in crystal registers.
The adjacent re-entry model of Keller was challenged by Flory [24]. In anearly theoretical treatment, Flory [24] examined some of the factors related tothe generation of a crystalline phase from long chain molecules in random confor-mations. He established that ”no more than half of the chains emanating fromthe lamellar crystal surface can be accommodated by the neighbouring disorderedamorphous phase”. As a result, more than half of those sequences must returnto the crystal face from which they departed. This re-entry is proposed to occurvia loops of varying lengths that are present in the spaces between the crystaland the amorphous regions. There also exist a number of chains that do not re-enter a given crystallite, but leave the basal plane of the crystal to become partof a disordered amorphous region. These chains could eventually enter anotherneighbouring crystallite. Such a possibility of chain folding is often referred to asthe ”switchboard model”.
When crystallized from the melt, the lamellae often aggregate together inthe form of a superstructure called a spherulite. Spherulites may be viewed asspherical aggregates of lamellae that originate from a common center and radiateoutwards as shown in figure 3.1b. The spherical shape is formed as a result ofbranching and splaying of lamellae at dislocation points. Typical dimensions ofspherulites are of the order of microns and sometimes, even millimeters. There-fore, they can be easily viewed under an optical microscope. The spherulitescontinue to grow radially until they impinge upon one another. A measure oftheir growth rate until the time of impingement provides a wealth of informationregarding the mechanism of crystallization in the polymer, and has been the focusof several investigations.
3.2.3 Extended-chain crystallite
Extended, or fully extended, chain crystallites contain long oriented chainsthat can be formed mechanically. Crystallization induced by orientation can bedescribed as stretching of long chains to form fibrous crystals. During stretching,distortion of chains from their most probable conformations results and hence adecrease in the conformational entropy takes place. If this deformation is main-tained in this lower conformational entropy state then less conformational entropyneeds to be sacrificed by transforming to a crystalline state. This decrease in to-
34 CHAPTER 3. POLYMER CRYSTALLIZATION
tal entropy of fusion allows the crystallization to occur at higher temperaturesthan will take place under quiescent conditions.
Natural and synthetic rubbers are excellent examples of such an effect asthey show great tendency to crystallize under stretched conditions, whereas theycrystallize slowly under quiescent conditions. Also, crystallization in an alreadyoriented polymer results in a reduction of retractive force (with respect to theoriented state). This can be explained on the basis of rubber-elasticity theoryaccording to which the force exerted by fixed chain ends is inversely proportionalto the number of statistical segments and the magnitude of end to end distance.The reduction in force results because of a lesser number of statistical segmentssitting in the amorphous domain and also because the end to end distance ofthe amorphous segments is smaller than that in the crystal. Melting of suchextended crystals leads to contraction, and crystallization leads to elongation.That is why the deformation is considered to be of affine type, since macroscopicdimensional changes and changes in retractive force can be related to the crystalphase transformation.
The formation of the so-called ’Shish-Kebab’ kind of morphology consists ofthe outside ’kebab-like’ regions which are essentially folded chain regions com-prised of chains which do not crystallize during the orientation process, whilethe inner ’shish’ regions form first. The formation of folded chain discs occursdue to nucleation events taking place on the extended chain surface. This hasbeen used as a strong argument in favor of kinetic theories that discuss the chainfolded model of crystallization. Keller and Machin [39] showed essentially a per-pendicularly oriented shish-kebab type lamellar morphology, they proposed a twostep nucleation and growth for crystallization under orientation. The nucleationprocess is thought to be associated with the formation of extended chain shishfrom oriented molecules and the growth process is associated with the formationof lamellar crystals from an isotropic melt by chain folding onto the line nuclei.Alternatively, Yeh [45] revealed the presence of a nodular structure (∼ 100A)within perpendicularly oriented “lamellae”. Indeed, Gent [26, 27] had concludedthat the form and the magnitude of the stress changes during the crystallizationof stretched networks are generally the same for different types of rubber. Thus,based on axial stress-relaxation evidence, Gent ruled out the possibility of chainfolding during oriented crystallization.
Thermodynamically, if the coiled chains in a polymer melt are stretched,their entropy approaches that of the crystalline state. The difference between theentropies of the oriented and crystalline states decreases and thus, as indicatedby equation (3.1), the melting point is raised. If the melting point is raised abovethe environment, stress crystallization takes place [72].
T ◦m = ∆H◦/∆S◦ , (3.1)
3.2. MODELS OF SEMI-CRYSTALLINE POLYMERS 35
where ∆H◦ and ∆S◦ are the enthalpy and the entropy of melting, respectively,defined as the changes in state for the conversion of 1 Mole from the crystal tothe melt phase.
The following relationship was derived by Flory [21] for the dependence of themelting point on strain for a crosslinked elastomer:
1/Tm − 1/T ◦m = −(R/∆H◦) g(λ) , (3.2)
where the function g(λ) - not the free enthalpy - depends on the type of appliedchain statistics. According to Flory [21, 72]:
g(λ) = (6/πN)1/2λ− (λ2/2 + 1/λ)/N (3.3)
where N is the number of statistical chain segments per network chain, and λ isthe deformation ratio.
The foregoing brief survey of semi-crystalline polymers, with its emphasis onthe importance of the types of crystalline chains would not be complete without abrief mention of amorphous polymer chains. The amorphous polymer chains arethose with a randomly coiled and entangled state. They possess a large specificvolume va compared with the crystalline volume vc domain at room temperature.Thus, the total volume of a piece of rubber is given by
V = mava +mcvc , (3.4)
where ma is the amorphous mass and mc is the crystalline mass. The total massis consequently
m = ma +mc , (3.5)
Accordingly, the specific volume of the rubber is given by the equation
v = (1− ξ)va + ξvc , (3.6)
where ξ denotes the degree of crystallinity,
ξ =mc
m=
Number of chain segment in crystallites
Total number of chains segments. (3.7)
Goritz [30] performed some experiments for cis-1,4-Polybutadiene rubber andreported a relationship between volume change and strain up to large extension;on the basis of an affine deformation this dependence is proportional to λ − 1,where λ is the extension ratio. Furthermore, he studied the elongation-induced
36 CHAPTER 3. POLYMER CRYSTALLIZATION
crystallization and found that the final degree of crystallization depends on tem-perature and elongation. The dependence on elongation does not follow Flory’stheory of crystallization induced by stretching polymeric networks [21, 31].
Toki [68, 69] extensively studied the strain-induced crystallization phenomenonin sulfur vulcanized natural rubber by X-ray diffraction techniques. The detectedstructures were not only in a stretched but also in a relaxed state to accommodatethe relatively weak X-ray intensity.
Figure 3.2: Structure change and selected Wide Angle X-ray Diffraction (WAXD)patterns during stretching and retraction process of rubber. Where λ is thedeformation ratio.
The crystallization curve and selected Wide Angle X-ray Diffraction (WAXD)patterns during stretching and retraction are shown in figure 3.2 1. It is seen thathighly oriented crystalline reflection peaks begin to appear at strains aroundλ = 2.0 at which orientation of the chain segments occurs. The intensity ofthese reflections increases with strain during stretching, and darker spots are no-ticed to form at the maximum stretching deformation ratio (λ = 5.0), while anamorphous halo is found to persist in WAXD during both processes of stretchingand retraction (even at the highest applied strain). When the mechanical draw-ing ceases and the retraction process occurs, secondary crystallites develop, andstress relaxation is a direct consequence of folded lamella formation at the surface
1The WAXD patterns appearing in this figure have been taken from the work of S.Toki[68,69].
3.3. CRYSTALLIZATION KINETICS 37
of extended-chain crystals. However, we believe that some of the strain-inducedcrystallites might transform their morphology to secondary crystallites that donot contribute to the stress. This is obvious since the reflection intensities willdecrease if they are compared at the same deformation ratio for retraction andstretching processes. While the retraction unloading process is proceeding thecrystallinity and the orientation are larger than during stretching at a certaindeformation ratio. This can be noticed at all deformation ratios (e.g. λ = 2.0),see figure 3.2. This also is shown by WAXD pattern in figure 3.2 during re-traction. For example, at the strain of 1.0, no crystalline pattern is observedduring stretching but clear crystalline reflections are seen during retraction. Thisis a great evidence for shish-kebab formation during retraction due to stress re-laxation which is responsible for having a hysteresis in the stress-strain curve.When that the strain-induced crystallites are totally molten at elevated temper-ature and no further folded crystallite types exist, then the crystallization curvecoincides during the stretching and retraction processes.
Based on this, crystallites formed by deformation may be composed of twotypes:
Type 1. The important portion of the crystallites are the extended-chaincrystallites that develop by the strain directly during stretching (loading process).These serve as nuclei for further crystallization.
Type 2. The secondary crystallite types are the folded-chain crystallites(lamellae, Shish-kebab structure). These develop during retraction on nuclei ofextended type and may decrease or increase with retraction depending on theprocess conditions. Without a further increase in strain, this type of crystalliteis able to form at low temperature.
3.3 Crystallization Kinetics
Our present concern is to simulate crystallization kinetics induced by defor-mation and taking place at different strain rates and temperatures. The simplestapplicable differential equation for this process, according to irreversible thermo-dynamics, is the following first order equation
ξ =−1τ
(ξ − ξ) , (3.8)
where τ = τ(T, λ, ξ) is the relaxation time and ξ = ξ(T, λ) is the equilibriumcrystallinity. For this we assume saturation behaviour:
ξ = ξ◦ + (ξs − ξ◦) tanh(λ− 1) , (3.9)
38 CHAPTER 3. POLYMER CRYSTALLIZATION
where ξ◦ is the equilibrium crystallinity at the reference state, ξs is the equilibriummaximum (saturation) degree of crystallinity, and λ is the extension ratio definedas the ratio of the final to the initial length for uniaxial extension.
ξ◦ and ξs are temperature dependent and given by the relations
ξ◦ =Tmo − ToTmo − T
ξ◦ , (3.10)
ξs =Tmo − ToTmo − T
ξs , (3.11)
where Tmo , To , T are the melting (absolute) temperature, the reference tem-perature, and the temperature, respectively, ξ◦ is the degree of crystallinity atthe reference state, while ξs is the maximum (saturation) degree of crystallinityat reference temperature.
After carrying out the integration and appropriate rearrangement of equation(3.8), we obtain
ξ(t) = ξ(0) e−∫ t0
dt′
τ(t′) + e−∫ t0
dxτ(x)
∫ t
0
[ξ(t′)
τ(t′)e∫ t′
01
τ(t′′)dt′′]
dt′ (3.12)
This equation implies two limiting cases that explain the content of the compli-cated relaxation behaviour and its effect on crystallization kinetics:
(A) In the limit of low temperatures, the relaxation time τ −→ ∞ which isindependent of strain rate. Then the crystallinity does not change with deforma-tion: ξ(t) = ξ(0).
(B) In the limit of high temperatures, the relaxation time τ −→ 0 which isindependent of strain rate. Then, the crystallinity will be momentarily at anequilibrium state.
Between these two extreme cases there exists a time delay for the equilibriumapproach which also is the reason for stress- and volume relaxations.
We consider now a loading process with constant loading speed ε
λ1(t)− 1 = εt , 0 ≤ t ≤ tf , (3.13)
where t is the loading time, and tf is the loading time required to reach themaximum deformation ratio. Furthermore, we assume that the relaxation timeτ is merely a function of temperature T namely
τ(T ) = aL exp[bL/(RT )] := τL , (3.14)
3.3. CRYSTALLIZATION KINETICS 39
where aL, bL are constants and R is the universal gas constant. From the dimen-sions of the parameters aL, bL, it can be concluded that bL is a jump energy permole for crystallization, and aL is an inverse jump frequency, and it is propor-tional to the jump probability of the chain segment for the transformation fromamorphous to crystalline state.
For an isothermal loading process one may then deduce from (3.12), togetherwith (3.9), (3.13) and (3.14),
ξ(t) = ξ(0) + (ξs − ξ◦)
[
tanh(εt)− e−tτL ετL
∫ tτL
0
ex
cosh2(ετLx)dx
]
, (3.15)
in 0 ≤ t ≤ tf .
The non-equilibrium crystallization at the end of the loading process is
ξ(tf ) = ξ(0) + (ξs − ξ◦)
[
tanh(εtf )− e−tfτL ετL
∫ tfτL
0
ex
cosh2(ετLx)dx
]
, (3.16)
where ξ(tf ) is the degree of crystallinity at the maximum deformation ratio forthe loading process and can be calculated directly from equation (3.15) for t = tf .
Next, we consider the corresponding isothermal unloading process with re-versed speed of deformation,
λ(t) = λf − ε(t− tf ) , tf ≤ t ≤ 2tf , (3.17)
where λf is the maximum deformation ratio at the end of loading. Using (3.12)we obtain for the non-equilibrium crystallization in unloading
ξ(t) = e−∫ ttf
dxτ(x)
{
ξ(tf ) +
∫ t
tf
[ξ(t′)
τ(t′)e∫ t′
tf
dt′′
τ(t′′)
]
dt′
}
, (3.18)
for tf ≤ t ≤ 2tf .
As mentioned before, in unloading, crystallite structures of shish-kebab-types areformed besides the extended crystallites of loading. This means, that the relax-ation time in unloading is different from that in loading.
We assume again a constant relaxation time τ for isothermal unloading butassume otherwise a temperature dependence as follows:
τ(T ) = au exp [bu/(RT )] := τu . (3.19)
40 CHAPTER 3. POLYMER CRYSTALLIZATION
Insertion into (3.18) yields then for the crystallinity during an unloading pro-cess2
ξ(t) = ξ(tf )e− t−tf
τu + ξo
(
1− e−t−tfτu
)
+ (ξs − ξo)
{
tanh[(λf − 1) (3.20)
−ε(t− tf )]− e−t−tfτu tanh(λf − 1)
+e−t−tfτu .ετu
∫ t−tfτu
0
ex
cosh2[(λf − 1)− ετux]dx
}
,
for tf ≤ t ≤ 2tf .
2The mathematical calculations of equations (3.15) and (3.20) are available upon request.
Chapter 4
Deformation-Induced
Crystallization: Statistical
Approach
4.1 Introduction
The rubber elasticity approach includes a great variety of descriptions, modelsand concepts. The research has started last century in the late thirties by Kuhn,Guth and H.F. Mark. It became a very active field in the forties and fifties withimportant contributions by Flory, James, Guth, Treloar, Wall and many otherresearchers, based mostly on the analysis of Gaussian chain models. The sixtiesand seventies were the times of the establishment of the basis for the statisticalmechanical treatment of polymers and elastomeric materials, with fundamentalworks by Flory and many other scientists. In the seventies the computer technol-ogy of polymers became very important and the role of these simulations rapidlyincreased in the eighties and the nineties.
The simple, elementary statistical theory which paved the way to the currentunderstanding of rubber elasticity was proposed in the pioneering work of Kuhn[41, 42]. Other important early contributions to the early rubber elasticity theorywere given by Flory [21]. Flory was the first to develop a thermodynamic theoryof strain induced crystallization which is considered to be the simplest and themost convenient among the multitude of the statistical theories. Starting fromthe simple model of Kuhn, Flory’s theory is based on many simplifying assump-tions. According to it, a rubber network consists of freely-joint Gaussian chains,of which the positions of crosslinking points deform affinely upon deformation.Each chain contains a certain number of statistically equivalent rigid and sim-ply connected segments with complete freedom of orientation. Flory, imposing
41
42 CHAPTER 4. STATISTICAL APPROACH
the assumption of constant volume, calculated the changes of the crystalline andamorphous entropies with deformation. So far, the following crucial points ofworthiness may be mentioned: (i) Flory’s theory is based on the assumptionthat, the change of entropy is unequal to zero in the undeformed state, in con-tradiction to his assumption since he performed his calculations starting fromthe totally crystalline network; (ii) the change of entropy in the deformed stateapproaches for complete crystallization a negative infinitely large value.
Flory’s theory is inadequate to describe real rubber, because of his assump-tions, that there is no crystallization in the undeformed state, and that completecrystallization is possible. Both assumptions are not consistent with reality.
In the present context, we correct the shortcomings of Flory’s theory. Wereturn to the picture of freely-joint chains crosslinked at junction points, of whichthe motions are affine to the macroscopic deformation. A modified Gaussiandistribution is employed for chains of finite lengths to describe the end-to-endvector distribution function and the contribution of that chain to crystallinity.
4.2 Overview of the Model
In our model, we start treating the amorphous chain. According to Kuhn[41, 42], we shall be concerned primarily with those statistical properties whichmay conveniently be dealt with in terms of an idealized chain of N numbers offreely rotating equivalent segments of length `. (A “chain” is defined as thatportion of the network extending from one crosslinking point to the next [21], asshown in figure 4.1).
Figure 4.1: Example of a long chain of freely rotating segments.
4.2. OVERVIEW OF THE MODEL 43
The statistical form of the long-chain molecule is illustrated by figure 4.2,in which the angle between successive segments (i.e. the valence angle) is fixedbut complete freedom of rotation of any given segment with respect to adjacentsegments in the chain is allowed. The actual chain conformation will be subjectto continual fluctuation due to thermal agitation which enhances these segmentsto shift at a rapid rate from one position to another, consistent with their at-tachments to neighbouring segments of the same chain and the availability of freespace in their immediate environment [21, 70].
Figure 4.2: Statistical schematic of a freely rotating segments around bonds.
Polymers can exist in various conformations and various configurations. Twopolymers which differ only by rotations about single bonds are said to be twoconformations of that polymer. A schematic view of two polymer conformationsis shown in figure 4.3. Two polymers which have the same chemical compositionbut can only be made identical (e.g. superposable) by breaking and reformingbonds are said to be two configurations of that polymer. No manner of rotationsabout single bonds can turn polymers in different configurational states intosuperposable polymers.
The above definitions of conformations and configurations are standard, butthey have not always been rigorously followed in the literature. For example,Flory used configuration in his writings when he meant conformation. Fortu-nately a writer’s meaning is usually obvious from the context.
There are different ways to characterize the size of a polymer chain. Thecontour length L is the total length of a stretched chain,
L = N` (4.1)
The contour length has a fixed value, no matter what the value of the chainconformation.
The so called freely joint chain (figure 4.1), or random walk model is employedto get the averages over all the possible chain conformations. In this model
44 CHAPTER 4. STATISTICAL APPROACH
(a) (b)
Figure 4.3: A schematic view of (a) polymer configuration and (b) polymer con-formation.
the angle of each segment is independent of every other, including the nearestneighbouring segments. To describe it, another measure of polymer chain size isneeded, the end-to-end vector. It is used when a chain is in a given conformationas shown in figure 4.4. The end-to-end length varies from one chain conformationto the next. The end-to-end vector r is the vector sum over the bonds `i for bondsi=1,2,3,...,N
rr
1α
Nα
5α
4α3α
2α
rer
rer
rer
rer
rer
rer
1lr
2lr 3l
r
4lr
5lr
Nlr
Figure 4.4: End-to-end chain length, with N segments: five segments are shownsomewhere in the chain, the remaining ones of which are represented by the dottedline till the N th segment. The angle αi is the angle between the ith segment andthe r axis.
r =N∑
i=1
`i . (4.2)
The end-to-end length can not be greater than the contour length. The end-to-end length changes when a polymer is subjected to applied forces.
4.2. OVERVIEW OF THE MODEL 45
The z -component of the end-to-end vector is
rz =N∑
i=1
zi, (4.3)
where zi = ` cosαi is the projection on the zi − axis of the ith vector and αi isthe angle of segment i relative to the zi − axis. If all the segment vectors havethe same length `, then
rz = `N∑
i=1
cosαi. (4.4)
The mean value of the end-to-end vector does not contain useful information,since it equals zero (〈r〉 = 0). This is so because the average over randomlyoriented vectors is 〈cosαi〉 = 0 assuming that all conformations have equal prob-abilities. Thus, the mean square root (rms) is a more expressive quantity for theconformation of the polymer chain [70]. So,
〈r2z〉 = N`2. (4.5)
Fully stretched, the size of the chain is determined by its contour length,L = N`. In its undeformed state, its average size is 〈r2z〉1/2 = N1/2`, so a polymerchain can be stretched by nearly a factor of
√N . However, this model suffers
from severe simplifications. The chains do not interact with any environment.Even as a single chain model this is a dramatic simplification, since the chain caninteract with itself.
It is important to realize, since we start treating the amorphous chain in ourmodel, that all conformations of the chain described within this theory are purelyentropic. The shape of the chain is driven purely by entropy. This means that
Figure 4.5: Conformational change in polymer.
46 CHAPTER 4. STATISTICAL APPROACH
the mean square root of the chain fluctuates around its value given by equation(4.5).
The shape, or “conformation” of a polymer molecule can range from thefully extended chain to the randomly coiled sphere as shown in figure 4.5. Theextended chain picture is the way we might choose to draw a polymer structure.The random coil picture, however, is a more realistic view of the shape of realpolymer molecules. Statistically, the coiled shape is much more likely than theextended one, simply because there are so many ways the chain can be coiled andonly one way it can be fully extended.
4.2.1 Thermodynamic approach of an amorphous network
To understand why rubbers are elastic, the full distribution function of theend-to-end lengths is needed to count all the stretched and all the coiled confor-mations of a polymer chain. More precisely, we would like to know how manydifferent conformations of the chain have the same end-to-end vector. Thus,Gaussian distribution is used in this context for the probability of a conforma-tion of the end-to-end vector of a randomly wriggling segment.
In the context of our recent model, we start treating the amorphous chain.According to Kuhn [41, 42], the number of conformations of the simply connectedchain from N statistically equivalent segments of length ` for a given end-to-enddistance R and under the prerequisite of large coiling R
L= R
N`<< 1 is given by
W (R) = K(β√π)3 exp [−β2R
2] , (4.6)
where β is a measure for the average end-to-end distance in the standard modelsof random walk,
β2 =3
2`
1
L, (4.7)
K is a proportionality constant, and L is the length of the totally stretchedmolecular chain.
Carved on the tombstone of Ludwig Boltzmann in the Zentralfriedhof (centralcemetery) in Vienna as shown in figure 4.6, is the inscription
S = k log W. (4.8)
This equation is the historical foundation of statistical mechanics. It connects themicroscopic and macroscopic properties. It defines the entropy S, a macroscopicquantity, in terms of the multiplicity W of the microscopic degrees of freedomof a system. For thermodynamics, k = 1.380662 × 10−23JK−1 is a quantity
4.2. OVERVIEW OF THE MODEL 47
Figure 4.6: Boltzmann grave stone in Vienna.
called Boltzmann’s constant, and Boltzmann’s inscription refers to the naturallogarithm, loge = ln.
Employing this fundamental equation (4.8) of Boltzmann’s formula to calcu-late the entropy of one chain molecule, will yield immediately the expression
H(θi) = k [3 ln (β√π)]− β2(θ21 + θ22 + θ23)] + k lnK . (4.9)
The number of chains with one end at the origin and the other end within theinterval (θi, θi + dθi) is proportional to equation (4.6) and given by
Z(θi) dθ1 dθ2 dθ3 = C
(β√π
)3
exp [−β2(θ21 + θ22 + θ23)] dθ1 dθ2 dθ3 ,(4.10)
where C is a constant that is determined by the requirement that the totalnumber of the chains in the material is σ . Then,
∫ ∞
−∞
∫ ∞
−∞
∫ ∞
−∞Z(θi) dθ1 dθ2 dθ3 = σ = C (4.11)
must hold. Rubbers and polymeric elastomers are chemically or physically cross-linked networks of polymer chains. The end points of the molecular chain arethe crosslinking points. One of the simplest and earliest assumptions regardingmicroscopic deformation in networks is that the crosslinking points in the networkmove affinely with the macroscopic deformation, which means that every part ofthe specimen deforms as does the whole (this is the elastic assumption). If onelays the co-ordinate axes of the chosen Cartesian co-ordinate system in the Eigendirections of the stretch tensor, the crosslinking points are shifted as shown infigure 4.7 according to
ϑ1 = Λ1θ1 , ϑ2 = Λ2θ2 , ϑ3 = Λ3θ3 . (4.12)
48 CHAPTER 4. STATISTICAL APPROACH
Figure 4.7: An affine deformation of a material.
Hence, the entropy of one chain molecule with affinely deformed endpoints is
H(ϑi) = k[3 ln (β√π)− β2(ϑ21 + ϑ22 + ϑ23)] + k lnK . (4.13)
Since an affine deformation of endpoints does not change the number of chainsof the network, one has
z(ϑi) dϑ1 dϑ2 dϑ3 = Z(θi) dθ1 dθ2 dθ3 . (4.14)
According to equations (4.10) (4.12), the number of chains for the affinely de-formed network is
z(ϑi) =σ
Λ1Λ2Λ3
(β√π
)3
exp
[
−β2(ϑ21Λ21
+ϑ22Λ22
+ϑ23Λ23
)
]
(4.15)
The entropies of the amorphous rubber in the undeformed and deformed statesare then
So =
∫ ∞
−∞
∫ ∞
−∞
∫ ∞
−∞H(θi) Z(θi) dθ1 dθ2 dθ3 (4.16)
= σk
[
3 ln
(β√π
)
− 3
2+ lnK
]
,
and
Sa =
∫ ∞
−∞
∫ ∞
−∞
∫ ∞
−∞H(ϑi) z(ϑi) dϑ1 dϑ2 dϑ3
=
∫ ∞
−∞
∫ ∞
−∞
∫ ∞
−∞H(ϑi) Z(θi) dθ1 dθ2 dθ3 (4.17)
= σk
[
3 ln
(β√π
)
− 1
2(Λ2
1 + Λ22 + Λ2
3) + lnK
]
.
4.2. OVERVIEW OF THE MODEL 49
The specific entropy of amorphous rubber can be expressed if one refers to a massunit, by division through the mass of network chains
m = σNmo , (4.18)
where mo is the mass of a segment. Thus, the specific entropy of the amorphousrubber networks is
sa = so −1
2
k
Nmo
(Λ21 + Λ2
2 + Λ23 − 3) , (4.19)
and this delivers just the stress coefficients (2.95) of the statistical theory for pureentropy elasticity.
4.2.2 Thermodynamic approach of a partially crystalline
network
The main purpose now is to propose a model that describes the deforma-tion induced crystallization of a network with partially crystallized chains. Theundeformed amorphous state has been chosen as a reference state for the entropy.
For partial crystallization some changes on the conformational entropy of themolecular chain must be made, since the molecular chain passes through differentdomains, mainly, amorphous and crystalline domains. However, when the chainfolds back to form a crystalline phase (lamellae), part of the amorphous chainforms closed loops which are free of force at the beginning of the deformation,until breakage of the crystalline folded-chains occurs, and then these closed loopchains become exposed to force. According to figure 4.8, the total number of chainsegments N is the summation of segments which are sitting in the crystallinedomains and those in the amorphous domains. The amorphous domain segmentsinclude segments which are exposed to deformation forces and those segmentssitting in the closed loops. Let ζ be the number of segments sitting within acrystalline domain (folded chain) in the chain. Then the total number of segmentsis given by
N = ζ︸︷︷︸
+ Nforce +Nloops︸ ︷︷ ︸
, (4.20)
crystalline amorphous
chain chain
segments segments
where N is the total number of chain segments, Nforce is the number of segmentsexposed to deformation stress, and Nloops is the number of segments sitting inthe force-free closed loops.
Both Nforce and Nloops have full conformational freedom. However with defor-mation, the number of segments exposed to force, Nforce increases as the folded
50 CHAPTER 4. STATISTICAL APPROACH
lamellae break. This breakage occurs at the early stages of deformation. Con-sequently, many loops will be opened and hence become part of the main chainwhich is exposed to force. This process continues until all loops are opened andall folded-parallel crystallites become extended. As a result, the number of seg-ments exposed to uniaxial stress Nforce, will become equal to the total numberof chain segments N .
The total length of the extended chain of N segments of length ` is shortenedas shown by the following equation and illustrated in figure 4.8.
Lξ = L− ζ`+ d = N`(1− ζ
N+
d
N`) . (4.21)
The degree of crystallinity ξ is introduced by
ξ =ζ
N=mc
m, (4.22)
where mc is the mass of the crystalline segments, m is the total mass of thechain, and d = |d| is the distance between the inlet and the exit of the chainsto the crystalline domain. This distance vector is proportional to the degree ofcrystallinity and is expressible as
d = aN` ξ , (4.23)
where a = |a| is a parameter of the theory depending on the type of crystallites.For parallel unfolded crystallites a = 1, and for folded or mixture type crystallitesa < 1.
Free loops
Free loops
Crystalline domain
rv
r ′v
rv ′′
dvα
Figure 4.8: A schematic of the proposed model of partially crystalline chain .
4.2. OVERVIEW OF THE MODEL 51
Consequently, the total length of the stretched and partially crystallized chainis
Lξ = L(1− ξ + aξ) . (4.24)
The length of the crystallite is equal to the length of the extended chain when-ever complete crystallization exists (which, theoretically, is never realized incrosslinked network) and parallel crystallites with a = 1 are formed. This will beconsistent with equation (4.1) that Lξ=1 = aL.
When the length of the amorphous chain L in equation (4.7) is replaced bythe length of the partially crystalline chain Lξ, the parameter β becomes
β2ξ =
3
2`
1
Lξ
= β2 1
(1− ξ + aξ). (4.25)
Since the parameter β is related to the mean square distance of the free chainends by 3
2β2= 〈r2〉, an increase from β to βξ means a reduction of the square
root mean of the chain by crystallization. Consequently, a piece of rubber withfree surfaces shrinks when it is crystallized.
The crystalline domains are relatively immobile compared to the chain seg-ments within the amorphous chain. This means that ζ = Nξ segments withinthe crystallites are frozen. Hence, the number of conformations of the N − ζsegments of the amorphous remainder of the chain is then
Wξ(r′ + r′′) = Kξ
(βξ√π
)3
exp [−β2ξ (r
′ + r′′)2] , (4.26)
where
r′ + r′′ = r− d . (4.27)
As shown in figure 4.8, equation (4.27) is the sum of possible statistical shifts ofthe N − ζ segments in the amorphous rest chain for a given distance vector r andgiven distance vector d between the inlet point and the exit point of the chain inthe crystallite.
The partially crystallized chain still contains a very large number of degreesof freedom. Therefore, Boltzmann’s formula (4.8) is applicable to calculate theconformational entropy of the chain. With equations (4.26) and (4.27) therefollows
Hξ(r,d) = k lnWξ
= k[3 ln
(βξ√π
)
− βξ2(r− d)2 + lnKξ] (4.28)
= k
[
3 ln (βξ√π)− βξ
2(r2 − 2 r d cosα + d2) + lnKξ
]
,
52 CHAPTER 4. STATISTICAL APPROACH
where α is the angle between the distance vector d and the distance vector r.Evidently, the value of α depends on the distance r = |r| of the chain end pointsand the “diameter” d = |d| of the crystallite. With increasing r and d the angleα decreases in the mean, i.e., the crystallites in the mean are directed into thedirection of the chain endpoints as well as by deformation and by crystallization,respectively.
For the calculation of the mean value 〈cosα〉 of cosα in equation (4.28) oneneeds the probability density for the angle α as shown in figure 4.8 at fixed valuesof r and d. From (4.26) and (4.27) this is
wξ(α; r; d) = C exp(A cosα) , A := β2ξ 2 r d , (4.29)
where C is a constant that can be determined by the requirement that wξ(α; r; d)is normalized to the complete solid angle, so that
∫ π
0
∫ 2π
0
wξ(α; r; d) sinα dα dϕ = C 4πsinh(A)
A= 1 , (4.30)
For the mean value of cosα there follows then
〈cosα〉 = L (A) = cothA− 1
A, (4.31)
where L (A) denotes the Langevin Function.
The mean value of the entropy (4.28) over all angles α at fixed values of rand d is then
〈Hξ(r,d)〉 = k[3 ln
(βξ√π
)
− βξ2(r2 + d2) (4.32)
+βξ2 2 r d L (βξ
2 2 r d) + lnKξ
].
If one end point of the chain is in the origin of a Cartesian co-ordinate systemand the other end point is at (x1, x2, x3), then r in equation (4.32) is to be replacedby
r =√
x21 + x22 + x23 . (4.33)
As a special case of equation (4.32) the mean entropy of a chain with degreeof crystallinity ξR, with one end point of the chain in the origin and the otherend at (X1, X2, X3), is as follows
〈HξR(R,dR)〉 = k[3 ln
(βR√π
)
− βR2(R2 + d2R) (4.34)
+βR2 2 RdR L (βR
2 2RdR) + lnKR
],
4.2. OVERVIEW OF THE MODEL 53
where R =√
X21 +X2
2 +X23 is the end-to-end distance between the chain ends,
dR = aN`ξR is the distance between the chain input and output to the crystallite,and β2
R = β2 11−ξR+aξR is the radius of inertia of the partially crystallized chain of
ξR.
For preparation of the subsequent calculations we need some formulae. Theseare the approximations [1]
zL (z) =1
3z2 − 1
45z4 , in 0 ≤ z ≤ 2 , (4.35)
zL (z) = z − 1 , in 2 ≤ z
for the Langevin Function, the error integral
erf(z) :=2√π
∫ z
0
exp (−x2) dx , (4.36)
and the integrals∫ z2
0
x12 e−xdx =
√π
2f1(z) ,
∫ z2
0
x32 e−xdx =
3√π
4f2(z) , (4.37)
∫ z2
0
x52 e−xdx =
15√π
8f3(z) ,
∫ z2
0
xe−xdx = 1− (1 + z2)e−z2
:= 1 +
√π
2f4(z) ,
where the functions fi(z) are given by the following expressions
f1(z) := erf(z)− 2√πz e−z
2
,
f2(z) := erf(z)− 2√πz (1 +
2
3z2)e−z
2
, (4.38)
f3(z) := erf(z)− 2√πz (1 +
2
3z2 +
4
15z4)e−z
2
.
Numerical calculation yields for large arguments z :
fi(z) = 1 for z ≥ 4 , i = 1, 2, 3 . (4.39)
The entropy of the partially crystallized rubber can be calculated, if the dis-tribution function for the number of chains is known. The number of chains isgiven for the purely amorphous material with finite chain length L = N`
Zo(θi) dθ1 dθ2 dθ3 = σ
(β√π
)31
f1(βL)exp[−β2(θ21 + θ22 + θ23)] dθ1 dθ2 dθ3 .(4.40)
54 CHAPTER 4. STATISTICAL APPROACH
Here f1(βL) comes from the finite chain length concept. However, this equa-tion is the same as equation (4.10) for infinite chain length, once L → ∞ thenf1(βL) = 1.
Since with crystallization no chains disappear, the number of chains in thepartially crystalline state is the same as in the amorphous undeformed referencestate |o. Then, one necessarly has
ZR(Xi) dX1 dX2 dX3 = Zo(θi) dθ1 dθ2 dθ3 , (4.41)
for the partially crystallized chain, of which the endpoints in the undeformedstate |R have the distance R. However, for the partially crystallized chains withdistance r in the deformed state the following expression is valid
zr(xi) dx1 dx2 dx3 = Zo(θi) dθ1 dθ2 dθ3 . (4.42)
To get the distribution function ZR(Xi) with respect to zr(xi), one must know howthe cross linking points (θ21+θ
22+θ
23) of the undeformed amorphous reference state
|o are transformed to the cross linking points (X1, X2, X3) in the reference state|R of the partially crystalline undeformed material. Furthermore the crosslinkingpoints (x1, x2, x3) of the partially crystalline and deformed state must be relatedto either one, |o or |R , of the undeformed states.
The transformation from the amorphous reference state |o with specific vol-ume vo to the partially crystalline reference state |R with specific volume vR isconnected with volume shrinkage. If crystallization takes place at constant hy-drostatic external pressure pR, the corresponding (affine) shift of all crosslinkingpoints is isotropic so that
Xi = Λcθi (i = 1, 2, 3) , where Λc =
(vRvo
) 13
. (4.43)
Equations (4.41) and (4.40) imply
ZR(Xi) =σ
f1(βL)
(γ√π
)3
exp[−γ2(X2
1 +X22 +X2
3 )], (4.44)
with
γ := β
(vovR
) 13
. (4.45)
The transformation from the amorphous reference state |o to the deformedpartially crystalline state goes via the partially crystalline (undeformed ) referencestate |R. The total shift of the crosslinking points is then
x1 = Λ1Λcθ1 , x2 = Λ2Λcθ2 , x3 = Λ3Λcθ3 . (4.46)
4.2. OVERVIEW OF THE MODEL 55
Inserting equation (4.46) into equation (4.42) with the help of equation (4.40),the following equation can be obtained
zr(xi) =1
Λ1Λ2Λ3
σ
f1(βL)
(γ√π
)3
exp
[
−γ2(x21
Λ21
+x22Λ22
+x23Λ23
)
]
. (4.47)
Now, the conformational entropy can be calculated for a partially crystallizednetwork at the undeformed reference state |R,
SKR =
∫ ∫ ∫
〈HξR(R,dR)〉ZR(Xi) dX1 dX2 dX3 . (4.48)
Inserting equations (4.35) and (4.44) yields, after transformation to sphericalcoordinates and performance of the angular integrations,
SKR =σk
f1(βL)
(γ√π
)3
4π[3 ln(
βR√π)− βR
2 d2R
+ lnKR
]∫ LR
dR
R2 e(−γ2R2) dR− σk
f1(βL)(γ√π)3 4π β2
R (4.49)
×∫ LR
dR
[R4 − 2R3 dR L (β2R 2RdR)]e
(−γ2R2) dR .
The R-integration must be performed from the smallest possible distance dR ofthe crosslinking points to the largest possible distance LR = N`(1− ξR) + dR ofthe partially crystalline chain. For the theoretical limit of complete crystallizationξR = 1 one has LR = dR = aN` , and the integrals in (4.49) vanish. This means,that the conformational entropy vanishes in the completely crystallized state, asit must do so.
The conformational entropy of the purely amorphous reference state |o is theother limiting case. This is obtained, if ξR = 0 and vR = vo is chosen. Withequations (4.40) or (4.44) and equation (4.23) we then obtain (d = 0, γ = β)
So =σk
f1(βL)
(β√π
)3
4π
[
3 ln(βR√π) + lnKo
] ∫ L
0
R2e−β2R2 dR (4.50)
− σk
f1(βL)
(β√π
)3
4πβ2
∫ L
0
R4e−β2R2 dR .
In the statistical theory of amorphous rubber one normally replaces the upperintegration limit L = N` by ∞. We will not do that, in order to have a smoothconnection to the partially crystallized reference state.
The integrations for the conformational entropy in the undeformed amorphousstate |o can also be performed with the result
So = σk
[
3 ln
(β√π
)
+ lnKo
]
− σ k3
2
f2(βL)
f1(βL). (4.51)
56 CHAPTER 4. STATISTICAL APPROACH
In the following we insert the approximations (4.35) for the Langevin Func-tion into equation (4.49). Separating the integration interval in domains dR ≤R ≤ 1
β2RdR
and 1β2RdR≤ R ≤ LR and performing the integrations yields for the con-
figurational entropy of the undeformed and partially crystalline reference state1
|R
SKR =σk
f1(βL)
[
3 ln
(βR√π
)
− βR2d2R + lnKR
]
[f1(γLR)− f1(γdR)]
− σk
f1(βL)
3
2
β2R
γ2[f2(γLR)− f2(γdR)] (4.52)
+σk
f1(βL)He(dR ≤ DR)
3
2
β2R
γ2
{4
3βR
2d2R [f2(γDR)− f2(γdR)]
−8
9
β6Rd
4R
γ2[f3(γDR)− f3(γdR)]
}
− σk
f1(βL)He(DR ≤ LR)
{
[f1(γLR)− f1(γDR)]
−2β2RdRγ
[f4(γLR)− f4(γDR)]
}
,
with
He(x ≤ y) :=
{1 for x ≤ y0 for x > y
}
,
DR = D(ξR) :=inf
0≤ξR≤1
{1
β2RdR
, LR
}
,
where He(x ≤ y) is the Heaviside unit jump that is used to distinguish bothintegration intervals of the Langevin function for its approximation shown byequation (4.35).
It is pointed out, that the parameter ln KR, besides the parameters N and`, depends in addition on the macroscopic variables ξR, TR, pR. The form of thisdependence is not given by the statistical theory. We have to determine this byreasonable macroscopic requirements. This will be done later on.
The purely amorphous limit of equation (4.51) results as a special case forξR = 0 and vR = vo, if lnKR|ξR=0
= lnKo. The theoretical limit of complete
1The computations of equation (4.52) have been done analytically and they are availableupon request.
4.2. OVERVIEW OF THE MODEL 57
crystallization2 is dR|ξR=1 = LR|ξR=1= DR|ξR=1
. The conformational entropy of
equation (4.52) is then zero, as it must be.
In the sequel, the conformational entropy in the deformed and partially crys-tallized state of crystallinity ξ is calculated starting from the following expressions
SK =
∫ ∫ ∫
〈Hξ(r,d)〉zr(xi) dx1dx2dx3 . (4.53)
If one inserts the expressions in (4.32) for the mean conformational entropy of onechain and (4.47) for the distribution of the chain end points and if one introducesthe isochoric deformations along the eigen-axes of deformation,
λi = (v
vR)−
13Λi (i = 1, 2, 3) , λ1λ2λ3 = 1 , (4.54)
then the following can be obtained
SK =σk
f1(βL)
(δ√π
)3 ∫ ∫ ∫ [
3 ln
(βξ√π
)
− β2ξ (r
2 + d2) + lnKξ
+β2ξ 2r dL (β2
ξ 2 r d)
]
exp
[
−δ2(x21
λ21+x22λ22
+x23λ23
)
]
dx1 dx2 dx3, (4.55)
where δ is the abbreviation
δ := β(vov)13 . (4.56)
To incorporate the integration limits spherical coordinates x1 = r cosϑ , x2 =r sinϑ cosϕ , x3 = r sinϑ sinϕ are introduced. The integration limits are thed ≤ r ≤ Lξ = N`(1 − ξ) + d, 0 ≤ ϑ ≤ π, 0 ≤ ϕ ≤ 2π. For the entropy thencefollows
SK =σk
f1(βL)(δ√π)3∫ π
0
dϑ
∫ 2π
0
dϕ
∫ Lξ
d
dr r2 sinϑ× exp(−δ2µr2) (4.57)
×[3 ln(
βξ√π)− β2
ξ (r2 + d2) + β2
ξ 2 r dL (β2ξ 2 r d) + lnKξ
],
where µ is the abbreviation
µ(ϑ, ϕ, λi) :=cos2 ϑ
λ21+
sin2 ϑ cos2 ϕ
λ22+
sin2 ϑ sin2 ϕ
λ23(4.58)
and
δ = β(vov)13 = βξ = β
1√1− ξ + aξ
. (4.59)
2In crosslinked high polymers; complete crystallization is not possible due to steric hin-drances of the chemical bonds around the cross links (excluded volume). The degree of crys-tallinity varies consequently between 0 ≤ ξ ≤ ξmax < 1 .
58 CHAPTER 4. STATISTICAL APPROACH
The r−integration can be performed at once using the approximation (4.35)for the Langevin function and using the relations (4.37). After some calculationone obtains3
SK =σk
f1(βL)
[
3 ln
(βξ√π
)
− β2ξ d
2 + lnKξ
]
[F1(δLξ, λi)− F1(δd, λi)]
− σk
f1(βL)
3
2
β2ξ
δ2[F2(δLξ, λi)− F2(δd, λi)] (4.60)
+σk
f1(βL)He(d ≤ Dξ)
3
2
β2ξ
δ2
{4
3βξ
2d2[F2(δDξ, λi)− F2(δd, λi)]
−8
9
β6ξd
4
δ2[F3(δDξ, λi)− F3(δd, λi)]
}
− σk
f1(βL)He(Dξ ≤ Lξ)
{
[F1(δLξ, λi)− F1(δDξ, λi)]
−2β2
ξd
δ[F4(δLξ, λi)− F4(δDξ, λi)]
}
,
with
He(x ≤ y) :=
{1 for x ≤ y0 for x > y
}
,
Dξ = D(ξ) :=inf
0≤ξR≤1
{
1
β2ξd, Lξ
}
.
The functions F1, F2, F3, F4 are given by the integrals
F1(α;λi) =1
4π
∫ π
0
∫ 2π
0
1
µ3/2f1(αµ
1/2) sinϑ dϑ dϕ ,
F2(α;λi) =1
4π
∫ π
0
∫ 2π
0
1
µ5/2f2(αµ
1/2) sinϑ dϑ dϕ , (4.61)
F3(α;λi) =1
4π
∫ π
0
∫ 2π
0
1
µ7/2f3(αµ
1/2) sinϑ dϑ dϕ ,
F4(α;λi) =1
4π
∫ π
0
∫ 2π
0
1
µ2f4(αµ
1/2) sinϑ dϑ dϕ ,
for α = δLξ or α = δd or α = δDξ.For the undeformed, partially crystallized reference state |R with ξ = ξR and
3The computations of equation (4.60) have been done analytically and they are availableupon request.
4.2. OVERVIEW OF THE MODEL 59
λi = 1 (i = 1, 2, 3) are µ = 1, δ = γ , d = dR, βξ = βR , and Dξ = DR. Then,Fa(αR; 1) = fa(αR) (a = 1, 2, 3, 4) for αR = γLR, αR = γdR, αR = γDR,respectively.
The major problem is now the performance of the integrations (4.61). Forsimplification we consider uniaxial extension. If λ1 ≥ 1 is the isochoric lengthratio in the direction of extension, then
λ2 = λ3 =1√λ1
. (4.62)
According to equation (4.58), µ is then independent of the angle ϕ and given by
µ = λ1
[
1− (1− 1
λ31) cos2 ϑ
]
. (4.63)
The ϕ-integration in equation (4.61) can be performed directly. After substitutionof
ω =
√
(1− 1
λ31) cos2 ϑ (4.64)
and integration by parts in ω, using the relations
1
(1− ω2)3/2=
d
dω
[ω
(1− ω2)1/2
]
,
1
(1− ω2)5/2=
d
dω
[ω
(1− ω2)3/2+ 2
ω
(1− ω2)1/2
]
, (4.65)
1
(1− ω2)7/2=
d
dω
[ω
(1− ω2)5/2+
4
3
ω
(1− ω2)3/2+
8
3
ω
(1− ω2)1/2
]
,
1
(1− ω2)2=
1
2
d
dω
[ω
(1− ω2)+ artanh(ω)
]
,
1
(1− ω2)=
d
dω[artanh(ω)] ;
e−α2λ1(1−ω2) = 1− (1− ω2)
∫ α2λ1
0
e−β(1−ω2) dβ ,
the further substitution of y = α2λ1ω2 and integration by parts once more using
60 CHAPTER 4. STATISTICAL APPROACH
equations (4.38) and (4.37)4 ,then yields4
F1(α;λ1) = f1(α
λ1) +
2√π
α
λ1e−α2
λ21 − 2√π
1
λ3/21
√De−α
2λ1
∫ α√λ1D
0
ex2
dx
= erf(α
λ1)− 2√
π
1
λ3/21
√De−α2
λ21 D(α√
λ1D) ,
F2(α;λ1) =1
3(λ21 +
2
λ1) f2(
α
λ1) +
2√π
2
3
α
λ1e−α2
λ21
[
α21
3(1 +
2
λ31) +
1
λ1
]
− 2√π
2
3
[
α2 +1
λ1
]1
λ3/21
√De−α
2λ1
∫ α√λ1D
0
ex2
dx
=1
3
(
λ21 +2
λ1
)
erf(α
λ1)− 2√
π
1
3αλ1 e
−α2
λ21
− 2√π
2
3(α2 +
1
λ1)
1
λ3/21
√De−α2
λ21 D(α√
λ1D) ,
F3(α;λ1) =1
5(λ41 +
4
3λ1 +
8
3
1
λ21) f3(
α
λ1) (4.66)
+2√π
4
15
α
λ1e−α2
λ21
[α4
5
(
1 +4
3
1
λ31+
8
3
1
λ61
)
− 4
3
α2
λ1
(
1− 1
λ31
)
+2
λ1
(
α2 +1
λ1
)]
− 2√π
4
15
[
α4 +2
λ1
(
α2 +1
λ1
)]1
λ3/21
√De−α
2λ1
∫ α√λ1D
0
ex2
dx
=1
5(λ41 +
4
3λ1 +
8
3
1
λ21) erf(
α
λ1)
− 2√π
2
15αλ1
[
α2 +2
λ1(1 +
4
3λ31)
]
e−α2
λ21
− 2√π
4
15
[
α4 +2
λ1(α2 +
1
λ1)
]1
λ3/21
√De−α2
λ21 D(α√
λ1D) ,
F4(α;λ1) =2√π
1
λ21√D
[∫ α
√λ1
0
e−y2
∫ y√D
0
(
ex2
dx)
dy − 1
2artanh(
√D)
]
− 2√π
λ12e−α2
λ21 − 2√π
α
λ1
e−α2λ1
√λ1D
∫ α√λ1D
0
ex2
dx
=1√λ1D
Derf(λ1√
λ1D;α
λ1)− 2√
π
1
2λ21√D
artanh(√D)
− 2√π
λ12e−α2
λ21 − 2√π
α
λ1√λ1D
e−α2
λ21 D(α√
λ1D) .
4The cumbersome computations of equations (4.66) have been done analytically and areavailable upon request.
4.2. OVERVIEW OF THE MODEL 61
where the abbreviation
D := 1− 1
λ31(4.67)
has been used, and D(z) denotes the Dawson-Integral [1]
D(z) := e−z2
∫ z
0
ex2
dx . (4.68)
Moreover, Derf(b; z) is a modified error function [57, 44], which is modified withthe Dawson-Integral,
Derf(b; z) :=2√π
∫ z
0
D(bx)e−x2
dx . (4.69)
If λ1 = 1 , then
Fj(α; 1) = fj(α) (j = 1, 2, 3, 4) . (4.70)
Therefore the conformational entropy at the undeformed partially crystallizedreference state |R, calculated by equation (4.60), is reduced to equation (4.52) inthe limiting case of ξ = ξR.
On the other hand, the conformational entropy of the totally amorphous ma-terial in the deformed state is also included in equation (4.60). It is obtained ifone sets ξ = 0 , v = vo , δ = β, Lξ = L , and d = 0. For α = δLξ = βL andα = δd = 0, respectively, one obtains from equation (4.66)
F1(βL;λ1) = erf(βL
λ1)− 2√
π
1
λ3/21
√De−β
2L2λ1
∫ βL√λ1D
0
ex2
dx ,
F2(βL;λ1) =1
3(λ21 +
2
λ1) erf(
βL
λ1)− 2√
π
1
3βLλ1e
−β2L2
λ21 (4.71)
− 2√π
2
3(β2L2 +
1
λ1)
1
λ3/21
√De−β
2L2λ1
∫ βL√λ1D
0
ex2
dx ,
F1(0;λ1) = 0 ,
F2(0;λ1) = 0 ,
and with this, (4.60) and (4.70) imply
Sa = σk
[
3 ln(β√π) + lnKa
]
× F1(βL;λ1)
F1(βL; 1)− σk
3
2
F2(βL;λ1)
F1(βL; 1). (4.72)
For the undeformed amorphous material limλ1→1 Sa = So. As a consequence, dueto (4.70),
Ka = Ko . (4.73)
62 CHAPTER 4. STATISTICAL APPROACH
Hence from (4.51) and (4.70) follows the entropy of the totally amorphous mate-rial
Sa − So = −σk32
F2(βL;λ1)− F2(βL; 1)
F1(βL; 1)+ σk [3 ln(
β√π) + ln Ko]
×F1(βL;λ1)− F1(βL; 1)
F1(βL; 1). (4.74)
For control we consider the infinitely long chain. According to (4.1) and (4.7) we
have βL =√
32N . Furthermore, since
limβL→∞
F1(βL) = 1 , limβL→∞
F2(βL) =1
3(λ21 +
2
λ1) , (4.75)
the entropy difference (4.74) is
limλ1→∞
(Sa − So) = −σk1
2
[
(λ21 +2
λ1)− 3
]
, (4.76)
the classical result, as given in (4.16) and (4.17).
So far, we considered only the conformational entropy of the chains. Thecrystalline regions themselves, however, also have entropy. That is due to thefact that, when the transformation occurs from the partially crystallized stateto the amorphous state, the entropy increases by the melting entropy ∆S. Theentropy of the partially crystallized rubber is then reduced as compared to theamorphous state (reference state), by the melting entropy
S − So = Sk − So −∆S . (4.77)
Let so = Sa(ξ = 0, T ) be the specific entropy of the undeformed, totally amor-phous material, sc(T ) the specific entropy of the crystalline domain, and mo themass of a statistical segment. Then the melting entropy per segment is
Sσ(T ) = mo[so(T )− sc(T )] . (4.78)
The melting entropy of the rubber is obtained by multiplication with the numberof total segments in the network σζ = σNξ, which is bounded in the crystallinedomains
∆S = σNξ Sσ(T ) . (4.79)
The entropy of the partially crystallized rubber5 follows from equations (4.77) to
5The computations of equation (4.80) have been done analytically and are available uponrequest.
4.2. OVERVIEW OF THE MODEL 63
(4.79) and equations (4.60) and (4.59):
S − So = −σNξSσ + σk3
2
F2(β; 1)
F1(β; 1)− σk
[
3 ln(β√π) + lnKo
]
+σk[3 ln(βξ√π)− β2
ξd2 + lnKξ]
F1(βξLξ;λ1)− F1(βξd;λ1)
F1(βL; 1)
−σk32
F2(βξLξ;λ1)− F2(βξd;λ1)
F1(βL; 1)(4.80)
+σk He(d ≤ Dξ) 2β2ξd
2
{F2(βξDξ;λ1)− F2(βξd;λ1)
F1(βL; 1)
−2
3β2ξd
2 F3(βξDξ;λ1)− F3(βξd;λ1)
F1(βL; 1)
}
−σk He(Dξ ≤ Lξ)
{F1(βξLξ;λ1)− F1(βξDξ;λ1)
F1(βL; 1)
−2βξdF4(βξLξ;λ1)− F4(βξDξ;λ1)
F1(βL; 1)
}
The entropy difference SR − So of the partially crystallized reference state |Rfor ξ = ξR, βξ = βR, Lξ = LR, d = dR , T = TR, and λ1 = 1 is included as aspecial case. Both entropy differences are smaller or equal to zero S−So ≤ 0 andSR−So ≤ 0 . The entropy of the rubber decreases with crystallization as well aswith deformation by increasing the state of ordering and orientation, as it mustdo so.
For the calculation of the stress one needs the free energy and for this theinternal energy. We assume now that within the molecular chain, apart from thekinetic and binding energies within the crystalline domains, no internal energyof deformation can be stored. This corresponds to the model of Kuhn (simplyand freely joint chains). We refer again to the undeformed totally amorphousstate as a reference state for the energy. Thus the binding energy is just meltingenergy. Consequently, the change of the internal energy with crystallization anddeformation is
U − Uo = −∆U = −σNξ Uσ(T ) , (4.81)
where Uσ(T ) is the melting energy per segment. This is given by
Uσ(T ) = mo[uo(T )− uc(T )] , (4.82)
where uo(T ) is the specific (thermal) internal energy of the amorphous unde-formed material and uc(T ) is the specific internal energy of the crystalline do-mains, both at temperature T .
64 CHAPTER 4. STATISTICAL APPROACH
The free energy related to the undeformed totally amorphous state at tem-perature T is given by
F − Fo = U − Uo − T (S − So) , Fo(T ) = Uo(T )− T So(T ) . (4.83)
For the calculation of the nominal stress for uniaxial extension we need thederivative of the free energy with respect to λ1 for fixed values of ξ and T .According to equations (4.81) and (4.82),
∂F
∂λ1= −T ∂S
∂λ1, (4.84)
since U,Uo, So and Fo are independent of λ1. The nominal stress is
σ1 =1
vR(vRvo
)1/3∂F
∂λ1. (4.85)
Dividing by the total mass of the rubber σNmo and using the relationsβξβ
= (vov)1/3 and βR
β= ( vo
vR)1/3, following from equation (4.59), for the volume
ratios, (4.85) takes the form
σ1 = ρRβξβR
1
σNmo
∂F
∂λ1= −ρR
βξβR
T
σNmo
∂S
∂λ1. (4.86)
Let NL be the Loschmidt-Avogadro number; then R = kNL is the universalgas constant and Mo = NLmo is the molecular weight of the statistical segment.
Using (4.80) the nominal stress in uniaxial extension thus becomes
σ1 = ρRβξβR
RTNMo
1
F1(βL; 1)
×{[
3 ln(βξ√π)− β2
ξd2 + lnKξ
]∂
∂λ1[F1(βξLξ;λ1)− F1(βξd;λ1)]
+3
2
∂
∂λ1[F2(βξLξ;λ1)− F2(βξd;λ1)]
−He(d ≤ Dξ) 2 β2ξd
2 ∂
∂λ1[F2(βξDξ;λ1)− F2(βξd;λ1)] (4.87)
+He(d ≤ Dξ)4
3β4ξd
4 ∂
∂λ1[F3(βξDξ;λ1)− F3(βξd;λ1)]
+He(Dξ ≤ Lξ)∂
∂λ1[F1(βξLξ;λ1)− F1(βξDξ;λ1)]
−He(Dξ ≤ Lξ) 2βξd∂
∂λ1[F4(βξLξ;λ1)− F4(βξDξ;λ1)]
}
.
4.2. OVERVIEW OF THE MODEL 65
The derivatives of the functions Fj(α, λ1), (j = 1, 2, 3, 4) are obtained from (4.66).After some lengthy calculations and appropriate rearrangement one obtains
∂F1(α;λ1)
∂λ1=
2
3
(
λ1 −1
λ21
)[
−9
4
α
λ1R1(α;λ1)
]
,
∂F2(α;λ1)
∂λ1=
2
3
(
λ1 −1
λ21
)[
erf
(α
λ1
)
− 2
3
α
λ1R2(α;λ1)
]
, (4.88)
∂F3(α;λ1)
∂λ1=
2
3
(
λ1 −1
λ21
)[6
5
(
λ21 +4
3
1
λ1
)
erf
(α
λ1
)
−3
5
α
λ1R3(α;λ1)
]
,
∂F4(α;λ1)
∂λ1= −1
2(λ1 −
1
λ21)
[3 +D
(λ1D)5/2Derf(λ1
√
λ1D;α
λ1)
+1
λ1R4(α;λ1)−
2√π
3 +D
2(λ1D)21√D
artanh(√D)
]
,
with the abbreviations
R1(α;λ1) =2√π
e−α2
λ21
(λ1D)2
{
1− (1 +2
3α2λ1D)
D(α√λ1D)
α√λ1D
}
,
R2(α;λ1) =2√π
e−α2
λ21
(λ1D)2
{
[α2 +1
3(2λ21 +
1
λ1)]
−[
(α2 +1
λ1)(1 +
2
3α2λ1D) +
2
3
D
λ1
]D(α
√λ1D)
α√λ1D
}
, (4.89)
R3(α;λ1) =2√π
e−α2
λ21
(λ1D)2
{[
α4 + α2 2
λ1(1 +
2
3λ31D) + 2λ41
]
−[
(α2 +1
λ1)2(1 +
2
3α2λ1D) + (α2 +
1
λ1)2D
λ1
+1
λ21(1 +
2
3D)
]D(α
√λ1D)
α√λ1D
}
,
R4(α;λ1) =2√π
e−α2
λ21
(λ1D)2
{[
3(α2 +1
2λ1) + λ21D
]
−α2
[
2(α2 +1
2λ1)λ1D + 3
]D(α
√λ1D)
α√λ1D
}
.
We insert now the expressions of equation (4.88) into equation (4.87), byidentification of α with βξLξ, βξd, and βξDξ, respectively. For the nominal stress
66 CHAPTER 4. STATISTICAL APPROACH
we obtain the expression
σ1 = ρRβξβR
RTNMo
(
λ1 −1
λ21
)1
F1(βL; 1)
×{
−[
3 ln
(βξ√π
)
− β2ξd
2 + lnKξ
]
×3
2
1
λ1〈βξLξ R1(βξLξ;λ1)− βξd R1(βξd;λ1)〉
+
[
erf(βξLξ
λ1)− erf(
βξd
λ1)
−3
2
1
λ1〈βξLξ R2(βξLξ;λ1)− βξd R2(βξd;λ1)〉
]
−He(d ≤ Dξ)4
3β2ξd
2
[
erf(βξDξ
λ1)− erf(
βξd
λ1) (4.90)
−3
2
1
λ1〈βξDξ R2(βξDξ;λ1)− βξd R2(βξd;λ1)〉
]
+He(d ≤ Dξ)8
15β4ξd
4
[
2(λ21 +4
3
1
λ1)
⟨
erf(βξDξ
λ1)− erf(
βξd
λ1)
⟩
− 1
λ1〈βξDξ R3(βξDξ;λ1)− βξd R3(βξd;λ1)〉
]
−He(Dξ ≤ Lξ)3
2
1
λ1〈βξLξ R1(βξLξ;λ1)− βξDξ R1(βξDξ;λ1)〉
+He(Dξ ≤ Lξ) βξd
[3 +D
(λ1D)5/2
⟨
Derf(λ1√
λ1D;βξLξ
λ1)
−Derf(λ1√
λ1D;βξDξ
λ1)
⟩
+1
λ1〈R4(βξLξ;λ1)−R4(βξDξ;λ1)〉
]}
.
4.2.3 Mooney representations
The phenomenological theory of Mooney [52] has played a dominant part inthe field of large elastic deformation.
Mooney’s theoretical assumptions, as has been noted earlier in connectionwith the statistical theory, is that the rubber is incompressible, and that it isisotropic in the unstrained state. Mooney formula is presented as follows:
σ1 = (λ1 −1
λ21)(2C1 +
2C2
λ1) , (4.91)
4.2. OVERVIEW OF THE MODEL 67
where σ1 is the nominal (engineering) stress (force per unit undeformed area),and C1, C2 are empirical constants. We now write equation (4.91) in the form
σ1(λ1 − 1
λ21)= 2C1 +
2C2
λ1. (4.92)
Figure 4.9: Mooney-Rivlin representation for cross-linked natural rubber, wheref ∗ equals to σ1
(λ1− 1
λ21)and α−1 equals 1
λ1.
It is clear that plotting σ1(λ1− 1
λ21)against 1
λ1should yield a line of slope 2C2, with
intercept 2(C1 + C2) on the vertical axis of 1λ= 1 . Thus more details about the
stress coefficients can be obtained using this formula. A large increase in modulusat high elongation is illustrated by figure 4.9 for natural rubber [50, 20] in theMooney-Rivlin representation. This increase in the modulus is generally observedin crystallizable networks with chemical cross-linking that undergo strain-inducedcrystallization.
This is included in the present statistical model, in which these stress coef-ficients C1 and C2 are functions of (λ1, ξ). Identification of (4.90) with (4.91)
68 CHAPTER 4. STATISTICAL APPROACH
yields for the Mooney coefficients:
2C1 = ρRβξβR
RTNMo
1
F1(βL; 1)
×{[
erf
(βξLξ
λ1
)
− erf
(βξd
λ1
)]
−He(d ≤ Dξ)4
3β2ξd
2
[
erf
(βξDξ
λ1
)
− erf
(βξd
λ1
)]
+He(d ≤ Dξ)8
15β4ξd
4
[
2(λ21 +4
3
1
λ1)
⟨
erf(βξDξ
λ1)− erf(
βξd
λ1)
⟩]
−He(Dξ ≤ Lξ) βξd
[3 +D
(λ1D)5/2
⟨
Derf(λ1√
λ1D;βξLξ
λ1)
−Derf(λ1√
λ1D;βξDξ
λ1)
⟩]}
,
(4.93)
2C2 = ρRβξβR
RTNMo
1
F1(βL; 1)
×{
− [3 ln(βξ√π)− β2
ξd2 + lnKξ]
×3
2〈βξLξ R1(βξLξ;λ1)− βξd R1(βξd;λ1)〉
−3
2〈βξLξ R2(βξLξ;λ1)− βξd R2(βξd;λ1)〉
+He(d ≤ Dξ)4
3β2ξd
23
2〈βξDξ R2(βξDξ;λ1)− βξd R2(βξd;λ1)〉
+He(d ≤ Dξ)8
15β4ξd
4 〈βξDξ R3(βξDξ;λ1)− βξd R3(βξd;λ1)〉
−He(Dξ ≤ Lξ)3
2〈βξLξ R1(βξLξ;λ1)− βξDξ R1(βξDξ;λ1)〉
+He(Dξ ≤ Lξ) βξd 〈R4(βξLξ;λ1)−R4(βξDξ;λ1)〉}
.
Chapter 5
Model Application
5.1 Model Parameters
Three crucial parameters are included in our proposed statistical theory ofdeformation induced crystallization: the degree of crystallinity ξ, the number ofsegments which are exposed to the deformation stress Nforce, the parameter a,and the entropy constant Kξ of partially crystallized rubber. Besides, we needthe total number of N of chain segments and their length `.
5.1.1 Degree of crystallinity ξ
The degree of crystallinity is a vital parameter to our statistical model. InChapter 3, a mathematical model has been developed to simulate the deformation-induced crystallization at different parameters (e.g. temperature and strain rate).
The relaxation time τ , for loading and unloading deformation, is greatly af-fected by temperature as it is evident by equations (3.14) and (3.19), and thestrain rates. The effect of strain rates is summarized by the following tables 5.1,5.2 for both polyisoprene rubber and polyethylene-butene copolymer as well1.
Table 5.1: Effect of strain rate on the constants of the relaxation time for loading-unloading polyisoprene rubber at all temperatures
Strain rate [min−1] aL [s] bL[J/mole] aU [s] bU [J/mole]
0.039 0.050 15000 0.005 150002.340 0.004 15000 0.002 15000
1These constants were fitted using Mathematica fitting technique.
69
70 CHAPTER 5. MODEL APPLICATION
Table 5.2: Effect of strain rate on the constants of the relaxation time for loading-unloading of the thermoplastic elastomer (both types) at all temperatures
Strain rate [min−1] aL[s] bL[J/mole] aU [s] bU [J/mole]
0.09 0.050 15000 0.0250 150005.40 0.001 15000 0.0002 15000
From the above tables, it is clear that aL and aU are dependent on both strainrates. Unfortunately, few experiments have been performed with respect to strainrates, however, this is not sufficient to perform fitting for this dependence.
The degree of crystallinity is calculated for both loading and unloading, fromequations (3.15) and (3.20), respectively. Then they are inserted into the stress-strain equation (4.90) as an input parameter. To meet agreement with the mea-surement data, the parameter a must be properly chosen. This is discussed inthe following section.
5.1.2 Parameter a
The parameter a as introduced by equation (4.23) and figure 4.8, is a measurefor the type of crystallite attributed to our molecular chain. Its value changes de-pending on the type of crystallites, whether extended or folded or mixed. Withinthe context of the statistical theory, the value of a is unknown. It must bedetermined by fitting of statistical stress-strain relation (4.90) to the measuredstress-strain curves for isothermal (and isobaric) uniaxial extension.
It turns out, that the parameter a depends on temperature, on deformationspeed and, of course, on the rubber-elastic and crystallizable materials consid-ered. Moreover, chain parameter a may depend on deformation λ1 for uniaxialextension.
The best fit to the stress-strain loading curves is obtained with the constantchain parameter a, independent of deformation λ1.
This reflects the physical expectation that during loading the extensional typeof crystallinity is favoured. Best fit values for the polyisoprene are given in table5.3 for different temperature and two loading speeds. Corresponding values forthe two thermoplastic elastomers ENX-7086 and ENX-7256 are given in tables5.4 and 5.5, respectively2.
2The constants shown in Tables 5.3, 5.4, and 5.5 were fitted using Mathematica fittingtechnique.
5.1. MODEL PARAMETERS 71
For unloading the crystallization behaviour is more complex. Besides theextended type of crystallization the folded type develops in unloading using theextended type as a nuclei for growing perpendicular to this to a shish-kebabstructure.The formation of these crystallites requires relaxation of chain ordering,for which λ1 is a measure. Consequently, the chain parameter a depends on λ1for unloading. With the following expression3:
a(T ) = ao + a1λ1 + a2λ21 + a3λ
31 + a4 cosh
√
λ−11 + a5 eλ21 , (5.1)
and perfect fitting of the unloading curves can be obtained. The temperaturedependent fitting parameters ao, a1, a2, a3, a4, and a5 obtained by Mathematicacurves-fitting technique are tabulated in Appendix A for two given strain rates,and the three considered rubber-like materials.
Table 5.3: Parameter a values for loading process of polyisoprene
Temperature [◦C] strain rate [min−1] a
21 0.039 and 2.34 0.26150 0.039 and 2.34 0.37580 0.039 0.490
Table 5.4: Parameter a values for loading process of ENX-7086
Temperature [◦C] strain rate [min−1] a
23 0.09 0.28023 5.40 0.15050 0.09 0.37050 5.40 0.380
Table 5.5: Parameter a values for loading process of ENX-7256
Temperature [◦C] strain rate [min−1] a
23 0.09 0.24023 5.40 0.25050 0.09 0.30050 5.40 0.150
3This formula has been fitted using Mathematica curves-fitting technique.
72 CHAPTER 5. MODEL APPLICATION
5.1.3 Number of segments exposed to deformation, Nforce
As has been discussed in equation (4.20), Nforce increases with deformationduring loading extension until it reaches the total number of chain segments N .This is expressed as4
Nforce(λ1) = bo + b1λ1 + b2λ21 + b3λ
31 + b4λ
41 + b5e
[
1.25(λ21+2λ1
)
], (5.2)
where bo, b1, b2, b3, b4, and b5 are adjustable fitting parameters of the model de-pending on temperature. The values of these fitting parameters obtained byMathematica curve-fitting technique are tabulated in Appendix B.
However for unloading, since all lamellae of the folded chain crystallites aresplit and become extended, Nforce will equal to the total number of chain segmentsas follows
Nforce = N . (5.3)
(The total number of segments per chain N can be obtained, if a reasonableassumption is made about the molecular weight Mo of the segment. For this it isobserved, that the identity unit of the molecule contains five carbon single bonds,around which almost iso-energetic rotations can take place. At a 1.5-fold length,e.g. 7.5 carbon single bonds, the end point of the 1.5-fold identity unit can reachalmost all positions in space if one end is held fixed. Thus the poly-cis-isoprenemolecule has the molecular weight of 183 g/mole and a total number of segmentsper one chain N = 55. However, the Ethylene-butene molecule has the molecularweight of 120 g/mole and a total number of segments per one chain N = 63.
It should be remarked, that the identity unit of the poly-cis-isoprene moleculeand ethylene-butene molecule without attacking the valence angles of the carbon-carbon distances in the extended state of the chain has a length of 8.8A. Thelength of the extended segment without attacking the valence angle is then ` =1.5× 8.8 A = 13.2 A)5.
5.1.4 Entropy constant Kξ of partially crystallized chains
Now the entropy constant Kξ of the conformational entropy of the partiallycrystallized state is proposed as the expression
Kξ = eνoNs , (5.4)
4This formula has been fitted using Mathematica curves-fitting technique.5These informations have been obtained by personal communication with Prof. Dr. Rolf
Hosemann, Bundesanstalt fur Materialprufung BAM-Berlin.
5.2. APPLICATION OF THE MODEL 73
where νo is an adjustable parameter. Ns is the number of free conformationaluncrystallized segments determined by
Ns = N(1− ξ) = N − ζ . (5.5)
νo is found to be temperature dependent for each material. The values of thisparameter, depending on the material, are shown in Table 5.66.
Table 5.6: Values of νo for three different polymeric materials.T(◦C) polyisoprene rubber νo(ENX − 7086) νo(ENX − 7256)
21 0.75 – –23 – 2.75 1.5050 0.60 1.65 0.5380 0.50 – –
5.2 Application of the Model
With the above proposed model we are now in the position with this statisticaltheory of deformation induced crystallization to describe in an analytical way thepseudo-plastic effect and hysteresis in cross-linked rubber, elastomers and highpolymers.
5.2.1 Polyisoprene crosslinked rubber
The old term Cauotchouc7 was taken from the word Cauo-Chu meaning the”weeping tree”. Many useful objects are made from the milk of the weeping tree.Batonists gave it the name Hevea Brasiliensis. The milk produced is an aqueousemulsion or dispersion of oils, fats, waxes, resins, starch, proteins. The maincomponent is polyisoprene that is described by the chemical formula (C5H8)n.C5H8 is called an isoprene and natural rubber is built up of regular sequencesof isoprene, which are arranged in cis-configuration, forming long chains of highelasticity, see figure 5.1. The chains are linked and lie in the material like agitatedsnakes, they are perfectly regular in the backbone and have freely rotating linksat given distance.
6These constants were fitted using Mathematica software.7This complicated French word is said to stem from the Indian word Ca-hu-chu which means
“weeping tree”. Others maintain that it comes from the Kechuan language where cauchu means“he who casts the evil eye”; they find that notion appropriate because of the atrocious conditionsunder which the Indians were forced to collect rubber. So we may safely assume that the originof the word is unknown. As caucho, caucciu and Kautschuk it provides the scientific name forrubber in Spanish, Italian and German.
74 CHAPTER 5. MODEL APPLICATION
Figure 5.1: Structural formula of one isoprene molecule.
Rubber at that time was called India rubber because it came from Indiadiscovered by Columbus. There were problems though with India rubber: The”Macintouchs” were stiff in cold weather and sticky when it was warm since theraw rubber is non-crosslinked. Something had to be done and Charles Goodyearin 1839 found out what; he invented the process of vulcanization of rubber.Rubber was mixed with sulphur and heated. Through a change in its chemicalstructure (i.e. crosslinking), it is converted to a condition in which the elasticproperties are conferred or re-established or improved. In this manner rubberbecame a dry flexible material largely unaffected by temperature changes in thenormal range [70, 62, 63]
5.2.1.1 Crystallization results for the statistical model
It is well known that natural and synthetic rubbers crystallize upon the ap-plication of stress at room temperature, and this has been studied in both thestretched and the unstretched condition at various temperatures. At low tem-peratures, the effect of strain on crystallization has been studied by Gent [26],Kim and Mandelkern [40], and Stevenson [65, 66]. In general, an applied strainincreases the rate of crystallization.
In this work, it is apparent that the equations obtained permit prediction ofcrystallinity at any strain rate or temperature within the studied range. However,it would also be interesting to use these equations to predict effects of changingthe values of strain rate and temperature beyond the range examined so far, eventhough the validity of the results would be uncertain.
The crystallization during stretching is less than that during an unloadingretraction process. Investigation of the influence of the draw temperature on thecrystallinity development has been performed at two different strain rates, and itis observed that increasing temperature always decreases the crystallinity valuesin both loading stretching and unloading retraction processes. At low strain rate(= 0.039 min−1) this behaviour is confirmed as shown for example in figure5.2. This is so, since the maximum saturated value of crystallinity is inverselytemperature dependent.
5.2. APPLICATION OF THE MODEL 75
0
0,05
0,1
0,15
0,2
0,25
0,3
1 2 3 4 5Strain [1]
Cry
stal
linit
y [
1]T =21°C
T= 50°C
T= 80°C
Figure 5.2: Theoretical results which show the effect of temperature on crys-tallization of polyisoprene rubber at low strain rate of 0.039 min−1 during theloading process.
Also, the crystallization during retraction is different from the crystallizationduring stretching; this is apparent at relatively low temperature (T= 21◦C) infigure 5.3. At moderate temperature (e.g. 50◦C), deviation will be noticed asshown in figure 5.4. However, crystallization deviation in stretching-retractionprocesses is diminished with increasing temperature and at low strain rates. Forexample at T= 80◦C, it is clear that crystallizations are compatible in loading andunloading processes with some deviation at a strain ratio λ1 = 4.75 as shown infigure 5.5. In a retraction process the curve goes back to the origin which indicatesthat melting of crystallites will occur at high temperature. This, the only typeof crystallite which will survive the high temperature is only the mechanically-induced-type (the extended one).
At low strain rate (= 0.039 min−1), the process is almost close to the equilib-rium state, and the deviation of crystallization during stretching and retractiondisappears at high temperatures. According to equation (3.8), the relaxationtime τ plays a vital role on the deviation of crystallization from the equilibriumvalues, while at high temperature, the relaxation time has a rather small value,which enables the process to be close to the equilibrium state, see figures 5.3, 5.4and 5.5.
The effect of strain rate has also been investigated and it was found, that atlow strain rate the crystallinity values are close to the equilibrium state and nolarge hysteresis loops are observed in a loading-unloading process. On the other
76 CHAPTER 5. MODEL APPLICATION
0
0,05
0,1
0,15
0,2
0,25
0,3
0,35
1 2 3 4 5Strain [1]
Cry
stal
linit
y [
1] έ = 0.039 1/min
έ = 2.34 1/min
eqmT= 21°C
Figure 5.3: Theoretical results which show the crystallization of polyisoprenerubber at 21◦C and different strain rates during the loading-unloading processes(arrows indicate load path direction).
hand, at high strain rate the values of crystallinity keep increasing during retrac-tion while the change in crystallinity during stretching is low. It is approved that
0
0,04
0,08
0,12
0,16
0,2
0,24
1 2 3 4 5Strain [1]
Cry
stal
linit
y [
1] έ = 0.039 1/min
έ = 2.34 1/min
eqmT= 50°C
Figure 5.4: Theoretical results which show the crystallization of polyisoprenerubber at 50◦C and different strain rates during the loading-unloading processes(arrows indicate load path direction).
5.2. APPLICATION OF THE MODEL 77
0
0,02
0,04
0,06
0,08
0,1
0,12
0,14
1 2 3 4 5Strain [1]
Cry
stal
linit
y [
1]έ = 0.039 1/min
eqm
T= 80°C
Figure 5.5: Theoretical results which show crystallization of polyisoprene rub-ber at 80◦C and low strain rates during the loading-unloading processes (arrowsindicate load path direction).
the type of crystallites during retraction is different from those in the stretchingprocess. Consequently, a residual crystallinity will exist at the end of the unload-ing retraction process, and this residual amount of crystallinity will cause thethermodynamical irreversibility.
5.2.1.2 Experimental part
Polyisoprene rubber probes (ρ = 0.9392g/cm3) have been made by Dr. Eiseleat Bayer AG, Leverkusen, however, the tensile experiments have been performedat the Bundesanstalt fur Materialprufung BAM-Berlin by Prof. Dr. Rolf Hose-mann. In these experiments, rectangular-shaped polyisoperene rubber sampleswere cut from the sheet. The tensile test device was employed to stretch and re-tract the samples at a certain chosen speed and temperature. Wide Angle X-rayDiffraction (WAXD) patterns were measured in the undeformed state and at theend of the loading state.
5.2.1.3 Uniaxial stress-strain results
For the stress-strain measurements, the sample was stretched and allowed toretract by the same strain rate. Generally, both sequential and simultaneousmeasurements of stress-strain and birefringence were made in order to under-stand and investigate what occurred during stretching loading and retractionunloading processes and at different temperatures [68, 69, 53, 67]. These authorsshowed that the birefringence during retraction is more than that developed dur-
78 CHAPTER 5. MODEL APPLICATION
ing stretching, but the stress during retraction is less than that developed duringstretching. This indicates that a substantial portion of the total orientation ofthe amorphous and crystalline regions is delayed until the retraction stage. Theinduced crystalline order itself can be analyzed directly by Wide Angle X-Raytechniques.
In what follows, we compare our predicted results with the experimental uni-axial extension tests of crosslinked isoprene rubbers. Both the stress-strain curvesand the evolution of the degree of crystallinity are presented at different modelparameters such as temperature and strain rate.
The increase of stress with temperature is due to rubber elasticity. This elasticforce is entirely due to entropic effects, specifically, the tendency of the networkchains to increase their entropy by retracting to more random conformations.This ideal situation would occur when intermolecular interactions do not dependon deformation (one of the major assumptions of molecular theories: absenceof energy effects). As can be seen in the final statistical formula of stress, seeequation (4.90), the force or stress at constant length is then proportional to theabsolute temperature. This effect is clearly shown in figure 5.6a, while stressstrain curves are shown at three different temperatures. As the temperature israised, the Brownian-type wriggling of the polymer is intensified, so that thematerial seeks more vigorously to assume its random high-entropy state. Fromanother view point, once the temperature is raised the crystalline portion of thechain starts to melt, thus the end-to-end distances for the remaining amorphousportions of the chain are increased and, due to that, the entropic effect is increasedas well. Figure 5.6b shows the effect of the temperature on crystallization.
The stress-strain curve shows high upturn with a significant hysteresis. Hys-teresis of rubber is defined as the amount of mechanical free energy dissipated orpart of it converted into heat and other forms of energy during cyclic deforma-tion. So, the rate of heat generation (dissipated deformation energy) is expectedto increase with an increase of the hysteresis loops [35, 36].
Figures 5.7, 5.8, 5.9 show the expected behaviour of the dependence of thehysteresis loops on strain rate and temperature (i.e., the hysteresis decreases withan increase in temperature and with a decrease in strain rate). It is clear, thatthe stress during retraction is much smaller than the stress during the stretch-ing loading process. In the unloading retraction process, the sample is allowedto retract after being stretched to a maximum strain, then the stress decreasesdrastically but the degree of the strain-induced crystallinity is still increasingduring the unloading process. Therefore, the degree of crystallinity during anunloading retraction process is higher than that during loading stretching. Bire-fringence measurements [68, 53, 67, 69] have shown that the birefringence during
5.2. APPLICATION OF THE MODEL 79
retraction is higher than that during stretching. This difference may be due tothe fact that the birefringence represents a measure of total orientation of amor-phous and crystalline chains. Thus, the secondary crystallites with folded-chain
(a)
0
0,5
1
1,5
2
2,5
1 2 3 4 5Strain [1]
Str
ess
σ1
[MP
a]
T=21°C (model)
T=21°C (exp)
T=50°C (model)
T=50°C (exp)
T=80°C (model)
T=80°C (exp)
(b)
0
0,05
0,1
0,15
0,2
0,25
0,3
1 2 3 4 5Strain [1]
Cry
stal
linit
y [
1]
T =21°C
T= 50°C
T= 80°C
Figure 5.6: Temperature effect at 0.039min−1 strain rate on, (a) stress-straincurves for uniaxial loading of polyisoprene rubber (theoretical results are rep-resented by the solid line, while the experimental results by points) and, (b)crystallinity for uniaxial loading of polyisoprene rubber (theoretical results).
80 CHAPTER 5. MODEL APPLICATION
lamellae develop during retraction and cause the stress relaxation. Consequently,the hysteresis of the stress-strain curve is attributed to the formation of the stressinduced crystallites and their transformation.
(a)
0
0,5
1
1,5
2
2,5
3
1 2 3 4 5
Strain [1]
Str
ess
σ1
[MP
a]
έ = 0.039 1/min
έ =2.34 1/min
T= 21°C
(b)
0
0,05
0,1
0,15
0,2
0,25
0,3
0,35
1 2 3 4 5Strain [1]
Cry
stal
linit
y [
1] έ = 0.039 1/min
έ = 2.34 1/min
eqmT= 21°C
Figure 5.7: Effect of strain rates on uniaxial loading-unloading of polyiso-prene rubber for, (a) stress-hysteresis at 21◦C (theoretical results are repre-sented by solid and dashed lines, while the experimental results by points) and,(b)crystallization at 21◦C (arrows indicate load path direction).
5.2. APPLICATION OF THE MODEL 81
Crystallization kinetics in stretching and retraction processes determine theamount of hysteresis of the stress-strain curves. Comparing the total cycles infigures 5.7, 5.8, 5.9 for the low strain rate, we recognise that the hysteresis loops
(a)
0
0,5
1
1,5
2
2,5
3
1 1,5 2 2,5 3 3,5 4 4,5 5
Strain [1]
Str
ess
σ1
[MP
A]
έ = 0.039 1/min
έ = 2.34 1/minT= 50°C
(b)
0
0,04
0,08
0,12
0,16
0,2
0,24
1 2 3 4 5Strain [1]
Cry
stal
linit
y [
1] έ = 0.039 1/min
έ = 2.34 1/min
eqmT= 50°C
Figure 5.8: Effect of strain rates on uniaxial loading-unloading of polyisoprenerubber for, (a) stress-hysteresis at 50◦C (theoretical results are represented bysolid and dashed lines, while the experimental results by points) and, (b) crys-tallization at 50◦C (arrows indicate load path direction).
82 CHAPTER 5. MODEL APPLICATION
(a)
0
0,5
1
1,5
2
2,5
3
1 1,5 2 2,5 3 3,5 4 4,5 5
Strain [1]
Str
ess
σ1
[MP
a] έ = 0.039 1/minT= 80°C
(b)
0
0,02
0,04
0,06
0,08
0,1
0,12
0,14
1 2 3 4 5Strain [1]
Cry
stal
linit
y [
1]
έ = 0.039 1/min
eqm
T= 80°C
Figure 5.9: Effect of strain rate on uniaxial loading-unloading of polyisoprenerubber for, (a) stress-hysteresis at 80◦C (theoretical results are represented bysolid and dashed lines, while the experimental results by points) and, (b) crys-tallization at 80◦C (arrows indicate load path direction).
5.2. APPLICATION OF THE MODEL 83
are getting narrower with increasing temperature, and dissappear at 80◦C. Thisis due to the fact that crystallinity formation decreases with increasing temper-ature. This is also related to the relaxation time which has smaller value whenthe temperature is lower. This explains qualitatively the different widths of thehysteresis loops. The disappearance of the hysteresis loop at 80◦C is due to thefact, that at 80◦C the crystallinity is assumed to be ”momentarily” at its equilib-rium value ξ(P, T = 80◦C,Λ1(t)), so no further crystallization formation occursduring the retraction unloading process.
For high strain rate, it is apparent that the hysteresis loops are always muchbroader than for low strain rate. This phenomenon is interpreted as follows:For high strain rate, the degree of crystallinity is always (for both loading andunloading) far away from its equilibrium value ξ(P, T,Λ1(t)). However, duringloading the degree of crystallinity formation is too small while its formation isrelatively large during the retraction unloading process. Therefore, stress hashigh values during stretching, and in the unloading process it has low values incomparison with the equilibrium values. According to this, two limiting cases arementioned for which no hysteresis loops are formed:
(i) Infinitely quick loading and unloading processes (infinitely large strainrate); in this case the crystallinity cannot follow the changes of the loading andso it will be kept frozen to the starting reference value ξR. As a result, the loadingand unloading stress curves will be the same.
(ii) Infinitely sluggish loading and unloading processes (infinitely small strainrates): in this case the crystallinity will change through a sequence of equilibriumstates ξ = ξ(P, T, λ1(t)).
Pseudo-plastic residual deformation is observed in the unloading retractionprocess as a result of the transformation of crystallites and the formation ofShish Kebab [45] structure, as shown in figure 5.10, due to stress relaxation duringunloading retraction process. This is clear in figures 5.7 and 5.8. At a temperatureof 80◦C, the stress during stretching and that during retraction coincide towardsthe origin, the strain induced crystallites are totally molten or equal to the statecrystallinity of the reference. This can be noticed in figure 5.9.
Two X-ray pictures have been obtained for polyisoprene rubber sample, onein the undeformed state (λ1 = 1) and the other at the maximum elongation ratioof the loading process (λ1 = 5). As shown in figure 5.11 the undeformed statepicture, there appear no oriented crystalline reflection peaks. However, at λ1 = 5,the sample is observed to be well oriented with sharp reflections on the equatorand on the first layer.
84 CHAPTER 5. MODEL APPLICATION
Figure 5.10: Shish-Kebab structure of a polyisoprene rubber sample.
(a) (b)
Figure 5.11: WAXD of polyisoprene rubber at 21◦C and high strain rate 2.34min−1, provided by Prof. T. Alts, for, (a) an undeformed state (λ1 = 1) and, (b)maximum deformation ratio (λ1 = 5).
5.2.1.4 Mooney representation results
The Mooney representations of our stress-strain measured data, will be dis-cussed as follows:
It is clear that plotting σ1(λ1− 1
λ21)against 1
λ1should yield a line of slope 2C2,
and an intercept with value 2(C1 + C2) on the vertical axis where 1λ= 1. Thus
more details about stress coefficients can be obtained using this formula. A largeincrease in modulus at high elongation; is illustrated by figure 4.9 for naturalrubber in the Mooney-Rivlin representation. This increase in modulus is gener-ally observed in crystallizable networks with chemical cross-linking that undergostrain-induced crystallization.
5.2. APPLICATION OF THE MODEL 85
At temperatures of 21◦C and 50◦C and at two different strain rates (0.039, and2.34 min−1), the loading curves for small deformation up to λ = 2.5 are inclined.However, the intersections and inclinations are different. At least, however, theexistence of this inclined line means, that in the loading case the stress coefficientsare constants. This means, since C1 and C2 are functions of ξ and that the degreeof crystallinity does not change during loading in this deformation interval (upto λ = 2.5).
Qualitatively, this effect can be understood as follows: For loading crystallitesof the folded chain type (lamellae) are destroyed at small deformation, and thenmany of the chain segments will become exposed to deformation stress. For largerdeformation, crystallites of extended type are formed. According to Avrami[10, 11, 12] nucleation and growth in uniaxial extension are linear with time. Asdeformation proceeds, a departure from linearity will arise and an upturn of theloading curve will occur as a result of deformation-induced crystallization.
To validate this view, Kuhn’s model is included in our statistical model as aspecial case, if we assume, that no state quantity depends on crystallinity and.If possibly existing crystallinity ξo does not change at all, then linear horizontallines will be achieved as shown in figures 5.12, 5.13 and represented by dashedline. This can be compared to our model where formation of crystallinity withdeformation is included. Thus, inclined lines will be achieved from our statisticalmodel for the Mooney stress. For unloading, hysteresis is observed, due to furtherformation and transformation of crystallinity as it has been found and discussedfor stress-strain curves. Hysteresis decreases with an increase of temperature,and with the decrease in strain rate as shown in figures 5.12, 5.13.
At high temperature (i.e. 80◦C), loading and unloading curves are compatibleand only a very small hysteresis at the beginning of unloading is observed, asshown in figure 5.14.
86 CHAPTER 5. MODEL APPLICATION
(a)
0
0,1
0,2
0,3
0,4
0,5
0,2 0,3 0,4 0,5 0,6 0,7 0,8 0,9 1
Mo
on
ey s
tres
s [M
Pa]
1/λ
21°C
έ = 0.039 1/min
Kuhn model
with � =
� �
(b)
0
0,1
0,2
0,3
0,4
0,5
0,2 0,3 0,4 0,5 0,6 0,7 0,8 0,9 1
Mo
on
ey s
tres
s [
MP
a]
1/λ [1]
21°C
έ=2.34 1/min
Kuhn model
with � = � �
Figure 5.12: Mooney-representation for uniaxial loading-unloading of polyiso-prene rubber at 21◦C (theoretical results are represented by solid the line, theexperimental results by points , while the dashed line is Kuhn’s model when nochange in crystallinity is assumed in our statistical model) for, (a) low strain rate= 0.039 (min−1) and, (b) high strain rate = 2.34 (min−1).
5.2. APPLICATION OF THE MODEL 87
(a)
0
0,1
0,2
0,3
0,4
0,5
0,2 0,3 0,4 0,5 0,6 0,7 0,8 0,9 1
Mo
on
ey s
tres
s [
MP
a]
1/λ
50°C
έ=0.039 1/min
Kuhn model
with � = � �
(b)
0
0,1
0,2
0,3
0,4
0,5
0,6
0,2 0,3 0,4 0,5 0,6 0,7 0,8 0,9 1
Mo
on
ey s
tres
s [M
Pa]
1/λ
50°C
έ=2.34 1/min
Kuhn model
with � = � �
Figure 5.13: Mooney-representation for uniaxial loading-unloading of polyiso-prene rubber at 50◦C (theoretical results are represented by the solid line, theexperimental results by points , while the dashed line is Kuhn’s model when nochange in crystallinity is assumed in our statistical model) for, (a) low strain rate= 0.039 (min−1) and, (b) high strain rate = 2.34 (min−1).
88 CHAPTER 5. MODEL APPLICATION
0
0,1
0,2
0,3
0,4
0,5
0,6
0,2 0,3 0,4 0,5 0,6 0,7 0,8 0,9 1
Mo
on
ey s
tres
s [
MP
a]
1/λ
80°C
έ=0.039 1/min
Kuhn model
with � = � �
Figure 5.14: Mooney-representation for uniaxial loading-unloading of polyiso-prene rubber at 80◦C (theoretical results are represented by the solid line, theexperimental results by points , while the dashed line is Kuhn’s model when nochange in crystallinity is assumed in our statistical model) for low strain rate =0.039 (min−1).
5.2.1.5 Volume change
According to equation (3.6), for a semi-crystalline polymer, the equilibriumvolume increases first with deformation since a destruction of lamellae (spherulite)occurs initially and a decrease in volume is obtained for large deformation due tothe formation of extended crystallites or orientation of both amorphous chainsand destroyed lamellae parts. A linear relationship between volume change andstrain was found up to large extension ratios. On the basis of an affine deforma-tion, one calculates a dependence which is proportional to λ− 1 [25, 16, 30].
As shown in figure 5.15 strain rates have a drastic impact on volume change atcertain temperatures. In our statistical theory, according to equation (3.6), a goodapproximation is achieved to predict the change of volume due to deformation-induced crystallization.
5.2. APPLICATION OF THE MODEL 89
(a)
0
0,1
0,2
0,3
0,4
0,5
1 2 3 4 5
Strain [1]
∆ V
/Vo [
1]
έ=0.039 1/min�=2.34 1/min
T = 21°C
(b)
0
0,1
0,2
0,3
1 2 3 4 5
Strain [1]
∆ V
/Vo [
1]
έ= 0.039 1/min�= 2.34 1/min
T = 50°C
(c)
0
0,05
0,1
0,15
0,2
1 2 3 4 5
Strain [1]
∆ V
/Vo [
1]
έ= 0.039 1/min
T = 80°C
Figure 5.15: Change of volume, model results, at different strain rates for, (a)21◦C, (b) 50◦C and, (c) 80◦C.
90 CHAPTER 5. MODEL APPLICATION
5.2.2 Polyolefin thermoplastic elastomers
Thermoplastic elastomers differ from the usual cross-linked elastomers in sofar as the cross-links are not covalent bonds but physical links, e.g. consistingof crystallized chain segments. These can be molten by heating, thus allowingthermoplastic processing [18].
The two polyolefin elastomers, that have been used in this study, are copoly-mers of ethylene-butene with two different degrees of crystallinity as shown intable 5.7.
Table 5.7: Physical and chemical properties of the thermoplastic ethylene-butenecopolymerCopolymer type Density [g/cm3] % Total Crystallinity Tm [◦C] Tg [◦C]
ENX-7256 0.885 21.5 70 -48ENX-7086 0.902 32.4 94 -39
Ethylene-butene copolymers have the chemical structure as shown in figure5.16. ENX-7256 has a unique broader molecular weight distribution with higherbranching levels that offers excellent clarity, processing and performance in foamsand extrusion applications such as tubing, profiles, wire and cable insulations.ENX-7086 has much higher levels of long chain branching than other commer-cially available polyolefin elastomers. It is suited for blow molding, extrusionand thermoforming applications where high level of shear thinning and high meltstrength may be required.
n
Figure 5.16: Chemical structure of ethylene-butene copolymer.
5.2.2.1 Crystallization results for the model
This difference in crystallinities may be recalled from the copolymer crystal-lization theories that the co-units present in a copolymer may either be completelyrejected from the crystal (exclusion) or uniformly included as an equilibrium re-quirement (inclusion) [21, 23, 59, 60, 2, 3].
5.2. APPLICATION OF THE MODEL 91
Flory’s prediction is that all branches longer than methyl are excluded fromthe crystal lattice [33, 4]. Thus, ethyl and butyl side chains are excluded fromthe crystal lattice. Therefore, the morphology in more branched copolymers mayinvolve fringed-micellelike crystals.
Deformation-induced crystallization in polyethylene-polybutene copolymersdepends on temperature and strain rate in a similar way as does polyisoprenerubber, although the molecular rearrangements taking place are different. In theearly stages of drawing an unoriented crystalline polymer, spherulites become
(a)
0
0,1
0,2
0,3
0,4
0,5
1 2 3 4 5 6 7Strain [1]
Cry
stal
linit
y [1
]
έ = 0.09 1/min
έ = 5.4 1/min
ENX-7256T= 23 °C
(b)
0
0,1
0,2
0,3
0,4
0,5
1 2 3 4 5 6 7
Strain [1]
Cry
stal
linit
y [1
]
έ= 0.09 1/min
έ= 5.4 1/min
ENX-7256T= 50 °C
Figure 5.17: Theoretical crystallization of ENX-7256 at different strain rates fortwo temperatures of, (a) at 23◦C, and (b) at 50◦C.
92 CHAPTER 5. MODEL APPLICATION
elongated in the draw direction. Then, chain slipping occurs within the lamellae(chain-folded crystals) and the lamellae break up into small crystallites connectedto each other by uncrystallized tie molecules.[58].
Due to this fact, crystallization is kept constant up to λ1 = 2 since breakingthe lamellae enhances the reorientation of these small broken crystallites in thedrawing direction. This is obviously shown in figures 5.17 and 5.18 during theloading stretching process.
(a)
0
0,1
0,2
0,3
0,4
0,5
0,6
1 2 3 4 5 6 7Strain [1]
Cry
stal
linit
y [1
]
έ = 0.09 1/min
έ = 5.4 1/minENX-7086
23°C
(b)
0
0,1
0,2
0,3
0,4
0,5
1 2 3 4 5 6 7Strain [1]
Cry
stal
linit
y [
1] έ = 5.4 1/min
έ = 0.09 1/min
ENX-708650°C
Figure 5.18: Theoretical crystallization of ENX-7086 at different strain rates fortwo temperatures of, (a) at 23◦C, and (b) at 50◦C.
5.2. APPLICATION OF THE MODEL 93
The same figures show the effect of strain rate on the evolution of crystallinityas a function of the deformation. In fact, it is clear that both materials do notshow drastic changes of crystallinity caused by changing strain rates at a certaintemperature during the loading process. This is clearly shown in figures 5.17 and5.18 for both copolymers.
The effect of temperature on crystallization is an important factor. An in-crease in temperature accelerates thermally activated processes and reduces re-laxation times. Consequently, the hysteresis between the loading and unloadingprocess is reduced.
5.2.2.2 Experimental part
We are indebted to Rieter Automative Germany GmbH for providing us withethylene-butene copolymer materials. Also another acknowledgment is to Ger-man Polymer Institute DKI -Darmstadt for their highly appreciated cooperationand help with the preparations of samples and running of the tensile loading-unloading experiments.
For the preparation for the experiments, two ethylene−butene copolymers(ENX-7086, ENX-7256) were dried under vacuum at 80◦C, extruded by twin mi-croextruder, and pressed to form a thin sheet by the following sequence: heating1 min at 1 bar and 150◦C, pressing 2 min at 36 bar and 150◦C , and cooling2 min at 36 bar and 23◦C. Then the samples were cut into a certain form (1.5mm thickness, 27.7 mm length, and 4 mm width) from the pressed sheet usinga standard cutting machine. A tensile machine (Zwick-020TH2A) was equippedwith an environmental chamber that was used for performing the loading andunloading tests. To correct for shrinkage at high temperatures (50◦C), samplelength correction was used for deformation of the samples under constant tem-perature and humidity. Each sample was drawn up to λ1 = 7 at two differenttemperatures, 23◦C and 50◦C, and two different deformation speeds, 2.5 mm/minand 150 mm/min.
5.2.2.3 Uniaxial stress-strain results
Since these ethylene-butene copolymers have a degree of crystallinity in theundeformed state of the order of 20-30%, deviation from rubbery behaviour is wellexpected at least in the small deformation region. Copolymer preparations witha density of less than 0.9 gcm−3 show increasingly fringed micelles as the dom-inant but not exclusive crystal morphology and exhibit mechanical and thermalproperties that are not found in standard polyethylene [13, 14].
Crystallization of copolymers is predominately by branching statistics. How-ever, in homopolymers it is largely influenced by the chain length and its distri-
94 CHAPTER 5. MODEL APPLICATION
bution, the extent of entanglement of chains in the melt and the undercooling. Itwas observed that the lamellar thickness at a selected crystallization temperatureincreases linearly with decreasing comonomer content (this is fully discussed inchapter two).
So far we considered the stress-strain response of amorphous chains (with lowdegree of crystallinity at the origin) that crystallize in the course of deformation.Stress-induced orientation reduces the energy barrier between the amorphous andcrystalline state, permitting crystallization at temperatures where none wouldoccur in the unoriented state.
Induction of crystallinity levels in the undrawn polymer can result in a brittlebehaviour that is difficult to draw. In general, increasing crystallinity in anyunoriented state increases the stress required for deformation, and shifts thestress-strain response towards brittle deformation.
Some copolymers with high levels of unoriented crystallinity can, however,be readily drawn. An unoriented, semicrystalline copolymer generally consists oflamellae structures. Chains fold back at the surface of each lamella.
The stress-strain response of a semicrystalline chain depends on temperatureand strain rate in a similar way as do amorphous chains e.g. in polyisoprenerubber (negligible degree of crystallinity at the reference state). In the early stagesof drawing an unoriented semi-crystallized chain, stress concentrates initially onspherulite which becomes elongated in the draw direction [32, 15], and in theregion of λ = 2− 2.5; chain tilting and slipping occur within the lamellae of thechain-folded crystals.
Necks begin to form in regions of stress concentration or in a region wherethere are fewer molecular entanglement. This leads to dramatic local orientationof the amorphous chain, and dramatic local deformation of the spherulites andlamellae in the crystallized portion of the chain.
Eventually, the plastic deformation of the spherulites induces the breakingof the lamellae into small crystallites connected to each other by conformationaltie segments. Spherulite deformation under uniaxial tension has been studied.Results indicate that the first deformation events occur near the center [73, 74].However, other researches showed, that the deformation starts from the equatorialregime and proceeds towards the polar regime of the spherulites [61].
Although stress-strain response is temperature and strain rate dependent,different results can be identified theoretically and experimentally for the twomaterials based on their difference in the degree of crystallinity in the undeformed
5.2. APPLICATION OF THE MODEL 95
(a)
0
2
4
6
8
10
12
14
16
18
1 2 3 4 5 6 7
Strain [1]
Str
ess
σ1
[MP
a]
ENX-7256
ENX-7086
T= 23°C
έ = 0.09 1/min
(b)
0
2
4
6
8
10
12
1 2 3 4 5 6 7Strain [1]
Str
esss
σ1
[MP
a]
ENX-7256
ENX-7086
T= 50°C
έ = 0.09 1/min
Figure 5.19: Effect of temperature on stress-strain loading curves at 0.09 (min−1)strain rate for, (a) at 23◦C and, (b) at 50◦C. (Theoretical results are representedby the solid line, while the experimental results by points).
96 CHAPTER 5. MODEL APPLICATION
origin state.
ENX-7086 has a total degree of crystallinity at the reference state of ξR =0.332, while ENX-7256 has ξR = 0.221. As a result one observes within a certaintemperature range and regardless of the range of strain rate: The higher thereference crystallinity is the higher is also the mechanical energy required tobreak up and reorient the crystals. This is clear from figure 5.19; ENX-7086(ξR = 0.332) has higher stress values compared to ENX-7256 (ξR = 0.221).
Since the reference crystallinity decreases with temperature, so the referencecrystallinity equally decreases at high temperatures (i.e. 50◦C) and due to that,the stress required initially will be less than that at room temperature (i.e. 23◦C).However, the number of segments that are sitting in the crystalline lamellae statewill be less and the required mechanical energy to break up the lamellae willdecrease. This is obviously shown in figure 5.20.
The effect of the strain rate is not so conspicuous as it is in polyisoprene rub-ber. For example, at a certain temperature, increasing the strain rate increasesthe initial stress required to deform the lamellae domain. However a slight dif-ference in stress value is found in the deformation range λ = 2 − 7 as shown infigure 5.21.
For the hysteresis, different loading-unloading processes have been performedto investigate the effect of temperature and strain rate on hysteresis.
As expected, the hysteresis decreases with increasing temperature for bothmaterials, ENX-7086 and ENX-7256. It is found that further crystallization for-mation proceeds during undeforming causing pseudo plastic residual deformation(strain residuals) as shown in figure 5.22.
The effect of strain rates on the hysteresis is shown for both materials in figure5.22. Increasing the strain rate will increase the hysteresis as well.
Three ENX-7256 (ξR = 0.221) samples were deformed up to three maximumdifferent deformation ratios (λf = 5, 6, 7) after which they were unloaded. Thiswas done to explain the behaviour of the material. As shown in figure 5.23 thethree loading curves are compatible with certain ranges while each sample has acertain different residual strain after completing the unloading process. Residualstrains for these, are caused by different crystallizations during unloading.
Doubts that hysteresis might have occurred due to some breakage and de-struction of the sample’s structure can be removed once the samples with certainresidual lengths are heated. Then a full shape recovery is achieved for all samples(the sample regains its original dimensions as in the reference state).
5.2. APPLICATION OF THE MODEL 97
(a)
0
2
4
6
8
10
12
14
16
18
1 2 3 4 5 6 7Strain [1]
Str
ess
σ1
[MP
a]
21°C
50°C
ENX-7086
έ = 5.4 1/min
(b)
0
1
2
3
4
5
6
7
8
9
1 2 3 4 5 6 7Strain [1]
Str
ess
σ1
[MP
a] 21°C
50°C
ENX-7256
έ = 5.4 1/min
Figure 5.20: Stress-strain curves at 5.4 (min−1) strain rates for, (a) ENX-7086and, (b) ENX-7256 (theoretical results are represented by the solid line, whilethe experimental results by points).
98 CHAPTER 5. MODEL APPLICATION
(a)
0
3
6
9
12
15
18
1 2 3 4 5 6 7Strain [1]
Str
ess
σ1
[MP
a] � = 0.09 1/min
� = 5.4 1/min
ENX-7086 T= 23°C
(b)
0
1
2
3
4
5
6
7
8
1 2 3 4 5 6 7
Strain [1]
Str
ess
σ1
[MP
a]
� = 0.09 1/min
� = 5.4 1/min
ENX-7256 T= 23°C
Figure 5.21: Effect of strain rate on stress-strain curves at 23◦C for, (a) ENX-7086and, (b) ENX-7256 (theoretical results are represented by solid and dashed lines,while the experimental results by points. Arrows indicate load path direction).
5.2. APPLICATION OF THE MODEL 99
(a)
0
2
4
6
8
10
12
1 2 3 4 5 6 7
Strain [1]
Str
ess
σ1
[MP
a]
� = 0.09 1/min
� = 5.4 1/min
ENX-7086 T= 50°C
(b)
0
0,5
1
1,5
2
2,5
3
3,5
4
1 2 3 4 5 6 7
Strain [1]
Str
ess
σ1
[MP
a]
� = 0.09 1/min
� = 5.4 1/min
ENX-7256 T= 50°C
Figure 5.22: Effect of strain rate on stress-strain curves at 50◦C for, (a) forENX-7086 and, (b) for ENX-7256 (theoretical results are represented by solidand dashed lines, while the experimental results by points. Arrows indicate loadpath direction).
100 CHAPTER 5. MODEL APPLICATION
(a)
0
1
2
3
4
5
6
7
8
1 2 3 4 5 6 7Strain [1]
Str
ess
[MP
a]
ENX-7256T= 23°C
έ= 5.4 1/min
(b)
0,15
0,2
0,25
0,3
0,35
0,4
0,45
0,5
1 2 3 4 5 6 7
Strain [1]
Cry
stal
linit
y [
1]
ENX-7256T= 23°C
έ= 5.4 1/min
Figure 5.23: Three deformation cycles at three maximum strains for ENX-7256at 23◦C and 5.4 min−1 strain rate: (a) stress-strain curves (b) crystallinity-straincurves (theoretical results are represented by solid and dashed lines, while theexperimental results by points. Arrows indicate load path direction).
5.2. APPLICATION OF THE MODEL 101
5.2.2.4 Mooney representations
For crystallizable networks, there is frequently a downturn in the reducedstress prior to its upturn [20, 50].
Mooney-Rivlin representations of the stress-strain curves do not show theupturn in the isotherm up to this value of the deformation ratio, λ1 = 7. However,the initiation of strain-induced crystallization is evidenced by the departure ofthe isotherm from linearity.
We believe if the sample had been deformed up to λ1 = 9 − 10, then anupturn in the isotherm would be obtained. The following figures show Mooney-Rivlin representations for crystallizable chains of these two copolymer elastomersENX-7086 and ENX-7256. This is shown in figures 5.24, 5.25, 5.26 and 5.27.
102 CHAPTER 5. MODEL APPLICATION
(a)
0
1
2
3
4
5
6
0,1 0,3 0,5 0,7 0,9
1/λ [1]
Mo
on
ey S
tres
s [
MP
a]
ENX-7256T= 23°C�
= 0.09 1/min
Kuhn model ( � = ��� )
(b)
0
1
2
3
4
5
6
7
0,1 0,3 0,5 0,7 0,9
1/λ [1]
Mo
on
ey S
tres
s [
MP
a]
ENX-7256T= 23°C�
= 5.4 1/min
Kuhn model ( � = ��� )
Figure 5.24: Mooney-representation of stress-strain for ENX-7256 at 23◦C for, (a)low strain rate = 0.09 (min−1) and, (b) high strain rate = 5.4 (min−1) (theoreticalresults are represented by the solid line, the experimental results by points , whilethe dashed line is Kuhn’s model when no change in crystallinity is assumed inour statistical model. Arrows indicate load path direction).
5.2. APPLICATION OF THE MODEL 103
(a)
0
0,5
1
1,5
2
2,5
3
0,1 0,3 0,5 0,7 0,9
1/λ [1]
Mo
on
ey S
tres
s [
MP
a] ENX-7256T= 50°C�
= 0.09 1/min
Kuhn model ( � = ��� )
(b)
0
0,5
1
1,5
2
2,5
3
0,1 0,3 0,5 0,7 0,9
1/λ [1]
Mo
on
ey S
tres
s [
MP
a]
ENX-7256T= 50°C�
= 5.4 1/min
Kuhn model ( � = ��� )
Figure 5.25: Mooney-representation stress-strain for ENX-7256 at 50◦C for, (a)low strain rate = 0.09 (min−1) and, (b) high strain rate = 5.4 (min−1) (theoreticalresults are represented by the solid line, the experimental results by points , whilethe dashed line is Kuhn’s model when no change in crystallinity is assumed inour statistical mode. Arrows indicate load path directionl).
104 CHAPTER 5. MODEL APPLICATION
(a)
0
2
4
6
8
0,1 0,3 0,5 0,7 0,9
1/λ [1]
Mo
on
ey S
tres
s [
MP
a]
ENX-7086T=23°C
έ = 0.09 1/min
Kuhn model ( � = ��� )
(b)
0
2
4
6
8
10
0,1 0,3 0,5 0,7 0,9
1/λ [1]
Mo
on
ey S
tres
s [
MP
a]
ENX-7086T=23°C
έ =5.4 1/min
Kuhn model ( � = ��� )
Figure 5.26: Mooney-representation of stress-strain for ENX-7086 at 23◦C for, (a)low strain rate = 0.09 (min−1) and, (b) high strain rate = 5.4 (min−1) (theoreticalresults are represented by the solid line, the experimental results by points , whilethe dashed line is Kuhn’s model when no change in crystallinity is assumed inour statistical model. Arrows indicate load path direction).
5.2. APPLICATION OF THE MODEL 105
(a)
0
2
4
6
8
0,1 0,3 0,5 0,7 0,9
1/ λ [1]
Mo
on
ey S
tres
s [
MP
a]
ENX-7086T=50°C
έ =0.09 1/min
Kuhn model ( � = ��� )
(b)
0
2
4
6
8
0,1 0,3 0,5 0,7 0,9
1/λ [1]
Mo
on
ey S
tres
s [
MP
a]
Kuhn model ( � = ��� )
ENX-7086T=50°C
έ =5.4 1/min
Figure 5.27: Mooney-representation of stress-strain for ENX-7086 at 50◦C for, (a)low strain rate = 0.09 (min−1) and, (b) high strain rate = 5.4 (min−1) (theoreticalresults are represented by the solid line, the experimental results by points , whilethe dashed line is Kuhn’s model when no change in crystallinity is assumed inour statistical model. Arrows indicate load path direction).
106 CHAPTER 5. MODEL APPLICATION
Chapter 6
Conclusions and
Recommendations
6.1 Conclusions
An overview about the thermodynamics of rubber-like high polymers is ob-tained and simplified by employing some approximations and internal constraints.Uniaxial extension at constant temperature and constant external pressure isdiscussed in the thermodynamic constitutive theory. Continuum theory is inad-equate to explicitly show the dependence of stress coefficients on the degree ofcrystallinity.
The crystallization formulation, which is based on irreversible thermodynam-ics, is adopted to describe the crystallization induced by deformation at differentranges of the temperature and strain rates and for uniaxial loading-unloading pro-cesses. Relaxation behaviour and its effect on crystallization kinetics has beenexplained in the context of the formulation of limiting cases.
The crystallization during stretching is less than that during unloading re-traction processes. The important portion of crystallites, that are induced bydeformation, are extended-chain crystallites that develop during the loading pro-cess, while during unloading other secondary crystallite types (folded-chain crys-tallites, shish-kebab structure) are formed.
Strain induced crystallization has been successfully modeled by the statisticalapproach in which the shortcomings of Flory’s theory have been corrected. Amodified Gaussian distribution is employed for chains of finite lengths to describethe end-to-end vector distribution function. The contribution of the chain tocrystallinity based on affine deformation of the network of finite chain lengths
107
108 CHAPTER 6. CONCLUSIONS AND RECOMMENDATIONS
has been fully described. The dependence of stress coefficients Cα(α = 1, 2)on the degree of crystallinity has been derived within the statistical framework.A good approximation is achieved to predict the change of volume due to thedeformation-induced crystallization phenomena.
Stress-strain curves and their Mooney representations are introduced in ourtheory and compared to the experimental data. Stress-strain curves show highupturn with significant hysteresis. Hysteresis loops are attributed to the forma-tion of deformation induced crystallites and their transformation.
Pseudo-plastic residual deformation is observed in the unloading retractionprocess as a result of the formation of the shish-kebab structures due to stressrelaxation. This is obvious at high strain rates and low temperature (i.e. abovethe glass transition temperature). Hysteresis loops and inelastic deformation donot show up at infinitely quick or infinitely sluggish loading-unloading processes.
The upturn in the Mooney representation curves at high deformation ratiosis clearly shown in polyisoprene rubber experiments. However, for ethylene-butene copolymer experiments, the initiation of strain induced crystallization isevidenced by departure of the isotherm from linearity. The modeled results arecompared to experiments and fair agreement is found.
Ethylene-butene copolymer behaviour deviates from rubbery behaviour atleast in the small deformation region, since they have a certain degree of crys-tallinity in the undeformed state. Although their stress-strain response is tem-perature and strain dependent in a similar way as amorphous chains e.g. polyiso-prene rubber, different results have been identified theoretically and experimen-tally based on their difference in the degree of crystallinity in the undeformedoriginal state.
6.2 Recommendations
From the theoretical and experimental works undertaken in this study, somerecommendations can be made. It is imperative to do the further:
Our model parameters, of which some were obtained by different curve-fittingtechniques, are by no means unique. Different fitting techniques will lead toequally valid results.
Extension of the theory for biaxial and triaxial stress are required to meetsome industrial processes such as blow molding. This will be a complicatedmission, but with the recent numerical softwares nothing is impossible. All-sidecompression can be included.
6.2. RECOMMENDATIONS 109
In-situ study of deformation-induced crystallization inside the polymer struc-ture with enlargement of the temperature range and extension of the strain rateranges will allow to meet the conditions for achieving tougher fibers in the fiberspinning process.
Our statistical model allows further to predict the heat effect for loading ofrubbery samples. Deformation experiments should be performed inside a de-formation calorimeter to study heat effects and the crystalline binding energy.Besides loading also unloading should be studied. [6, 7, 17, 19]
110 CHAPTER 6. CONCLUSIONS AND RECOMMENDATIONS
Appendix A
Table A.1: Parameter a: Values of adjustable constants during unloading processfor polyisoprene rubber:T[◦C] ε [min−1] ao a1 a2 a3 a4 a5
21 0.039 5.6740 -1.9490 0.4850 -0.0412 -2.4574 8.473×10−1321 2.340 -3.5450 0.9460 -0.2490 0.0263 2.1090 -1.623×10−1250 0.039 3.96843 -1.0537 0.2007 - 0.0119 2.6702 -3.905×10−1350 2.340 -3.4050 0.6340 -0.1602 0.0173 2.3570 -1.670×10−1280 0.039 -0.6490 0.3308 -0.077 0.0069 0.5020 -6.283×10−14
Table A.2: Parameter a: Values of adjustable constants during unloading processfor ENX-7256 elastomer:T [◦C] ε [min−1] ao a1 a2 a3 a4 a5
21 0.09 1.4790 -0.5740 0.1220 -0.0077 -0.3370 -1.011×10−2221 5.40 -1.0872 -0.0463 0.0137 -0.0002 1.2130 -1.011×10−2250 0.09 1.9815 -0.7783 0.1638 -0.0109 -0.3180 -8.920×10−2350 5.40 6.4008 -1.725 0.3287 -0.0208 -2.6570 -1.412×10−22
Table A.3: Parameter a: Values of adjustable constants during unloading processfor ENX-7086 elastomer:T [◦C] ε [min−1] ao a1 a2 a3 a4 a5
21 0.039 0.4650 -0.0598 -0.0063 0.0020 0.2026 -2.700×10−2221 2.340 -0.7140 0.1339 -0.0446 0.0050 0.9742 -3.350×10−2250 0.039 3.0470 -0.8500 0.17210 -0.0100 -0.9580 -2.440×10−2250 2.340 6.2010 -1.7700 0.3640 -0.0230 -2.5100 -2.150×10−22
111
112 APPENDIX A.
Appendix B
Table B.1: Nforce: Values of adjustable constants during loading process forpolyisoprene rubber:T [◦C] ε [min−1] bo b1 b2 b3 b4 b5
21 0.039 -13.1890 87.3690 -41.5650 8.3930 -0.6110 04.4121 2.340 10.5900 49.9100 -22.1000 4.2480 -0.2980 -99.0050 0.039 26.2251 47.3980 25.9200 5.6220 -0.4260 -545.3250 2.340 54.0045 -02.8210 00.9250 -0.0720 -0.0030 -485.0980 0.039 27.1387 32.131 -13.492 2.3590 -0.1490 -959.78
Table B.2: Nforce: Values of adjustable constants during loading process forENX−7256 elastomer:T [◦C] ε [min−1] bo b1 b2 b3 b4 b5
21 0.09 -03.8753 07.6210 0.4370 0.256 -0.041 -013.73021 5.40 5.69468 -03.0910 4.0500 -0.2590 -0.0130 -098.53150 0.09 32.5786 -13.1900 6.9700 -0.8330 0.0260 -533.66050 5.40 -07.4905 22.867 -5.7880 1.1470 -0.0840 -162.590
Table B.3: Nforce: Values of adjustable constants during loading process forENX−7086 elastomer:T [◦C] ε [min−1] bo b1 b2 b3 b4 b5
21 0.09 -16.1380 17.2300 -2.7958 0.5860 -0.0451 167.9921 5.40 -13.15 14.817 -2.2043 0.5017 -0.0394 103.2450 0.09 -07.536 10.643 -0.0554 0.0149 -0.0114 095.6350 5.40 -06.543 08.7738 0.3945 0.0862 -0.0183 039.98
113
114 APPENDIX B.
Bibliography
[1] Abramowitz, U.; Stegun, I. A. Handbook of Mathematical functions, DoverPubl:New York,1972.
[2] Alamo, R.; Domzy, R.; Mandelkern, L. J. Phys. Chem.1984,88, 6587.
[3] Alamo, R.; Mandelkern, L. Macromolecules 1989,22, 1273.
[4] Alamo, R.; Mandelkern, L. Thermochim. Acta.1994,238, 155.
[5] Alts, T. Thermodynamik elastischer Korper mit thermo-kinematischenZwangsbedingungen-fadenverstarkte Materialien -, Universitatsbibliothekder TUB-Abt.Publ.:Berlin,1979.
[6] Alts, T. Progr. Colloid and Polymer Sci. 1979,66,367.
[7] Alts, T. Progr. Colloid and Polymer Sci. 1980,67, 183.
[8] Alts, T. Arch. Mech. 1981,33,4, 523.
[9] Anthony, R.L.; Caston, R.H.; Guth E. J. Phys. Chem.1942,46, 826.
[10] Avrami, M. J. Chem. Phys.1939,7, 1103.
[11] Avrami, M. J. Chem. Phys.1940,8, 212.
[12] Avrami, M. J. Chem. Phys.1941,9, 177.
[13] Bensason, S.; Minik, J.; Moet, A.; Chum, S.; Hiltner, A.; Baer, E. J:Applied Polym. Sci.1996,34, 1301.
[14] Bensason, S.; Stepanov, S.; Chum, S.; Hiltner, A.; Baer E. Macromolecules1997,30, 2436.
[15] Branov, V. G.; Gasparyan, K. A. J. Polym. Sci. A-2 1970,8, 1015.
[16] Christensen, R. G.; Hoeve, A. J. J. Polym. Sci.1970,8, 1503.
115
116 BIBLIOGRAPHY
[17] Dick, W.; Muller, F. H. Kolloid-Z 1960,172, 1.
[18] Ehrenstein, W. G. Polymeric Materials Structure-Properties-Applications,Carl Hanser Verlag:Munich,2001.
[19] Eisele, U. Kautschuk und Gummi Kunstoffe 1972,25, 347.
[20] Erman, B.; Mark, E. J. Structures and Properties of Rubberlike Networks ,Oxford University Press, Inc.:New York, 1997.
[21] Flory, P. J. J. Chem. Phys.1947,15, 397.
[22] Flory, P. J.Principles of Polymer Chemistry, Cornell University Press:NewYork,,1953.
[23] Flory, P. J. Trans. Faraday Soc.1955,51, 848.
[24] Flory, P. J. J. Am. Chem. Soc.1962,17, 3,223.
[25] Flory, P. J. Trans. Faraday Soc.1961,57, 829.
[26] Gent, A. N. Trans. Faraday Soc.1954,50, 521.
[27] Gent, A. N. J. Polym. Sci. A1966,4, 447
[28] Gough, J. Mem. Lit. Philos. London 1805,1, 288.
[29] Goritz, D.; Kiss, M. Rubb. Chem. Tech.1973,251, 892.
[30] Goritz, D.; Kiss, M. Rubb. Chem. Tech.1986,59, 40.
[31] Goritz, D. Colloid and Polym. Sci.1982,260, 193.
[32] Hay, I. L.; Keller, A. Kolloid Z 1965,204, 43.
[33] Hoffman, J. D.; Weeks, J. J. J. Chem. Phys.1965,42, 4301.
[34] Joule, J. P. Philos. Trans. Roy. Soc. London 1859,91, 149.
[35] Kar, K. K.; Bhowmick, A. K. J. Applied Polym. Sci.1997,64, 1541.
[36] Kar, K. K.; Bhowmick, A. K. J. Applied Polym. Sci.1997,65, 1429.
[37] Keller, A. Phil. Mag.1957,2, 1171.
[38] Keller, A. Rep. Prog. Phys.1968,31, 623.
[39] Keller, A.; Machin, M. J. J. Macromol. Sci. Phys.1967,1, 41.
[40] Kim, H.; Mandelkern, L. J. Polym. Sci.1968,A2, 181.
BIBLIOGRAPHY 117
[41] Kuhn, W. Kolloid-Z 1936,76, 258.
[42] Kuhn, W. J. Polym. Sci.1946,1, 380.
[43] Liu, I-Shi Arch. Rat. Mech. Anal.1972,46, 131.
[44] Lohmander, B.; Rittsten, U. S. Kungl. Fysiogr. Saallsk. i Lund Forh1958,28, 45.
[45] Luch, D.; Yeh, G.S. J. Appl. Phys.1972,43, 4326.
[46] Luch, D.; Yeh, G.S. J. Macromol. Sci. Phys.1973,B7, 121.
[47] Mandelkern, J. Crystallization of Polymers, McGraw Hill Book Com-pany:New York, ,1964.
[48] Mandelkern, J. An Introduction to Macromolecules, Springer-Verlag:NewYork, 1983.
[49] Mandelkern, J. The Crystalline State in Physical Properties of Polymers,Ed.,J.E. Mark, ACS Washington D.C.,1984.
[50] Mark, E. J.; Erman, B. Rubberlike Elasticity: A molecular Primer ,JohnWiley Sons, Inc.:Canada, 1988.
[51] Meyer, H. K.; Ferri, C. Helv. Chim. Acta 1935,18, 570.
[52] Mooney, M. J. Appl. Phys.1940,11, 582.
[53] Mukherjee, D. P. Rubber Chem. Technol.1974,47, 1234.
[54] Muller, I. Thermodynamik-Grundlagen der Material-Theorie, Dusseldorf:Bertelsmann Universitatverlag,1973.
[55] Rivlin, R. S. Philos. Trans. Roy. Soc.1949,A242, 173.
[56] Rivlin, R. S.; Saunders, D. W. Philos. Trans. Roy. Soc. London 1951,A243,251.
[57] Rosser, J. B. Theory and Application of∫ z
0exp (−x2) dx and
∫ z
0exp (−P 2 Y 2)dy
∫ y
0exp (x2) dx , Mapleton House, Brooklyn:N.Y.,
1948.
[58] Salem D.R. Structure Formation in Polymeric Fibers, Carl Hanser Verlag,Munich.,2001.
[59] Sanchez, I. C.M; Eby, R. K. Macromolecules 1975,8, 638.
118 BIBLIOGRAPHY
[60] Sanchez, I. C.; Eby, R. K. J. Res. Natl. Bur. Std-A Phys. Chem.1973,77A,353.
[61] Schultz, J. Polym. Mater. Sci.,Prentice Hall, Englewood Cliffs:NJ,1974.
[62] Semegen, S. T. Encycolopedia of Science and Technology 1987,12, 360.
[63] Semegen, S. T. Encycolopedia of Science and Technology 1987,12, 374.
[64] Smith, G. F. Arch. Rat. Mech. Anal.1965,18, 282.
[65] Stevenson, A. J. Polym. Sci. Phys.1983,21, 553.
[66] Stevenson, A. Polymer 1986,27, 1211.
[67] Suzuki, A.; Oikawa, H.; Murakami, K. L. J. Macromol. Sci. Phys.1985,B23, 535.
[68] Toki, S.; Fujimaki, T.; Okuyama, M. Polymer 2000,41, 5423.
[69] Toki, S.; Hsiao, B.S.; Sics, I.; Ran, S.; Liu, L. Polymer 2003,44, 6003.
[70] Treloar, L.R.G. The Physics of Rubber Elasticity,3rd ed. Ox-ford:Clarendon,1975.
[71] Truesdell, C.; Toupin, R. The Classical Field Theories, Springer-Verlag,1960.
[72] Ulrich, E. Introduction to Polymer Physics, Springer-Verlag,1990.
[73] Weynant, E.; Haudin, J. M.; G’Sell, C. J. Mater. Sci.1980,15, 2677.
[74] Weynant, E.; Haudin, J. M.; G’Sell, C. J. Mater. Sci.1982,17, 1017.
[75] Wood, L. A. Rubber Chem. Technol.1966,39, 132.
[76] Yeh, G. S. Y. Rubber Chem. Technol.1977,50, 863.
CURRICULUM VITAE
PERSONAL INFORMATIONS
Name: Motasem N. H. SaidanAddresse: Heinheimerstrasse 86, D-64289 DarmstadtDate of birth: Dec 31,1974Place of birth: Sahab - JordanNationality: JordanianMarital status: Single
EDUCATION
01/2002 - 01/2005 PhD in EngineeringTechnical University of Darmstadt, Darmstadt, Germany
09/1998 - 08/2001 M.Sc in Chemical EngineeringUniversity of Jordan, Amman, Jordan
09/1993 - 06/1998 B.Sc in Chemical EngineeringUniversity of Jordan, Amman, Jordan.
0/81992 - 08/1993 High school certificate, academic branchSahab Secondary School, Sahab, Jordan
PROFESSIONAL EXPERIENCES
10/2002 - 01/2005 Research assistantGerman Polymer Institute-DKI, Darmstadt, Germany
07/2001 - 01/2002 Polymer laboratories supervising engineerAl-Balqa’a Applied University, Salt, Jordan
07/1998 - 08/2000 Design and sales engineerIrshidat Co. for water Treatment, Amman, Jordan
07/1997 - 09/1997 Training engineerPublic Power Corporation, Ptolemais, Greece.
119